#------------------------------------------------------------------------------
#$Date: 2016-03-22 21:26:17 +0200 (Tue, 22 Mar 2016) $
#$Revision: 179019 $
#$URL: svn://www.crystallography.net/cod/cif/4/12/17/4121795.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4121795
loop_
_publ_author_name
'Yang, Huayan'
'Wang, Yu'
'Yan, Juanzhu'
'Chen, Xi'
'Zhang, Xin'
'Häkkinen, Hannu'
'Zheng, Nanfeng'
_publ_section_title
;
 Structural Evolution of Atomically Precise Thiolated Bimetallic
 [Au12+nCu32(SR)30+n](4-) (n = 0, 2, 4, 6) Nanoclusters.
;
_journal_issue                   20
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              7197
_journal_page_last               7200
_journal_paper_doi               10.1021/ja501811j
_journal_volume                  136
_journal_year                    2014
_chemical_formula_moiety         'C252 H142 Au18 Cu32 F108 S36, 4(C16 H36 N)'
_chemical_formula_sum            'C332 H314 Au18 Cl7 Cu32 F108 N4 S36'
_chemical_formula_weight         13392.86
_chemical_name_systematic
;
 ? 
;
_space_group_crystal_system      monoclinic
_space_group_IT_number           13
_space_group_name_Hall           '-P 2yac'
_space_group_name_H-M_alt        'P 1 2/n 1'
_symmetry_space_group_name_Hall  '-P 2yac'
_symmetry_space_group_name_H-M   'P 1 2/n 1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_date             2014-01-09
_audit_creation_method
;
  Olex2 1.2
  (compiled Apr 23 2013 17:54:37, GUI svn.r4466)
;
_cell_angle_alpha                90.00
_cell_angle_beta                 97.456(4)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   21.8379(8)
_cell_length_b                   21.0323(11)
_cell_length_c                   43.031(2)
_cell_measurement_reflns_used    14997
_cell_measurement_temperature    100.00(10)
_cell_measurement_theta_max      65.3270
_cell_measurement_theta_min      4.1190
_cell_volume                     19597.1(16)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
;
_computing_molecular_graphics
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_publication_material
;
O. V. Dolomanov, L. J. Bourhis, R. J. Gildea, J. A. K. Howard and H. Puschmann,
OLEX2: a complete structure solution, refinement and analysis program.
J. Appl. Cryst. (2009). 42, 339-341.
;
_computing_structure_refinement
;
XH, G.M. Sheldrick, Acta Cryst.
(2008). A64, 112-122
;
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      100.00(10)
_diffrn_detector_area_resol_mean 10.3415
_diffrn_measured_fraction_theta_full 0.9428
_diffrn_measured_fraction_theta_max 0.9862
_diffrn_measurement_details
;
  1 omega -127.00  -35.00   1.0000   15.0000
omega____ theta____ kappa____ phi______ frames
    -      -40.7424 -178.0000   30.0000 92

  2 omega -117.00  -13.00   1.0000   15.0000
omega____ theta____ kappa____ phi______ frames
    -      -40.7424  -77.0000   30.0000 104

  3 omega   35.00   91.00   1.0000   25.0000
omega____ theta____ kappa____ phi______ frames
    -      108.1940  -30.0000  -60.0000 56

  4 omega   33.00  139.00   1.0000   25.0000
omega____ theta____ kappa____ phi______ frames
    -      108.1940  -77.0000 -150.0000 106

  5 omega   79.00  153.00   1.0000   25.0000
omega____ theta____ kappa____ phi______ frames
    -      108.1940   30.0000  150.0000 74

  6 omega   33.00  105.00   1.0000   25.0000
omega____ theta____ kappa____ phi______ frames
    -      108.1940 -125.0000 -150.0000 72

  7 omega   30.00   91.00   1.0000   25.0000
omega____ theta____ kappa____ phi______ frames
    -      108.1940  -30.0000    0.0000 61
;
_diffrn_measurement_device_type  'SuperNova, Dual, Cu at zero, Atlas'
_diffrn_measurement_method       'ω scans'
_diffrn_orient_matrix_UB_11      -0.0423241000
_diffrn_orient_matrix_UB_12      -0.0186252000
_diffrn_orient_matrix_UB_13      -0.0300385000
_diffrn_orient_matrix_UB_21      0.0150062000
_diffrn_orient_matrix_UB_22      -0.0706517000
_diffrn_orient_matrix_UB_23      0.0065595000
_diffrn_orient_matrix_UB_31      -0.0552807000
_diffrn_orient_matrix_UB_32      -0.0048368000
_diffrn_orient_matrix_UB_33      0.0188580000
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_type           'Cu K\a'
_diffrn_radiation_wavelength     1.5418
_diffrn_reflns_av_R_equivalents  0.0635
_diffrn_reflns_av_unetI/netI     0.0763
_diffrn_reflns_limit_h_max       17
_diffrn_reflns_limit_h_min       -24
_diffrn_reflns_limit_k_max       23
_diffrn_reflns_limit_k_min       -23
_diffrn_reflns_limit_l_max       48
_diffrn_reflns_limit_l_min       -46
_diffrn_reflns_number            54998
_diffrn_reflns_theta_full        61.17
_diffrn_reflns_theta_max         61.17
_diffrn_reflns_theta_min         3.43
_diffrn_source                   'SuperNova (Cu) X-ray Source'
_exptl_absorpt_coefficient_mu    17.211
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.19506
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.36.28 (release 01-02-2013 CrysAlis171 .NET)
(compiled Feb  1 2013,16:14:44)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.270
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       plane
_exptl_crystal_F_000             12702
_exptl_crystal_size_max          0.1
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.03
_platon_squeeze_details
;
SQUEEZE removed 8 disordered dichloromethane molecules per formula unit.
;
_refine_diff_density_max         5.866
_refine_diff_density_min         -5.272
_refine_diff_density_rms         0.320
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.071
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     1971
_refine_ls_number_reflns         29916
_refine_ls_number_restraints     392
_refine_ls_restrained_S_all      1.267
_refine_ls_R_factor_all          0.1109
_refine_ls_R_factor_gt           0.0889
_refine_ls_shift/su_max          0.002
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.1421P)²+307.0838P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.2447
_refine_ls_wR_factor_ref         0.2637
_reflns_number_gt                21313
_reflns_number_total             29916
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja501811j_si_005.cif
_cod_data_source_block           Au12Cu32@Au6
_cod_depositor_comments
'Adding full bibliography for 4121793--4121797.cif.'
_cod_original_cell_volume        19596.9(16)
_cod_database_code               4121795
#BEGIN Tags that were not found in dictionaries:
_reflns_odcompleteness_completeness 94.28
_reflns_odcompleteness_iscentric 1
_reflns_odcompleteness_theta     66.97
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups, All C(H,H) groups
 At 1.5 times of:
  All C(H,H,H) groups
2. Restrained distances
 F44-C105 = F43-C105 = F45-C105
 1.3 with sigma of 0.02
 F43-F45
 2.4 with sigma of 0.02
 F45-F44
 2.4 with sigma of 0.02
 F44-F43
 2.4 with sigma of 0.02
 C135-C131
 2.5 with sigma of 0.02
 C135-C139
 1.5 with sigma of 0.02
 C139-C135
 2.5 with sigma of 0.02
 C139-C127
 2.5 with sigma of 0.02
 C127-C131
 2.5 with sigma of 0.02
 N1-C136
 2.5 with sigma of 0.02
 C135-C137
 2.5 with sigma of 0.02
 C136-C138
 2.5 with sigma of 0.02
 N1-C132
 2.5 with sigma of 0.02
 C131-C133
 2.5 with sigma of 0.02
 C132-C134
 2.5 with sigma of 0.02
 N1-C128
 2.5 with sigma of 0.02
 C127-C129
 2.5 with sigma of 0.02
 C128-C130
 2.5 with sigma of 0.02
 C139-C141
 2.5 with sigma of 0.02
 C155-C157 = N2-C155 = C158-C157 = C159-C158 = N2-C147 = C148-C147 = C149-C148
 = C149-C150 = N2-C143 = C144-C143 = C145-C144 = C146-C145 = N2-C151 = C151-
 C152 = C153-C152 = C153-C154
 1.5 with sigma of 0.02
 C155-C147
 2.5 with sigma of 0.02
 C147-C143
 2.5 with sigma of 0.02
 C143-C151
 2.5 with sigma of 0.02
 C151-C155
 2.5 with sigma of 0.02
 C148-N2
 2.5 with sigma of 0.02
 C147-C149
 2.5 with sigma of 0.02
 C148-C150
 2.5 with sigma of 0.02
 N2-C144
 2.5 with sigma of 0.02
 C143-C145
 2.5 with sigma of 0.02
 C144-C146
 2.5 with sigma of 0.02
 N2-C152
 2.5 with sigma of 0.02
 C151-C153
 2.5 with sigma of 0.02
 C152-C154
 2.5 with sigma of 0.02
 N2-C157
 2.5 with sigma of 0.02
 C155-C158
 2.5 with sigma of 0.02
 C157-C159
 2.5 with sigma of 0.02
 F39-C91
 1.3 with sigma of 0.02
 F41-C98 = F42-C98 = F40-C98
 1.3 with sigma of 0.02
 F42-F41
 2.4 with sigma of 0.02
 F42-F40
 2.4 with sigma of 0.02
 F40-F41
 2.4 with sigma of 0.02
 F39-C91 = F38-C91 = F37-C91
 1.3 with sigma of 0.02
 F38-F37
 2.4 with sigma of 0.02
 F39-F37
 2.4 with sigma of 0.02
 F39-F38
 2.4 with sigma of 0.02
 N1-C135 = N1-C139 = N1-C131 = N1-C127
 1.5 with sigma of 0.02
 C127-C135
 2.45 with sigma of 0.02
 C135-C131
 2.45 with sigma of 0.02
 C131-C139
 2.45 with sigma of 0.02
 C139-C127
 2.45 with sigma of 0.02
 N1-C131 = N1-C139 = N1-C127 = N1-C135 = C131-C132 = C133-C132 = C134-C133 =
 C136-C135 = C136-C137 = C138-C137 = C140-C139 = C140-C141 = C142-C141 = C127-
 C128 = C129-C128 = C129-C130
 1.5 with sigma of 0.02
 N1-C140
 2.5 with sigma of 0.02
 C140-C142
 2.5 with sigma of 0.02
 C140-C139 = C140-C141 = N1-C131 = N1-C139 = N1-C127 = N1-C135 = C136-C135
 1.5 with sigma of 0.02
 N1-C135 = N1-C127 = N1-C139 = N1-C131
 2.45 with sigma of 0.02
 N1-C131 = N1-C135 = N1-C127 = N1-C139
 1.45 with sigma of 0.02
 C127-C135
 2.45 with sigma of 0.02
 C127-C139
 2.45 with sigma of 0.02
 C131-C135
 2.45 with sigma of 0.02
 C84-C81
 1.5 with sigma of 0.02
3. Rigid bond restraints
 S3, C68
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 S15, C99
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 S12, C78
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C64, C65
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C8, C13
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C27, C26
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C85, C86
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C100, C99
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C97, C92
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 N2, C155
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 N2, C143
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 N2, C151
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 S3, C15
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 S15, C99
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 S12, C78
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C64, C65
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C8, C13
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C27, C26
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C85, C86
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C85, C86
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C85, C90
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C100, C99
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C97, C92
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 N2, C155
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.01
 C157, C155
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 S12, C99
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 S13, C85
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 S12, C78
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C100, C99
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
 C157, C158
 with sigma for 1-2 distances of 0.02 and sigma for 1-3 distances of 0.02
4. Uiso/Uaniso restraints and constraints
C85 \\sim C86 \\sim S13: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C99 \\sim C104 \\sim C100 \\sim S15: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
N2 \\sim C143 \\sim C151 \\sim C147 \\sim C155: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C85 \\sim C86 \\sim C90: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C99 \\sim C104 \\sim C100 \\sim S15: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
N2 \\sim C143 \\sim C151 \\sim C147 \\sim C155: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C136 \\sim C135 \\sim C137: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C99 \\sim C100 \\sim C104: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C103 \\sim C104 \\sim C102: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C157 \\sim C155 \\sim C158: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C140 \\sim C141: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C104 \\sim C103 \\sim C99: within 1.7A with sigma of 0.01 and sigma for terminal atoms of 0.02
C155 \\sim C157 \\sim N2: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C139 \\sim C140 \\sim N1: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C141 \\sim C142 \\sim C140: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
C137 \\sim C138 \\sim C136: within 3.8A with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(F5) \\sim Ueq: with sigma of 0.1 and sigma for terminal atoms of 0.2
Uanis(C1) \\sim Ueq: with sigma of 0.1 and sigma for terminal atoms of 0.2
: with sigma of 0.1 and sigma for terminal atoms of 0.2
Uanis(C1) \\sim Ueq: with sigma of 0.1 and sigma for terminal atoms of 0.2
: with sigma of 0.1 and sigma for terminal atoms of 0.2
Uanis(F36) \\sim Ueq, Uanis(F35) \\sim Ueq, Uanis(F34) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(F38) = Uanis(C85)
Uanis(F22) = Uanis(F22A) = Uanis(F24) = Uanis(F24A) = Uanis(F23) = Uanis(F23A)
Uanis(F33A) = Uanis(F33) = Uanis(F32A) = Uanis(F32) = Uanis(F31A) = Uanis(F31)
Uanis(C86) = Uanis(C87) = Uanis(C88) = Uanis(C89) = Uanis(F37) = Uanis(C91) = Uanis(F39) = Uanis(C79) = Uanis(C82) = Uanis(C81) = Uanis(C80) = Uanis(C84) = Uanis(C83) = Uanis(C90) = Uanis(C78) = Uanis(C144) = Uanis(C145) = Uanis(C146) = Uanis(C143) = Uanis(C154) = Uanis(C153) = Uanis(C152) = Uanis(C151) = Uanis(C155) = Uanis(C159) = Uanis(C134) = Uanis(C133) = Uanis(C132) = Uanis(C131) = Uanis(C142) = Uanis(C141) = Uanis(C139) = Uanis(N1) = Uanis(C127) = Uanis(C128) = Uanis(C129) = Uanis(C130) = Uanis(C137) = Uanis(C138) = Uanis(F41) = Uanis(C98) = Uanis(F42) = Uanis(F40) = Uanis(C99)
5. Others
 Sof(F23A)=Sof(F22A)=Sof(F24A)=1-FVAR(1)
 Sof(F24)=Sof(F23)=Sof(F22)=FVAR(1)
 Sof(F33A)=Sof(F32A)=Sof(F31A)=1-FVAR(2)
 Sof(F33)=Sof(F31)=Sof(F32)=FVAR(2)
6.a Free rotating group:
 F44(F43,F45), F36(F34,F35)
6.b Secondary CH2 refined with riding coordinates:
 C147(H14A,H14B), C148(H14C,H14D), C141(H14P,H14Q), C157(H15D,H15E), C158(H15F,
 H15G), C140(H14R,H14S), C132(H13A,H13B), C152(H15H,H15I), C155(H15J,H15K),
 C149(H14E,H14F), C143(H14G,H14H), C128(H12A,H12B), C137(H13C,H13D), C135(H13E,
 H13F), C133(H13G,H13H), C136(H13L,H13M), C153(H15L,H15M), C151(H15Q,H15R),
 C131(H13T,H13U), C127(H12C,H12D), C144(H14I,H14J), C145(H14K,H14L), C129(H12E,
 H12F), C139(H13V,H13W)
6.c Aromatic/amide H refined with riding coordinates:
 C6(H6), C44(H44), C9(H9), C111(H111), C23(H23), C3(H3), C45(H45), C5(H5),
 C20(H20), C76(H76), C101(H101), C100(H100), C104(H104), C103(H103), C114(H114),
  C121(H121), C47(H47), C10(H10), C27(H27), C110(H110), C16(H16), C58(H58),
 C48(H48), C107(H107), C117(H117), C65(H65), C68(H68), C59(H59), C26(H26),
 C125(H125), C69(H69), C24(H24), C122(H122), C66(H66), C115(H115), C86(H86),
 C87(H87), C89(H89), C90(H90), C124(H124), C2(H2), C17(H17), C118(H118),
 C108(H108), C62(H62), C12(H12), C51(H51), C72(H72), C13(H13), C34(H34),
 C75(H75), C19(H19), C41(H41), C55(H55), C61(H61), C52(H52), C73(H73), C54(H54),
  C40(H40), C30(H30), C33(H33), C31(H31), C37(H37), C38(H38), C93(H93),
 C97(H97), C96(H96), C94(H94), C82(H82), C80(H80), C79(H79)
6.d Fitted hexagon refined as free rotating group:
 C102(C101,C100,C99,C104,C103), C85(C86,C87,C88,C89,C90), C93(C92,C97,C96,C95,
 C94), C83(C82,C81,C80,C79,C78)
6.e Idealised Me refined as rotating group:
 C150(H15A,H15B,H15C), C130(H13I,H13J,H13K), C142(H14T,H14U,H14V), C138(H13N,
 H13O,H13P), C159(H15N,H15O,H15P), C134(H13Q,H13R,H13S), C146(H14M,H14N,H14O),
 C154(H15S,H15T,H15U)
;
#END Tags that were not found in dictionaries
loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 'x, y, z'
2 '-x+1/2, y, -z+1/2'
3 '-x, -y, -z'
4 'x-1/2, -y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Au1 Au 0.83478(3) 0.77083(4) 0.711393(19) 0.0311(2) Uani 1 1 d . . .
Au2 Au 0.81335(3) 0.87687(4) 0.746248(18) 0.0306(2) Uani 1 1 d . . .
Au3 Au 0.72327(3) 0.83643(4) 0.697947(19) 0.0313(2) Uani 1 1 d . . .
Au4 Au 0.81335(4) 0.66226(4) 0.745923(19) 0.0321(2) Uani 1 1 d . . .
Au5 Au 0.72581(3) 0.70299(4) 0.697933(19) 0.0323(2) Uani 1 1 d . . .
Au6 Au 0.63316(3) 0.76830(4) 0.723608(19) 0.0316(2) Uani 1 1 d . . .
Au7 Au 0.7500 1.15264(7) 0.7500 0.0467(3) Uani 1 2 d S . .
Au8 Au 0.7500 0.38712(7) 0.7500 0.0511(4) Uani 1 2 d S . .
Au9 Au 1.11488(4) 0.76677(6) 0.73564(3) 0.0559(3) Uani 1 1 d . . .
Au10 Au 0.65352(6) 0.76138(8) 0.56359(3) 0.0774(4) Uani 1 1 d . . .
Cu1 Cu 0.84287(14) 1.04475(15) 0.74936(7) 0.0404(7) Uani 1 1 d . . .
Cu2 Cu 0.83663(14) 0.49362(16) 0.73835(8) 0.0435(7) Uani 1 1 d . . .
Cu3 Cu 1.03479(14) 0.76715(15) 0.78364(8) 0.0423(7) Uani 1 1 d . . .
Cu4 Cu 0.99075(14) 0.77024(16) 0.68917(8) 0.0445(7) Uani 1 1 d . . .
Cu5 Cu 0.83474(13) 0.65597(14) 0.68488(7) 0.0372(7) Uani 1 1 d . . .
Cu6 Cu 0.60797(13) 0.88408(14) 0.69953(7) 0.0348(6) Uani 1 1 d . . .
Cu7 Cu 0.73633(13) 0.95973(14) 0.71527(7) 0.0339(6) Uani 1 1 d . . .
Cu8 Cu 0.73023(13) 0.57926(15) 0.71612(7) 0.0377(7) Uani 1 1 d . . .
Cu9 Cu 0.82999(13) 0.88966(13) 0.68514(7) 0.0343(6) Uani 1 1 d . . .
Cu10 Cu 0.61451(13) 0.64767(14) 0.69862(7) 0.0365(7) Uani 1 1 d . . .
Cu11 Cu 0.92922(13) 0.84002(14) 0.73885(7) 0.0384(7) Uani 1 1 d . . .
Cu12 Cu 0.92999(13) 0.69792(14) 0.73862(7) 0.0370(7) Uani 1 1 d . . .
Cu13 Cu 0.67662(18) 0.8579(2) 0.61472(8) 0.0614(10) Uani 1 1 d . . .
Cu14 Cu 0.69043(18) 0.6714(2) 0.61214(9) 0.0646(10) Uani 1 1 d . . .
Cu15 Cu 0.77193(14) 0.77717(15) 0.65316(7) 0.0392(7) Uani 1 1 d . . .
Cu16 Cu 0.63727(14) 0.76110(16) 0.66101(7) 0.0412(7) Uani 1 1 d . . .
S4 S 0.9895(2) 0.8627(3) 0.78439(14) 0.0416(12) Uani 1 1 d . . .
S9 S 0.9836(2) 0.6740(3) 0.78613(13) 0.0406(12) Uani 1 1 d . . .
S10 S 0.9419(2) 0.6778(2) 0.68815(13) 0.0391(11) Uani 1 1 d . . .
S7 S 0.9365(2) 0.8624(3) 0.68757(14) 0.0444(13) Uani 1 1 d . . .
S2 S 0.8634(2) 0.9906(3) 0.79447(12) 0.0389(11) Uani 1 1 d . . .
S18 S 0.8149(2) 0.5495(2) 0.69392(13) 0.0393(11) Uani 1 1 d . . .
S3 S 0.8263(2) 1.0008(3) 0.70213(12) 0.0379(11) Uani 1 1 d U . .
S16 S 0.6341(2) 0.5362(3) 0.71446(13) 0.0406(12) Uani 1 1 d . . .
S11 S 0.7884(2) 0.6795(3) 0.63345(13) 0.0410(12) Uani 1 1 d . . .
S15 S 0.6165(3) 0.6602(3) 0.64382(15) 0.0577(15) Uani 1 1 d U . .
S8 S 0.7758(3) 0.8781(3) 0.63299(13) 0.0481(13) Uani 1 1 d . . .
S13 S 0.6010(3) 0.8578(4) 0.64607(15) 0.0582(15) Uani 1 1 d U . .
S17 S 0.8387(3) 0.3887(3) 0.72652(15) 0.0517(14) Uani 1 1 d . . .
S1 S 0.8555(3) 1.1503(3) 0.75863(14) 0.0503(14) Uani 1 1 d . . .
S5 S 1.1393(3) 0.7520(3) 0.78876(17) 0.0576(16) Uani 1 1 d . . .
S6 S 1.0909(3) 0.7862(3) 0.68311(17) 0.0589(16) Uani 1 1 d . . .
S14 S 0.6500(5) 0.6540(5) 0.5612(2) 0.097(3) Uani 1 1 d . . .
S12 S 0.6502(5) 0.8690(6) 0.56207(18) 0.098(3) Uani 1 1 d U . .
F50 F 1.1003(6) 0.2625(8) 0.8003(4) 0.070(4) Uani 1 1 d . . .
F49 F 1.0499(9) 0.2738(10) 0.8391(4) 0.087(6) Uani 1 1 d . . .
F1 F 1.0305(7) 1.2810(7) 0.6593(4) 0.068(4) Uani 1 1 d . . .
F19 F 1.1066(8) 1.0898(9) 0.6296(5) 0.090(6) Uani 1 1 d . . .
F10 F 1.1606(8) 1.1283(8) 0.7925(5) 0.091(6) Uani 1 1 d . . .
F20 F 1.1002(8) 1.1309(8) 0.6743(5) 0.083(5) Uani 1 1 d . . .
F21 F 1.0246(9) 1.1390(8) 0.6387(5) 0.091(6) Uani 1 1 d . . .
F51 F 1.0341(7) 0.1922(8) 0.8091(5) 0.082(5) Uani 1 1 d . . .
F3 F 0.9486(9) 1.2660(11) 0.6271(4) 0.095(6) Uani 1 1 d . . .
C43 C 0.9815(9) 0.9294(12) 0.6800(6) 0.049(6) Uani 1 1 d . . .
F12 F 1.1033(8) 1.1411(8) 0.7505(5) 0.087(6) Uani 1 1 d . . .
F7 F 0.8268(10) 1.2341(11) 0.5959(6) 0.114(8) Uani 1 1 d . . .
F30 F 1.0844(9) 0.4159(10) 0.6443(6) 0.107(7) Uani 1 1 d . . .
C6 C 0.8498(11) 1.2258(10) 0.7052(6) 0.045(5) Uani 1 1 d . . .
H6 H 0.8066 1.2296 0.7056 0.054 Uiso 1 1 calc R . .
F52 F 0.7851(11) 0.4408(10) 0.5484(4) 0.101(7) Uani 1 1 d . . .
C22 C 1.0364(10) 0.9287(13) 0.7797(7) 0.055(7) Uani 1 1 d . . .
F11 F 1.1867(8) 1.0901(10) 0.7498(6) 0.107(7) Uani 1 1 d . . .
C64 C 0.9911(11) 0.6087(10) 0.6834(7) 0.052(6) Uani 1 1 d U . .
F53 F 0.6929(11) 0.4216(12) 0.5565(5) 0.109(7) Uani 1 1 d . . .
F29 F 1.0888(11) 0.4014(10) 0.6944(7) 0.117(8) Uani 1 1 d . . .
C57 C 1.0333(10) 0.6069(10) 0.7883(6) 0.046(5) Uani 1 1 d . . .
F46 F 0.6078(13) 0.2660(10) 0.6325(5) 0.110(7) Uani 1 1 d . . .
C106 C 0.6207(9) 0.4717(10) 0.6864(5) 0.038(5) Uani 1 1 d . . .
F47 F 0.6190(11) 0.3307(10) 0.5961(5) 0.109(8) Uani 1 1 d . . .
C44 C 0.9840(9) 0.9841(10) 0.6970(5) 0.038(5) Uani 1 1 d . . .
H44 H 0.9637 0.9846 0.7152 0.046 Uiso 1 1 calc R . .
F2 F 0.9567(9) 1.3489(8) 0.6561(5) 0.097(7) Uani 1 1 d . . .
C116 C 0.9929(11) 0.2885(9) 0.7889(6) 0.043(5) Uani 1 1 d . . .
C71 C 0.8446(11) 0.6710(12) 0.6063(5) 0.047(6) Uani 1 1 d . . .
C9 C 0.9247(11) 1.0872(10) 0.8308(6) 0.049(6) Uani 1 1 d . . .
H9 H 0.9415 1.1002 0.8125 0.059 Uiso 1 1 calc R . .
F48 F 0.5301(10) 0.3137(12) 0.6095(5) 0.112(8) Uani 1 1 d . . .
C119 C 1.0442(12) 0.2541(14) 0.8082(7) 0.058(7) Uani 1 1 d . . .
C111 C 0.6689(10) 0.4368(12) 0.6789(6) 0.048(6) Uani 1 1 d . . .
H111 H 0.7095 0.4462 0.6885 0.058 Uiso 1 1 calc R . .
C8 C 0.8825(12) 1.0358(12) 0.8288(5) 0.051(6) Uani 1 1 d U . .
F8 F 0.7567(15) 1.2686(12) 0.6207(6) 0.139(11) Uani 1 1 d . . .
C23 C 1.0304(10) 0.9819(14) 0.7969(7) 0.059(7) Uani 1 1 d . . .
H23 H 1.0026 0.9822 0.8121 0.071 Uiso 1 1 calc R . .
C3 C 0.9736(14) 1.2120(11) 0.7023(7) 0.061(7) Uani 1 1 d . . .
H3 H 1.0164 1.2058 0.7013 0.073 Uiso 1 1 calc R . .
C45 C 1.0140(11) 1.0390(11) 0.6897(6) 0.050(6) Uani 1 1 d . . .
H45 H 1.0165 1.0751 0.7031 0.060 Uiso 1 1 calc R . .
C5 C 0.8804(13) 1.2590(12) 0.6828(5) 0.054(6) Uani 1 1 d . . .
H5 H 0.8569 1.2872 0.6687 0.064 Uiso 1 1 calc R . .
C20 C 0.8543(13) 1.0769(13) 0.6538(6) 0.060(7) Uani 1 1 d . . .
H20 H 0.8903 1.0514 0.6541 0.071 Uiso 1 1 calc R . .
C36 C 1.1199(11) 0.7177(13) 0.6633(6) 0.051(6) Uani 1 1 d . . .
C76 C 0.8925(12) 0.7142(14) 0.6063(7) 0.059(7) Uani 1 1 d . . .
H76 H 0.8959 0.7492 0.6203 0.071 Uiso 1 1 calc R . .
C102 C 0.4291(9) 0.6199(13) 0.5882(6) 0.116(6) Uani 1 1 d GU . .
C101 C 0.4640(11) 0.6704(12) 0.5793(6) 0.113(15) Uani 1 1 d G . .
H101 H 0.4488 0.6957 0.5616 0.136 Uiso 1 1 calc R . .
C100 C 0.5212(11) 0.6838(12) 0.5961(7) 0.108(4) Uani 1 1 d GU . .
H100 H 0.5451 0.7184 0.5900 0.129 Uiso 1 1 calc R . .
C99 C 0.5435(11) 0.6468(16) 0.6219(7) 0.1504(17) Uani 1 1 d GU . .
C104 C 0.5085(14) 0.5963(14) 0.6308(5) 0.111(4) Uiso 1 1 d GU . .
H104 H 0.5238 0.5710 0.6484 0.133 Uiso 1 1 calc R . .
C103 C 0.4513(13) 0.5829(11) 0.6139(6) 0.119(6) Uani 1 1 d GU . .
H103 H 0.4275 0.5484 0.6200 0.143 Uiso 1 1 calc R . .
C113 C 0.8969(12) 0.3508(13) 0.7530(7) 0.060(7) Uani 1 1 d . . .
C114 C 0.8851(11) 0.3108(11) 0.7779(6) 0.049(6) Uani 1 1 d . . .
H114 H 0.8441 0.3032 0.7822 0.058 Uiso 1 1 calc R . .
C121 C 0.8343(12) 0.4582(13) 0.6500(5) 0.057(7) Uani 1 1 d . . .
H121 H 0.8704 0.4465 0.6635 0.068 Uiso 1 1 calc R . .
C50 C 0.8250(14) 0.8771(13) 0.6026(5) 0.058(7) Uani 1 1 d . . .
C47 C 1.0408(11) 0.9840(12) 0.6430(6) 0.053(6) Uani 1 1 d . . .
H47 H 1.0600 0.9837 0.6244 0.063 Uiso 1 1 calc R . .
C4 C 0.9405(11) 1.2524(10) 0.6806(6) 0.045(5) Uani 1 1 d . . .
C10 C 0.9417(13) 1.1184(13) 0.8582(7) 0.064(7) Uani 1 1 d . . .
H10 H 0.9701 1.1527 0.8591 0.077 Uiso 1 1 calc R . .
C27 C 1.0800(11) 0.9309(13) 0.7578(6) 0.054(6) Uani 1 1 d U . .
H27 H 1.0851 0.8942 0.7455 0.065 Uiso 1 1 calc R . .
C110 C 0.6594(12) 0.3875(12) 0.6573(6) 0.054(6) Uani 1 1 d . . .
H110 H 0.6931 0.3629 0.6521 0.064 Uiso 1 1 calc R . .
C16 C 0.7580(10) 1.1015(11) 0.6723(5) 0.042(5) Uani 1 1 d . . .
H16 H 0.7288 1.0926 0.6863 0.051 Uiso 1 1 calc R . .
C1 C 0.8862(11) 1.1878(9) 0.7265(6) 0.045(5) Uani 1 1 d U . .
C58 C 1.0230(11) 0.5563(11) 0.7685(5) 0.048(6) Uani 1 1 d . . .
H58 H 0.9891 0.5578 0.7523 0.057 Uiso 1 1 calc R . .
C123 C 0.7671(11) 0.4460(13) 0.6007(6) 0.052(6) Uani 1 1 d . . .
C48 C 1.0112(11) 0.9286(13) 0.6527(5) 0.052(6) Uani 1 1 d . . .
H48 H 1.0115 0.8906 0.6407 0.062 Uiso 1 1 calc R . .
C107 C 0.5606(12) 0.4597(14) 0.6731(7) 0.067(8) Uani 1 1 d . . .
H107 H 0.5276 0.4859 0.6778 0.081 Uiso 1 1 calc R . .
C120 C 0.7963(10) 0.5061(10) 0.6588(5) 0.043(5) Uani 1 1 d . . .
N2 N 0.7535(11) 0.7390(14) 0.3727(6) 0.147(4) Uani 1 1 d DU . .
C117 C 1.0077(11) 0.3286(13) 0.7651(7) 0.061(7) Uani 1 1 d . . .
H117 H 1.0492 0.3343 0.7612 0.074 Uiso 1 1 calc R . .
F54 F 0.7672(16) 0.3557(11) 0.5694(4) 0.150(13) Uani 1 1 d . . .
C65 C 0.9679(12) 0.5654(12) 0.6623(7) 0.059(6) Uani 1 1 d U . .
H65 H 0.9289 0.5712 0.6501 0.071 Uiso 1 1 calc R . .
C15 C 0.8120(10) 1.0645(9) 0.6739(5) 0.038(5) Uani 1 1 d U . .
C68 C 1.0838(11) 0.5529(12) 0.6959(6) 0.055(6) Uani 1 1 d . . .
H68 H 1.1231 0.5482 0.7080 0.066 Uiso 1 1 calc R . .
C59 C 1.0593(11) 0.5041(12) 0.7713(7) 0.055(6) Uani 1 1 d . . .
H59 H 1.0503 0.4699 0.7570 0.067 Uiso 1 1 calc R . .
C26 C 1.1147(10) 0.9831(13) 0.7539(7) 0.059(7) Uani 1 1 d U . .
H26 H 1.1437 0.9821 0.7393 0.070 Uiso 1 1 calc R . .
F6 F 0.9829(16) 1.1782(12) 0.9129(5) 0.149(12) Uani 1 1 d . . .
C125 C 0.7412(11) 0.5238(11) 0.6384(6) 0.050(6) Uani 1 1 d . . .
H125 H 0.7158 0.5569 0.6446 0.060 Uiso 1 1 calc R . .
C25 C 1.1078(10) 1.0389(13) 0.7713(7) 0.056(6) Uani 1 1 d . . .
F28 F 1.1593(8) 0.4585(10) 0.6753(7) 0.129(10) Uani 1 1 d . . .
C67 C 1.0612(12) 0.5062(12) 0.6738(8) 0.070(9) Uani 1 1 d . . .
C46 C 1.0411(10) 1.0391(12) 0.6612(7) 0.054(6) Uani 1 1 d . . .
C69 C 1.0491(10) 0.6036(12) 0.6996(6) 0.048(6) Uani 1 1 d . . .
H69 H 1.0647 0.6366 0.7135 0.058 Uiso 1 1 calc R . .
C24 C 1.0657(12) 1.0372(14) 0.7924(7) 0.063(7) Uani 1 1 d . . .
H24 H 1.0599 1.0742 0.8043 0.076 Uiso 1 1 calc R . .
C122 C 0.8196(13) 0.4276(13) 0.6217(7) 0.065(8) Uani 1 1 d . . .
H122 H 0.8449 0.3937 0.6161 0.078 Uiso 1 1 calc R . .
C66 C 1.0046(12) 0.5102(14) 0.6589(7) 0.066(8) Uani 1 1 d . . .
H66 H 0.9881 0.4763 0.6459 0.079 Uiso 1 1 calc R . .
C115 C 0.9345(10) 0.2834(10) 0.7956(6) 0.045(5) Uani 1 1 d . . .
H115 H 0.9273 0.2596 0.8135 0.054 Uiso 1 1 calc R . .
C85 C 0.5223(12) 0.855(2) 0.6283(8) 0.133(4) Uani 1 1 d GU . .
C86 C 0.4906(17) 0.8005(17) 0.6350(8) 0.1504(17) Uani 1 1 d GU . .
H86 H 0.5116 0.7674 0.6471 0.180 Uiso 1 1 calc R . .
C87 C 0.4283(17) 0.7942(16) 0.6239(9) 0.1504(17) Uani 1 1 d G . .
H87 H 0.4066 0.7568 0.6284 0.180 Uiso 1 1 calc R . .
C88 C 0.3976(12) 0.843(2) 0.6062(9) 0.1504(17) Uani 1 1 d G . .
C89 C 0.4292(17) 0.8972(17) 0.5995(8) 0.1504(17) Uani 1 1 d G . .
H89 H 0.4082 0.9302 0.5874 0.180 Uiso 1 1 calc R . .
C90 C 0.4916(17) 0.9035(16) 0.6106(9) 0.1504(17) Uani 1 1 d GU . .
H90 H 0.5133 0.9408 0.6061 0.180 Uiso 1 1 calc R . .
C124 C 0.7244(14) 0.4926(13) 0.6094(6) 0.060(7) Uani 1 1 d . . .
H124 H 0.6870 0.5019 0.5964 0.072 Uiso 1 1 calc R . .
C2 C 0.9475(11) 1.1818(10) 0.7245(6) 0.046(5) Uani 1 1 d . . .
H2 H 0.9722 1.1557 0.7391 0.055 Uiso 1 1 calc R . .
C17 C 0.7469(13) 1.1484(13) 0.6518(6) 0.057(6) Uani 1 1 d . . .
H17 H 0.7102 1.1728 0.6514 0.068 Uiso 1 1 calc R . .
F16 F 1.2385(14) 0.5423(14) 0.6234(7) 0.148(11) Uani 1 1 d . . .
C118 C 0.9574(12) 0.3608(15) 0.7466(7) 0.067(8) Uani 1 1 d . . .
H118 H 0.9653 0.3888 0.7302 0.080 Uiso 1 1 calc R . .
C29 C 1.1781(10) 0.8233(13) 0.8028(6) 0.055(6) Uani 1 1 d . . .
C108 C 0.5497(14) 0.4091(17) 0.6529(7) 0.075(9) Uani 1 1 d . . .
H108 H 0.5086 0.3971 0.6452 0.089 Uiso 1 1 calc R . .
F17 F 1.1958(12) 0.5881(16) 0.5829(6) 0.140(11) Uani 1 1 d . . .
F14 F 1.3117(12) 1.0140(15) 0.8171(7) 0.146(11) Uani 1 1 d . . .
C62 C 1.0832(13) 0.6059(12) 0.8107(7) 0.066(8) Uani 1 1 d . . .
H62 H 1.0917 0.6409 0.8246 0.079 Uiso 1 1 calc R . .
C12 C 0.8771(16) 1.0509(15) 0.8840(6) 0.075(9) Uani 1 1 d . . .
H12 H 0.8622 1.0379 0.9028 0.090 Uiso 1 1 calc R . .
C51 C 0.8131(14) 0.8379(15) 0.5768(7) 0.069(8) Uani 1 1 d . . .
H51 H 0.7776 0.8112 0.5750 0.083 Uiso 1 1 calc R . .
F9 F 0.7410(16) 1.1977(18) 0.5833(8) 0.23(2) Uani 1 1 d . . .
C72 C 0.8415(15) 0.6213(18) 0.5875(6) 0.081(10) Uani 1 1 d . . .
H72 H 0.8078 0.5926 0.5869 0.098 Uiso 1 1 calc R . .
C32 C 1.2382(11) 0.9346(18) 0.8230(9) 0.083(10) Uani 1 1 d . . .
C13 C 0.8580(12) 1.0207(12) 0.8576(5) 0.053(6) Uani 1 1 d U . .
H13 H 0.8275 0.9885 0.8575 0.064 Uiso 1 1 calc R . .
F18 F 1.1440(14) 0.5181(14) 0.6053(8) 0.161(13) Uani 1 1 d . . .
C11 C 0.9173(15) 1.0998(15) 0.8848(7) 0.073(8) Uani 1 1 d . . .
F15 F 1.2382(11) 1.0391(13) 0.8417(9) 0.171(15) Uani 1 1 d . . .
C49 C 1.0687(14) 1.1001(17) 0.6504(9) 0.077(9) Uani 1 1 d . . .
C60 C 1.1121(11) 0.4995(15) 0.7958(8) 0.072(9) Uani 1 1 d . . .
C34 C 1.2323(12) 0.8398(14) 0.7921(8) 0.070(8) Uani 1 1 d . . .
H34 H 1.2474 0.8141 0.7766 0.084 Uiso 1 1 calc R . .
C75 C 0.9351(14) 0.7061(19) 0.5858(7) 0.077(9) Uani 1 1 d . . .
H75 H 0.9670 0.7367 0.5852 0.092 Uiso 1 1 calc R . .
C18 C 0.7884(14) 1.1620(13) 0.6309(6) 0.067(8) Uani 1 1 d . . .
C19 C 0.8435(13) 1.1277(15) 0.6329(6) 0.062(7) Uani 1 1 d . . .
H19 H 0.8738 1.1390 0.6199 0.075 Uiso 1 1 calc R . .
C41 C 1.0785(13) 0.6870(14) 0.6406(6) 0.062(7) Uani 1 1 d . . .
H41 H 1.0364 0.6996 0.6368 0.074 Uiso 1 1 calc R . .
C109 C 0.5996(15) 0.3752(17) 0.6437(7) 0.077(9) Uani 1 1 d . . .
C55 C 0.8736(14) 0.9185(17) 0.6043(7) 0.074(8) Uani 1 1 d . . .
H55 H 0.8803 0.9480 0.6212 0.089 Uiso 1 1 calc R . .
C61 C 1.1208(14) 0.5540(14) 0.8130(9) 0.082(10) Uani 1 1 d . . .
H61 H 1.1566 0.5559 0.8281 0.099 Uiso 1 1 calc R . .
F13 F 1.3067(15) 0.9850(16) 0.8626(8) 0.163(12) Uani 1 1 d . . .
C52 C 0.8507(13) 0.8362(17) 0.5538(7) 0.073(8) Uani 1 1 d . . .
H52 H 0.8430 0.8073 0.5367 0.088 Uiso 1 1 calc R . .
C126 C 0.752(2) 0.4127(19) 0.5693(8) 0.094(12) Uani 1 1 d . . .
C53 C 0.9019(15) 0.8791(19) 0.5560(7) 0.082(10) Uani 1 1 d . B .
C73 C 0.8876(19) 0.611(2) 0.5687(8) 0.102(13) Uani 1 1 d . . .
H73 H 0.8881 0.5725 0.5572 0.123 Uiso 1 1 calc R . .
C112 C 0.5856(17) 0.3217(18) 0.6194(8) 0.081(9) Uani 1 1 d . . .
C54 C 0.9138(16) 0.9175(19) 0.5813(9) 0.093(11) Uani 1 1 d . . .
H54 H 0.9494 0.9439 0.5835 0.111 Uiso 1 1 calc R . .
C40 C 1.1008(14) 0.6379(15) 0.6241(8) 0.074(8) Uani 1 1 d . . .
H40 H 1.0740 0.6156 0.6087 0.089 Uiso 1 1 calc R . .
C74 C 0.9324(17) 0.656(3) 0.5667(8) 0.112(17) Uani 1 1 d . A .
F33 F 0.953(2) 0.654(4) 0.5162(15) 0.151(16) Uani 0.60(4) 1 d P A 1
C30 C 1.1539(12) 0.8647(16) 0.8220(7) 0.070(8) Uani 1 1 d . . .
H30 H 1.1149 0.8549 0.8284 0.084 Uiso 1 1 calc R . .
C33 C 1.2667(12) 0.8944(13) 0.8035(9) 0.081(11) Uani 1 1 d . . .
H33 H 1.3067 0.9030 0.7981 0.097 Uiso 1 1 calc R . .
F4 F 0.964(2) 1.0988(14) 0.9362(5) 0.196(18) Uani 1 1 d . . .
F24 F 0.917(3) 0.876(3) 0.5015(14) 0.124(9) Uani 0.53(3) 1 d P B 1
C21 C 0.7782(17) 1.2141(15) 0.6073(8) 0.080(10) Uani 1 1 d . . .
F44 F 0.3705(16) 0.597(2) 0.5390(6) 0.28(3) Uani 1 1 d GD . .
F43 F 0.3384(14) 0.552(2) 0.5836(8) 0.26(3) Uani 1 1 d GD . .
F45 F 0.3276(15) 0.6621(19) 0.5753(12) 0.28(3) Uani 1 1 d GD . .
C7 C 0.9688(13) 1.2860(13) 0.6553(7) 0.062(7) Uani 1 1 d . . .
C28 C 1.1380(12) 1.0990(15) 0.7648(8) 0.069(8) Uani 1 1 d . . .
C147 C 0.7651(19) 0.7649(16) 0.3417(7) 0.150(4) Uani 1 1 d DU . .
H14A H 0.7255 0.7811 0.3308 0.180 Uiso 1 1 calc R . .
H14B H 0.7933 0.8018 0.3456 0.180 Uiso 1 1 calc R . .
C70 C 1.0994(15) 0.4418(17) 0.6726(13) 0.099(14) Uani 1 1 d . . .
C148 C 0.7918(19) 0.7205(17) 0.3201(7) 0.129(19) Uani 1 1 d D . .
H14C H 0.7647 0.6828 0.3164 0.155 Uiso 1 1 calc R . .
H14D H 0.8327 0.7058 0.3302 0.155 Uiso 1 1 calc R . .
F5 F 0.8990(17) 1.170(2) 0.9239(8) 0.22(2) Uani 1 1 d U . .
C31 C 1.1832(14) 0.9211(18) 0.8331(9) 0.086(10) Uani 1 1 d . . .
H31 H 1.1655 0.9486 0.8469 0.103 Uiso 1 1 calc R . .
C39 C 1.1619(16) 0.622(2) 0.6301(8) 0.100(13) Uani 1 1 d . . .
C37 C 1.1788(15) 0.701(2) 0.6682(9) 0.096(12) Uani 1 1 d . . .
H37 H 1.2059 0.7237 0.6834 0.115 Uiso 1 1 calc R . .
F31 F 1.025(3) 0.689(3) 0.5498(12) 0.151(16) Uani 0.60(4) 1 d P A 1
C38 C 1.2019(16) 0.653(2) 0.6521(9) 0.103(13) Uani 1 1 d . . .
H38 H 1.2443 0.6414 0.6560 0.124 Uiso 1 1 calc R . .
C42 C 1.183(2) 0.567(2) 0.6083(12) 0.113(15) Uani 1 1 d . . .
F23 F 0.980(3) 0.821(3) 0.5331(12) 0.124(9) Uani 0.53(3) 1 d P B 1
C150 C 0.8360(17) 0.7178(19) 0.2687(8) 0.110(14) Uani 1 1 d D . .
H15A H 0.8357 0.7419 0.2492 0.165 Uiso 1 1 calc R . .
H15B H 0.8188 0.6753 0.2639 0.165 Uiso 1 1 calc R . .
H15C H 0.8786 0.7139 0.2790 0.165 Uiso 1 1 calc R . .
F22 F 0.988(3) 0.916(3) 0.5335(12) 0.124(9) Uani 0.53(3) 1 d P B 1
C14 C 0.939(2) 1.1354(18) 0.9161(8) 0.099(13) Uani 1 1 d . . .
C141 C 0.941(2) 1.1363(19) 0.5565(8) 0.1504(17) Uani 1 1 d DU . .
H14P H 0.9685 1.1715 0.5653 0.180 Uiso 1 1 calc R . .
H14Q H 0.9105 1.1289 0.5710 0.180 Uiso 1 1 calc R . .
C157 C 0.8650(15) 0.755(2) 0.3933(10) 0.150(5) Uani 1 1 d DU . .
H15D H 0.8525 0.7974 0.4003 0.179 Uiso 1 1 calc R . .
H15E H 0.8772 0.7602 0.3721 0.179 Uiso 1 1 calc R . .
C93 C 0.6926(12) 0.5697(12) 0.5211(6) 0.123(15) Uiso 1 1 d G . .
H93 H 0.6617 0.5425 0.5274 0.147 Uiso 1 1 calc R . .
C92 C 0.7010(12) 0.6302(12) 0.5341(5) 0.087(10) Uani 1 1 d GU . .
C97 C 0.7461(13) 0.6701(11) 0.5249(6) 0.137(19) Uani 1 1 d GU . .
H97 H 0.7519 0.7113 0.5337 0.165 Uiso 1 1 calc R . .
C96 C 0.7828(12) 0.6495(15) 0.5028(7) 0.123(16) Uani 1 1 d G . .
H96 H 0.8137 0.6768 0.4965 0.148 Uiso 1 1 calc R . .
C95 C 0.7744(13) 0.5891(16) 0.4898(6) 0.125(16) Uani 1 1 d G . .
C94 C 0.7293(15) 0.5492(11) 0.4990(7) 0.114(15) Uani 1 1 d G . .
H94 H 0.7235 0.5079 0.4902 0.137 Uiso 1 1 calc R . .
C35 C 1.2698(13) 0.9923(19) 0.8347(11) 0.099(14) Uani 1 1 d . . .
C158 C 0.9197(14) 0.733(2) 0.4150(10) 0.149(6) Uani 1 1 d DU . .
H15F H 0.9568 0.7563 0.4105 0.179 Uiso 1 1 calc R . .
H15G H 0.9266 0.6870 0.4112 0.179 Uiso 1 1 calc R . .
C140 C 0.908(2) 1.1575(15) 0.5258(10) 0.149(4) Uiso 1 1 d DU . .
H14R H 0.8661 1.1396 0.5235 0.179 Uiso 1 1 calc R . .
H14S H 0.9298 1.1393 0.5089 0.179 Uiso 1 1 calc R . .
C105 C 0.351(3) 0.6052(19) 0.5678(9) 0.21(4) Uani 1 1 d D . .
C132 C 0.7261(13) 1.266(3) 0.5006(10) 0.1504(17) Uani 1 1 d D . .
H13A H 0.7266 1.2465 0.4797 0.180 Uiso 1 1 calc R . .
H13B H 0.7205 1.3124 0.4973 0.180 Uiso 1 1 calc R . .
C77 C 0.974(2) 0.647(3) 0.5441(11) 0.14(2) Uani 1 1 d . . .
C152 C 0.6754(19) 0.827(2) 0.3745(10) 0.1504(17) Uani 1 1 d D . .
H15H H 0.6441 0.7933 0.3704 0.180 Uiso 1 1 calc R . .
H15I H 0.6797 0.8482 0.3543 0.180 Uiso 1 1 calc R . .
C155 C 0.8108(14) 0.7115(16) 0.3914(10) 0.1504(17) Uani 1 1 d DU . .
H15J H 0.8019 0.7019 0.4128 0.180 Uiso 1 1 calc R . .
H15K H 0.8214 0.6710 0.3816 0.180 Uiso 1 1 calc R . .
C149 C 0.799(2) 0.751(2) 0.2893(7) 0.15(2) Uani 1 1 d D . .
H14E H 0.7572 0.7570 0.2777 0.184 Uiso 1 1 calc R . .
H14F H 0.8172 0.7935 0.2936 0.184 Uiso 1 1 calc R . .
F40 F 0.8491(12) 0.5066(12) 0.4813(6) 0.1504(17) Uani 1 1 d D . .
C143 C 0.704(2) 0.6891(17) 0.3693(8) 0.1504(17) Uani 1 1 d DU . .
H14G H 0.6718 0.7021 0.3523 0.180 Uiso 1 1 calc R . .
H14H H 0.7226 0.6489 0.3626 0.180 Uiso 1 1 calc R . .
C128 C 0.823(3) 1.2531(19) 0.4412(7) 0.1504(17) Uani 1 1 d D . .
H12A H 0.8511 1.2901 0.4413 0.180 Uiso 1 1 calc R . .
H12B H 0.7816 1.2692 0.4440 0.180 Uiso 1 1 calc R . .
C137 C 0.937(2) 1.3930(17) 0.5309(9) 0.1504(17) Uani 1 1 d DU . .
H13C H 0.9659 1.3931 0.5150 0.180 Uiso 1 1 calc R . .
H13D H 0.9053 1.4261 0.5249 0.180 Uiso 1 1 calc R . .
C135 C 0.8755(16) 1.3105(12) 0.4986(7) 0.158(6) Uiso 1 1 d DU . .
H13E H 0.9074 1.3071 0.4842 0.190 Uiso 1 1 calc R . .
H13F H 0.8457 1.3438 0.4903 0.190 Uiso 1 1 calc R . .
C133 C 0.6716(14) 1.241(2) 0.5141(14) 0.1504(17) Uani 1 1 d D . .
H13G H 0.6569 1.2023 0.5024 0.180 Uiso 1 1 calc R . .
H13H H 0.6852 1.2282 0.5361 0.180 Uiso 1 1 calc R . .
C130 C 0.871(2) 1.175(2) 0.4075(11) 0.1504(17) Uani 1 1 d D . .
H13I H 0.8735 1.1444 0.4248 0.226 Uiso 1 1 calc R . .
H13J H 0.9104 1.1986 0.4088 0.226 Uiso 1 1 calc R . .
H13K H 0.8644 1.1522 0.3875 0.226 Uiso 1 1 calc R . .
C136 C 0.905(2) 1.3288(19) 0.5304(8) 0.156(6) Uiso 1 1 d DU . .
H13L H 0.9361 1.2961 0.5382 0.188 Uiso 1 1 calc R . .
H13M H 0.8735 1.3298 0.5449 0.188 Uiso 1 1 calc R . .
F32 F 1.006(3) 0.594(3) 0.5468(12) 0.151(16) Uani 0.60(4) 1 d P A 1
C142 C 0.980(2) 1.079(2) 0.5559(11) 0.1504(17) Uani 1 1 d DU . .
H14T H 1.0119 1.0787 0.5740 0.226 Uiso 1 1 calc R . .
H14U H 0.9986 1.0776 0.5365 0.226 Uiso 1 1 calc R . .
H14V H 0.9534 1.0409 0.5569 0.226 Uiso 1 1 calc R . .
F41 F 0.7756(11) 0.5462(13) 0.4413(6) 0.1504(17) Uani 1 1 d D . .
C153 C 0.653(2) 0.876(2) 0.3964(9) 0.1504(17) Uani 1 1 d D . .
H15L H 0.6373 0.8526 0.4138 0.180 Uiso 1 1 calc R . .
H15M H 0.6890 0.9014 0.4056 0.180 Uiso 1 1 calc R . .
C138 C 0.972(2) 1.409(2) 0.5624(10) 0.1504(17) Uani 1 1 d DU . .
H13N H 1.0061 1.3798 0.5674 0.226 Uiso 1 1 calc R . .
H13O H 0.9438 1.4065 0.5785 0.226 Uiso 1 1 calc R . .
H13P H 0.9876 1.4529 0.5619 0.226 Uiso 1 1 calc R . .
C159 C 0.911(2) 0.742(3) 0.4488(9) 0.1504(17) Uani 1 1 d D . .
H15N H 0.8845 0.7788 0.4507 0.226 Uiso 1 1 calc R . .
H15O H 0.9517 0.7495 0.4611 0.226 Uiso 1 1 calc R . .
H15P H 0.8925 0.7039 0.4566 0.226 Uiso 1 1 calc R . .
C134 C 0.6185(17) 1.285(2) 0.5140(13) 0.1504(17) Uani 1 1 d D . .
H13Q H 0.5802 1.2635 0.5057 0.226 Uiso 1 1 calc R . .
H13R H 0.6245 1.3221 0.5007 0.226 Uiso 1 1 calc R . .
H13S H 0.6157 1.3000 0.5354 0.226 Uiso 1 1 calc R . .
C151 C 0.7350(16) 0.7990(16) 0.3873(11) 0.1504(17) Uani 1 1 d DU . .
H15Q H 0.7340 0.7908 0.4099 0.180 Uiso 1 1 calc R . .
H15R H 0.7677 0.8310 0.3857 0.180 Uiso 1 1 calc R . .
C131 C 0.7860(12) 1.256(2) 0.5188(8) 0.1504(17) Uani 1 1 d D . .
H13T H 0.7826 1.2188 0.5328 0.180 Uiso 1 1 calc R . .
H13U H 0.7962 1.2933 0.5323 0.180 Uiso 1 1 calc R . .
C127 C 0.8452(17) 1.2112(15) 0.4674(6) 0.1504(17) Uani 1 1 d D . .
H12C H 0.8888 1.1998 0.4663 0.180 Uiso 1 1 calc R . .
H12D H 0.8206 1.1715 0.4658 0.180 Uiso 1 1 calc R . .
C144 C 0.676(2) 0.6766(19) 0.3981(10) 0.1504(17) Uani 1 1 d D . .
H14I H 0.6445 0.7099 0.4005 0.180 Uiso 1 1 calc R . .
H14J H 0.7076 0.6786 0.4166 0.180 Uiso 1 1 calc R . .
C83 C 0.5612(16) 0.9572(18) 0.5418(9) 0.1504(17) Uani 1 1 d G . .
C82 C 0.5007(19) 0.9750(14) 0.5315(8) 0.1504(17) Uani 1 1 d G . .
H82 H 0.4902 1.0188 0.5294 0.180 Uiso 1 1 calc R . .
C81 C 0.4555(12) 0.929(2) 0.5243(8) 0.1504(17) Uani 1 1 d GD . .
C80 C 0.4709(16) 0.8648(18) 0.5274(8) 0.1504(17) Uani 1 1 d G . .
H80 H 0.4400 0.8333 0.5224 0.180 Uiso 1 1 calc R . .
C79 C 0.5314(19) 0.8470(14) 0.5377(8) 0.1504(17) Uani 1 1 d G . .
H79 H 0.5419 0.8032 0.5398 0.180 Uiso 1 1 calc R . .
C78 C 0.5765(12) 0.893(2) 0.5449(8) 0.1504(17) Uani 1 1 d GU . .
F27 F 1.2040(8) 0.4523(9) 0.8164(7) 0.118(9) Uani 1 1 d . . .
F25 F 1.1535(11) 0.4118(11) 0.7734(9) 0.155(14) Uani 1 1 d . . .
F26 F 1.1211(11) 0.3977(10) 0.8189(8) 0.135(11) Uani 1 1 d . . .
C63 C 1.1474(16) 0.441(2) 0.8008(16) 0.13(2) Uani 1 1 d . . .
C91 C 0.313(2) 0.8292(13) 0.5902(8) 0.1504(17) Uani 1 1 d D . .
C145 C 0.645(2) 0.6117(18) 0.3968(10) 0.1504(17) Uani 1 1 d D . .
H14K H 0.6149 0.6084 0.3774 0.180 Uiso 1 1 calc R . .
H14L H 0.6763 0.5781 0.3962 0.180 Uiso 1 1 calc R . .
C146 C 0.611(2) 0.602(2) 0.4249(11) 0.1504(17) Uani 1 1 d D . .
H14M H 0.5691 0.5873 0.4179 0.226 Uiso 1 1 calc R . .
H14N H 0.6103 0.6416 0.4364 0.226 Uiso 1 1 calc R . .
H14O H 0.6331 0.5692 0.4385 0.226 Uiso 1 1 calc R . .
C154 C 0.605(2) 0.919(2) 0.3817(11) 0.1504(17) Uani 1 1 d D . .
H15S H 0.6207 0.9430 0.3651 0.226 Uiso 1 1 calc R . .
H15T H 0.5925 0.9477 0.3975 0.226 Uiso 1 1 calc R . .
H15U H 0.5689 0.8936 0.3727 0.226 Uiso 1 1 calc R . .
C129 C 0.819(2) 1.220(2) 0.4096(7) 0.1504(17) Uani 1 1 d D . .
H12E H 0.7799 1.1970 0.4056 0.180 Uiso 1 1 calc R . .
H12F H 0.8197 1.2531 0.3931 0.180 Uiso 1 1 calc R . .
N1 N 0.8402(10) 1.2433(12) 0.4997(6) 0.1504(17) Uani 1 1 d DU . .
C139 C 0.9038(13) 1.2276(14) 0.5213(8) 0.1504(17) Uani 1 1 d DU . .
H13V H 0.9391 1.2432 0.5111 0.180 Uiso 1 1 calc R . .
H13W H 0.9048 1.2491 0.5418 0.180 Uiso 1 1 calc R . .
F39 F 0.3040(13) 0.8920(11) 0.5893(7) 0.1504(17) Uani 1 1 d D . .
C98 C 0.8233(17) 0.5575(16) 0.4644(10) 0.1504(17) Uani 1 1 d D . .
F42 F 0.8598(12) 0.6092(12) 0.4621(7) 0.1504(17) Uani 1 1 d D . .
F38 F 0.3272(12) 0.8001(12) 0.5635(5) 0.133(4) Uani 1 1 d D . .
F37 F 0.2951(14) 0.7892(13) 0.6129(6) 0.1504(17) Uani 1 1 d D . .
C84 C 0.3898(18) 0.953(3) 0.5243(15) 0.1504(17) Uani 1 1 d D . .
F36 F 0.383(5) 1.009(3) 0.5257(18) 0.61(8) Uani 1 1 d GU . .
F34 F 0.349(2) 0.916(3) 0.5361(10) 0.25(2) Uani 1 1 d GU . .
F35 F 0.373(2) 0.937(3) 0.4900(9) 0.26(2) Uani 1 1 d GU . .
C56 C 0.948(3) 0.873(3) 0.5303(15) 0.132(17) Uiso 1 1 d . . .
F23A F 0.999(3) 0.866(4) 0.5420(14) 0.124(9) Uani 0.47(3) 1 d P B 2
F22A F 0.946(3) 0.937(3) 0.5181(13) 0.124(9) Uani 0.47(3) 1 d P B 2
F24A F 0.916(4) 0.844(3) 0.5052(16) 0.124(9) Uani 0.47(3) 1 d P B 2
F33A F 0.972(4) 0.687(5) 0.521(2) 0.151(16) Uani 0.40(4) 1 d P A 2
F32A F 0.960(3) 0.581(5) 0.5237(17) 0.151(16) Uani 0.40(4) 1 d P A 2
F31A F 1.031(4) 0.644(6) 0.5515(18) 0.151(16) Uani 0.40(4) 1 d P A 2
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
C C 0.0181 0.0091 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
H H 0.0000 0.0000 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Au Au -4.4197 7.2980 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cu Cu -1.9646 0.5888 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
S S 0.3331 0.5567 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0727 0.0534 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
N N 0.0311 0.0180 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Cl Cl 0.3639 0.7018 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
Au2 Au1 Au3 60.59(3) . .
Au2 Au1 Au4 108.61(4) . .
Au2 Au1 Au5 109.15(3) . .
Au2 Au1 Au6 60.65(3) . 2_656
Au3 Au1 Au4 108.17(3) . .
Au3 Au1 Au6 108.38(3) . 2_656
Au5 Au1 Au3 60.60(3) . .
Au5 Au1 Au4 59.48(3) . .
Au5 Au1 Au6 107.24(3) . 2_656
Au6 Au1 Au4 59.34(3) 2_656 .
Cu5 Au1 Au2 166.32(7) . .
Cu5 Au1 Au3 113.97(7) . .
Cu5 Au1 Au4 59.85(7) . .
Cu5 Au1 Au5 59.50(6) . .
Cu5 Au1 Au6 113.35(7) . 2_656
Cu5 Au1 Cu9 130.62(9) . .
Cu5 Au1 Cu12 68.44(9) . .
Cu5 Au1 Cu15 71.12(10) . .
Cu9 Au1 Au2 59.13(6) . .
Cu9 Au1 Au3 58.55(6) . .
Cu9 Au1 Au4 164.59(7) . .
Cu9 Au1 Au5 113.44(7) . .
Cu9 Au1 Au6 114.92(7) . 2_656
Cu11 Au1 Au2 59.68(7) . .
Cu11 Au1 Au3 115.14(7) . .
Cu11 Au1 Au4 112.50(8) . .
Cu11 Au1 Au5 165.01(7) . .
Cu11 Au1 Au6 59.25(7) . 2_656
Cu11 Au1 Cu5 129.71(9) . .
Cu11 Au1 Cu9 70.81(9) . .
Cu11 Au1 Cu12 67.28(10) . .
Cu11 Au1 Cu15 130.84(10) . .
Cu12 Au1 Au2 113.26(7) . .
Cu12 Au1 Au3 164.52(7) . .
Cu12 Au1 Au4 58.85(7) . .
Cu12 Au1 Au5 112.78(7) . .
Cu12 Au1 Au6 58.69(7) . 2_656
Cu12 Au1 Cu9 132.64(9) . .
Cu15 Au1 Au2 111.26(7) . .
Cu15 Au1 Au3 57.23(7) . .
Cu15 Au1 Au4 115.69(8) . .
Cu15 Au1 Au5 60.79(7) . .
Cu15 Au1 Au6 163.99(7) . 2_656
Cu15 Au1 Cu9 65.45(9) . .
Cu15 Au1 Cu12 134.03(10) . .
Au1 Au2 Au2 107.42(3) . 2_656
Au1 Au2 Au3 60.27(3) . .
Au1 Au2 Au3 108.19(4) . 2_656
Au1 Au2 Au6 60.26(3) . 2_656
Au3 Au2 Au2 58.76(3) . 2_656
Au3 Au2 Au2 60.17(3) 2_656 2_656
Au3 Au2 Au3 107.27(4) 2_656 .
Au3 Au2 Au6 59.83(3) 2_656 2_656
Au3 Au2 Au6 107.82(4) . 2_656
Au6 Au2 Au2 107.59(3) 2_656 2_656
Cu6 Au2 Au1 112.25(7) 2_656 .
Cu6 Au2 Au2 114.92(7) 2_656 2_656
Cu6 Au2 Au3 163.54(7) 2_656 .
Cu6 Au2 Au3 59.51(6) 2_656 2_656
Cu6 Au2 Au6 57.94(6) 2_656 2_656
Cu6 Au2 Cu7 72.52(9) 2_656 2_656
Cu7 Au2 Au1 113.46(7) . .
Cu7 Au2 Au1 162.88(7) 2_656 .
Cu7 Au2 Au2 57.16(6) 2_656 2_656
Cu7 Au2 Au2 59.48(6) . 2_656
Cu7 Au2 Au3 113.72(7) . 2_656
Cu7 Au2 Au3 110.39(7) 2_656 .
Cu7 Au2 Au3 59.29(7) . .
Cu7 Au2 Au3 59.03(6) 2_656 2_656
Cu7 Au2 Au6 114.49(7) 2_656 2_656
Cu7 Au2 Au6 164.66(7) . 2_656
Cu7 Au2 Cu6 133.07(9) . 2_656
Cu7 Au2 Cu7 67.00(12) . 2_656
Cu7 Au2 Cu9 66.71(9) . .
Cu7 Au2 Cu11 132.06(9) . .
Cu9 Au2 Au1 60.03(6) . .
Cu9 Au2 Au2 111.51(7) . 2_656
Cu9 Au2 Au3 58.72(7) . .
Cu9 Au2 Au3 164.40(7) . 2_656
Cu9 Au2 Au6 115.38(7) . 2_656
Cu9 Au2 Cu6 132.63(9) . 2_656
Cu9 Au2 Cu7 129.74(9) . 2_656
Cu11 Au2 Au1 58.50(7) . .
Cu11 Au2 Au2 163.34(7) . 2_656
Cu11 Au2 Au3 113.78(7) . .
Cu11 Au2 Au3 113.26(7) . 2_656
Cu11 Au2 Au6 58.75(7) . 2_656
Cu11 Au2 Cu6 67.65(9) . 2_656
Cu11 Au2 Cu7 135.02(9) . 2_656
Cu11 Au2 Cu9 70.70(9) . .
Au1 Au3 Au2 59.14(3) . .
Au1 Au3 Au5 59.30(3) . .
Au2 Au3 Au1 108.36(4) 2_656 .
Au2 Au3 Au2 61.07(3) 2_656 .
Au2 Au3 Au5 108.42(3) 2_656 .
Au2 Au3 Au5 106.95(4) . .
Au2 Au3 Au6 60.86(3) 2_656 .
Au2 Au3 Cu16 114.88(7) 2_656 .
Au6 Au3 Au1 107.84(4) . .
Au6 Au3 Au2 109.10(4) . .
Au6 Au3 Au5 59.94(3) . .
Au6 Au3 Cu16 58.28(7) . .
Cu6 Au3 Au1 164.17(7) . .
Cu6 Au3 Au2 115.65(7) . .
Cu6 Au3 Au2 59.41(7) . 2_656
Cu6 Au3 Au5 112.76(7) . .
Cu6 Au3 Au6 58.25(7) . .
Cu6 Au3 Cu16 70.53(9) . .
Cu7 Au3 Au1 111.02(7) . .
Cu7 Au3 Au2 59.79(6) . 2_656
Cu7 Au3 Au2 57.68(6) . .
Cu7 Au3 Au5 163.30(7) . .
Cu7 Au3 Au6 116.12(7) . .
Cu7 Au3 Cu6 72.81(9) . .
Cu7 Au3 Cu9 66.20(8) . .
Cu7 Au3 Cu16 137.81(9) . .
Cu9 Au3 Au1 59.73(6) . .
Cu9 Au3 Au2 59.01(7) . .
Cu9 Au3 Au2 113.82(7) . 2_656
Cu9 Au3 Au5 113.33(7) . .
Cu9 Au3 Au6 165.50(7) . .
Cu9 Au3 Cu6 132.65(9) . .
Cu9 Au3 Cu16 130.74(9) . .
Cu15 Au3 Au1 59.59(7) . .
Cu15 Au3 Au2 166.50(8) . 2_656
Cu15 Au3 Au2 112.05(7) . .
Cu15 Au3 Au5 61.09(7) . .
Cu15 Au3 Au6 114.90(8) . .
Cu15 Au3 Cu6 131.00(10) . .
Cu15 Au3 Cu7 128.17(10) . .
Cu15 Au3 Cu9 66.83(9) . .
Cu15 Au3 Cu16 67.67(10) . .
Cu16 Au3 Au1 109.97(7) . .
Cu16 Au3 Au2 161.89(8) . .
Cu16 Au3 Au5 56.23(7) . .
Au1 Au4 Au4 107.41(3) . 2_656
Au1 Au4 Au5 107.43(4) . 2_656
Au5 Au4 Au1 59.79(3) . .
Au5 Au4 Au4 60.03(3) . 2_656
Au5 Au4 Au4 58.72(3) 2_656 2_656
Au5 Au4 Au5 106.92(4) . 2_656
Au5 Au4 Au6 108.23(4) . 2_656
Au6 Au4 Au1 60.29(3) 2_656 .
Au6 Au4 Au4 107.47(3) 2_656 2_656
Au6 Au4 Au5 60.13(3) 2_656 2_656
Cu5 Au4 Au1 57.80(7) . .
Cu5 Au4 Au4 114.26(7) . 2_656
Cu5 Au4 Au5 162.68(7) . 2_656
Cu5 Au4 Au5 58.93(6) . .
Cu5 Au4 Au6 112.36(7) . 2_656
Cu8 Au4 Au1 164.46(7) 2_656 .
Cu8 Au4 Au1 114.93(8) . .
Cu8 Au4 Au4 59.29(7) 2_656 2_656
Cu8 Au4 Au4 56.99(6) . 2_656
Cu8 Au4 Au5 59.70(7) 2_656 2_656
Cu8 Au4 Au5 110.11(7) . 2_656
Cu8 Au4 Au5 113.33(7) 2_656 .
Cu8 Au4 Au5 59.42(7) . .
Cu8 Au4 Au6 113.71(8) 2_656 2_656
Cu8 Au4 Au6 163.01(7) . 2_656
Cu8 Au4 Cu5 72.66(9) . .
Cu8 Au4 Cu5 132.91(10) 2_656 .
Cu8 Au4 Cu8 66.19(13) 2_656 .
Cu8 Au4 Cu10 66.15(9) 2_656 2_656
Cu8 Au4 Cu12 132.16(10) 2_656 .
Cu10 Au4 Au1 116.33(7) 2_656 .
Cu10 Au4 Au4 110.95(7) 2_656 2_656
Cu10 Au4 Au5 164.50(7) 2_656 .
Cu10 Au4 Au5 58.72(6) 2_656 2_656
Cu10 Au4 Au6 60.73(7) 2_656 2_656
Cu10 Au4 Cu5 133.75(9) 2_656 .
Cu10 Au4 Cu8 128.41(10) 2_656 .
Cu10 Au4 Cu12 71.63(9) 2_656 .
Cu12 Au4 Au1 59.22(7) . .
Cu12 Au4 Au4 163.94(7) . 2_656
Cu12 Au4 Au5 113.38(7) . .
Cu12 Au4 Au5 114.32(7) . 2_656
Cu12 Au4 Au6 59.14(7) . 2_656
Cu12 Au4 Cu5 67.76(9) . .
Cu12 Au4 Cu8 134.66(9) . .
Au1 Au5 Au3 60.10(3) . .
Au1 Au5 Au4 109.11(4) . 2_656
Au1 Au5 Au6 108.12(4) . .
Au4 Au5 Au1 60.73(3) . .
Au4 Au5 Au3 108.77(4) . .
Au4 Au5 Au3 107.31(3) 2_656 .
Au4 Au5 Au4 61.26(3) . 2_656
Au4 Au5 Au6 108.89(4) . .
Au4 Au5 Cu15 114.59(7) . .
Au6 Au5 Au3 59.48(3) . .
Au6 Au5 Au4 59.37(3) . 2_656
Cu5 Au5 Au1 58.43(7) . .
Cu5 Au5 Au3 112.58(7) . .
Cu5 Au5 Au4 59.95(7) . .
Cu5 Au5 Au4 116.30(7) . 2_656
Cu5 Au5 Au6 165.03(8) . .
Cu5 Au5 Cu8 73.13(9) . .
Cu5 Au5 Cu15 69.63(9) . .
Cu8 Au5 Au1 115.83(7) . .
Cu8 Au5 Au3 163.34(7) . .
Cu8 Au5 Au4 57.42(6) . 2_656
Cu8 Au5 Au4 59.47(7) . .
Cu8 Au5 Au6 110.99(7) . .
Cu8 Au5 Cu15 137.57(9) . .
Cu10 Au5 Au1 165.98(7) . .
Cu10 Au5 Au3 114.41(7) . .
Cu10 Au5 Au4 58.81(7) . 2_656
Cu10 Au5 Au4 113.27(7) . .
Cu10 Au5 Au6 60.48(7) . .
Cu10 Au5 Cu5 131.53(10) . .
Cu10 Au5 Cu8 65.29(9) . .
Cu10 Au5 Cu15 131.32(10) . .
Cu15 Au5 Au1 58.34(7) . .
Cu15 Au5 Au3 56.33(7) . .
Cu15 Au5 Au4 162.26(8) . 2_656
Cu15 Au5 Au6 110.26(7) . .
Cu16 Au5 Au1 115.46(8) . .
Cu16 Au5 Au3 61.57(8) . .
Cu16 Au5 Au4 167.45(8) . .
Cu16 Au5 Au4 112.30(7) . 2_656
Cu16 Au5 Au6 59.86(7) . .
Cu16 Au5 Cu5 129.84(10) . .
Cu16 Au5 Cu8 127.84(10) . .
Cu16 Au5 Cu10 67.39(9) . .
Cu16 Au5 Cu15 67.93(9) . .
Au1 Au6 Au2 59.10(3) 2_656 2_656
Au3 Au6 Au1 106.84(3) . 2_656
Au3 Au6 Au2 59.31(3) . 2_656
Au3 Au6 Au5 60.57(3) . .
Au4 Au6 Au1 60.37(3) 2_656 2_656
Au4 Au6 Au2 108.18(4) 2_656 2_656
Au4 Au6 Au3 109.08(3) 2_656 .
Au4 Au6 Au5 60.50(3) 2_656 .
Au5 Au6 Au1 107.78(4) . 2_656
Au5 Au6 Au2 107.70(3) . 2_656
Cu6 Au6 Au1 112.49(7) . 2_656
Cu6 Au6 Au2 59.37(7) . 2_656
Cu6 Au6 Au3 59.80(6) . .
Cu6 Au6 Au4 165.89(7) . 2_656
Cu6 Au6 Au5 114.71(7) . .
Cu6 Au6 Cu10 132.23(9) . .
Cu6 Au6 Cu11 68.24(9) . 2_656
Cu6 Au6 Cu12 129.46(9) . 2_656
Cu6 Au6 Cu16 72.41(10) . .
Cu10 Au6 Au1 114.32(7) . 2_656
Cu10 Au6 Au2 163.39(7) . 2_656
Cu10 Au6 Au3 113.27(7) . .
Cu10 Au6 Au4 58.44(7) . 2_656
Cu10 Au6 Au5 58.12(6) . .
Cu11 Au6 Au1 58.11(7) 2_656 2_656
Cu11 Au6 Au2 58.77(7) 2_656 2_656
Cu11 Au6 Au3 112.81(7) 2_656 .
Cu11 Au6 Au4 112.39(7) 2_656 2_656
Cu11 Au6 Au5 163.50(8) 2_656 .
Cu11 Au6 Cu10 133.16(9) 2_656 .
Cu11 Au6 Cu12 67.09(9) 2_656 2_656
Cu11 Au6 Cu16 135.15(10) 2_656 .
Cu12 Au6 Au1 59.34(7) 2_656 2_656
Cu12 Au6 Au2 112.45(7) 2_656 2_656
Cu12 Au6 Au3 164.65(7) 2_656 .
Cu12 Au6 Au4 59.41(7) 2_656 2_656
Cu12 Au6 Au5 114.90(7) 2_656 .
Cu12 Au6 Cu10 70.77(9) 2_656 .
Cu12 Au6 Cu16 130.67(10) 2_656 .
Cu16 Au6 Au1 163.60(7) . 2_656
Cu16 Au6 Au2 116.07(8) . 2_656
Cu16 Au6 Au3 61.13(7) . .
Cu16 Au6 Au4 111.06(8) . 2_656
Cu16 Au6 Au5 57.30(7) . .
Cu16 Au6 Cu10 65.45(9) . .
Cu1 Au7 Cu1 83.68(12) 2_656 .
S1 Au7 Cu1 129.86(17) 2_656 .
S1 Au7 Cu1 47.74(17) . .
S1 Au7 Cu1 47.74(17) 2_656 2_656
S1 Au7 Cu1 129.86(17) . 2_656
S1 Au7 S1 177.6(3) . 2_656
Cu2 Au8 Cu2 84.06(12) . 2_656
S17 Au8 Cu2 48.21(16) 2_656 2_656
S17 Au8 Cu2 130.18(17) . 2_656
S17 Au8 Cu2 130.18(17) 2_656 .
S17 Au8 Cu2 48.21(16) . .
S17 Au8 S17 178.4(3) . 2_656
Cu3 Au9 Cu4 84.41(9) . .
S5 Au9 Cu3 51.00(16) . .
S5 Au9 Cu4 134.67(16) . .
S6 Au9 Cu3 128.80(17) . .
S6 Au9 Cu4 45.78(15) . .
S6 Au9 S5 177.5(3) . .
Cu14 Au10 Cu13 84.68(13) . .
S14 Au10 Cu13 135.5(3) . .
S14 Au10 Cu14 51.4(3) . .
S14 Au10 S12 174.7(4) . .
S12 Au10 Cu13 49.0(2) . .
S12 Au10 Cu14 133.5(2) . .
Cu7 Cu1 Au7 90.63(10) 2_656 .
S2 Cu1 Au7 115.35(17) . .
S2 Cu1 Cu7 47.88(15) . 2_656
S2 Cu1 S1 109.8(2) . .
S3 Cu1 Au7 106.79(18) . .
S3 Cu1 Cu7 100.25(17) . 2_656
S3 Cu1 S2 124.8(2) . .
S3 Cu1 S1 124.8(2) . .
S1 Cu1 Au7 48.27(17) . .
S1 Cu1 Cu7 123.6(2) . 2_656
Cu8 Cu2 Au8 91.28(10) . .
S18 Cu2 Au8 117.62(19) . .
S18 Cu2 Cu8 48.96(15) . .
S18 Cu2 S17 109.1(3) . .
S16 Cu2 Au8 104.97(18) 2_656 .
S16 Cu2 Cu8 99.64(18) 2_656 .
S16 Cu2 S18 124.6(2) 2_656 .
S16 Cu2 S17 125.6(3) 2_656 .
S17 Cu2 Au8 49.09(18) . .
S17 Cu2 Cu8 123.4(2) . .
S4 Cu3 Au9 108.88(18) . .
S4 Cu3 S9 123.6(2) . .
S4 Cu3 S5 124.1(3) . .
S9 Cu3 Au9 112.44(18) . .
S9 Cu3 S5 111.6(3) . .
S5 Cu3 Au9 51.40(19) . .
Cu11 Cu4 Au9 89.27(11) . .
Cu11 Cu4 Cu12 58.66(10) . .
Cu12 Cu4 Au9 87.83(11) . .
S10 Cu4 Au9 111.34(19) . .
S10 Cu4 Cu11 100.48(18) . .
S10 Cu4 Cu12 47.58(16) . .
S10 Cu4 S7 120.1(2) . .
S10 Cu4 S6 126.7(3) . .
S7 Cu4 Au9 116.2(2) . .
S7 Cu4 Cu11 48.18(17) . .
S7 Cu4 Cu12 100.05(18) . .
S6 Cu4 Au9 46.51(19) . .
S6 Cu4 Cu11 122.1(2) . .
S6 Cu4 Cu12 131.9(2) . .
S6 Cu4 S7 112.2(3) . .
Au1 Cu5 Au4 62.35(7) . .
Au1 Cu5 Au5 62.07(7) . .
Au1 Cu5 Cu12 56.59(8) . .
Au4 Cu5 Cu12 55.84(8) . .
Au5 Cu5 Au4 61.12(7) . .
Au5 Cu5 Cu12 105.67(11) . .
S10 Cu5 Au1 81.63(15) . .
S10 Cu5 Au4 102.97(17) . .
S10 Cu5 Au5 143.70(18) . .
S10 Cu5 Cu12 47.52(15) . .
S18 Cu5 Au1 142.17(18) . .
S18 Cu5 Au4 80.02(16) . .
S18 Cu5 Au5 97.47(16) . .
S18 Cu5 Cu12 106.07(19) . .
S18 Cu5 S10 112.3(2) . .
S18 Cu5 S11 107.0(2) . .
S11 Cu5 Au1 100.79(17) . .
S11 Cu5 Au4 141.74(17) . .
S11 Cu5 Au5 80.62(15) . .
S11 Cu5 Cu12 145.16(19) . .
S11 Cu5 S10 108.3(2) . .
Au2 Cu6 Au3 61.07(6) 2_656 .
Au2 Cu6 Cu11 55.98(8) 2_656 2_656
Au3 Cu6 Cu11 105.34(11) . 2_656
Au6 Cu6 Au2 62.69(7) . 2_656
Au6 Cu6 Au3 61.95(7) . .
Au6 Cu6 Cu11 56.33(8) . 2_656
S4 Cu6 Au2 103.36(18) 2_656 2_656
S4 Cu6 Au3 143.97(18) 2_656 .
S4 Cu6 Au6 82.03(15) 2_656 .
S4 Cu6 Cu11 47.90(16) 2_656 2_656
S2 Cu6 Au2 80.08(15) 2_656 2_656
S2 Cu6 Au3 96.93(16) 2_656 .
S2 Cu6 Au6 142.46(18) 2_656 .
S2 Cu6 Cu11 107.27(18) 2_656 2_656
S2 Cu6 S4 112.9(2) 2_656 2_656
S2 Cu6 S13 108.5(3) 2_656 .
S13 Cu6 Au2 141.30(19) . 2_656
S13 Cu6 Au3 80.28(16) . .
S13 Cu6 Au6 98.6(2) . .
S13 Cu6 Cu11 142.8(2) . 2_656
S13 Cu6 S4 107.2(2) . 2_656
Au2 Cu7 Au2 63.36(7) . 2_656
Au2 Cu7 Au3 63.03(7) . .
Au2 Cu7 Cu1 120.02(12) . 2_656
Au2 Cu7 Cu1 76.94(9) 2_656 2_656
Au2 Cu7 Cu7 57.58(8) . 2_656
Au2 Cu7 Cu7 55.42(7) 2_656 2_656
Au2 Cu7 Cu9 57.57(8) . .
Au2 Cu7 Cu9 107.50(11) 2_656 .
Au3 Cu7 Au2 61.17(7) . 2_656
Au3 Cu7 Cu1 131.13(12) . 2_656
Au3 Cu7 Cu7 106.13(6) . 2_656
Au3 Cu7 Cu9 56.95(8) . .
Cu7 Cu7 Cu1 63.14(10) 2_656 2_656
Cu9 Cu7 Cu1 170.91(14) . 2_656
Cu9 Cu7 Cu7 112.42(13) . 2_656
S2 Cu7 Au2 81.18(16) 2_656 2_656
S2 Cu7 Au2 144.49(18) 2_656 .
S2 Cu7 Au3 99.22(17) 2_656 .
S2 Cu7 Cu1 47.49(16) 2_656 2_656
S2 Cu7 Cu7 104.46(19) 2_656 2_656
S2 Cu7 Cu9 140.16(19) 2_656 .
S2 Cu7 S3 133.2(2) 2_656 .
S3 Cu7 Au2 82.15(16) . .
S3 Cu7 Au2 144.67(19) . 2_656
S3 Cu7 Au3 110.97(17) . .
S3 Cu7 Cu1 117.82(18) . 2_656
S3 Cu7 Cu7 100.50(19) . 2_656
S3 Cu7 Cu9 54.04(15) . .
Au4 Cu8 Au4 63.72(7) 2_656 .
Au4 Cu8 Au5 62.88(7) 2_656 .
Au4 Cu8 Cu2 78.04(10) . .
Au4 Cu8 Cu2 121.66(13) 2_656 .
Au4 Cu8 Cu8 58.00(8) 2_656 2_656
Au4 Cu8 Cu8 55.81(8) . 2_656
Au4 Cu8 Cu10 57.76(8) 2_656 .
Au4 Cu8 Cu10 107.93(11) . .
Au5 Cu8 Au4 61.11(7) . .
Au5 Cu8 Cu2 131.69(12) . .
Au5 Cu8 Cu8 106.35(7) . 2_656
Au5 Cu8 Cu10 57.06(8) . .
Cu8 Cu8 Cu2 64.31(11) 2_656 .
Cu10 Cu8 Cu2 170.93(14) . .
Cu10 Cu8 Cu8 112.94(13) . 2_656
S18 Cu8 Au4 81.10(16) . .
S18 Cu8 Au4 144.67(19) . 2_656
S18 Cu8 Au5 98.22(16) . .
S18 Cu8 Cu2 47.95(16) . .
S18 Cu8 Cu8 105.5(2) . 2_656
S18 Cu8 Cu10 138.6(2) . .
S18 Cu8 S16 132.3(2) . .
S16 Cu8 Au4 82.98(16) . 2_656
S16 Cu8 Au4 145.72(18) . .
S16 Cu8 Au5 111.92(18) . .
S16 Cu8 Cu2 116.38(19) . .
S16 Cu8 Cu8 100.51(19) . 2_656
S16 Cu8 Cu10 54.88(16) . .
Au1 Cu9 Cu7 105.41(10) . .
Au1 Cu9 Cu15 56.62(8) . .
Au2 Cu9 Au1 60.84(6) . .
Au2 Cu9 Cu7 55.72(8) . .
Au2 Cu9 Cu15 105.65(11) . .
Au3 Cu9 Au1 61.72(6) . .
Au3 Cu9 Au2 62.26(6) . .
Au3 Cu9 Cu7 56.86(8) . .
Au3 Cu9 Cu15 55.38(8) . .
Cu15 Cu9 Cu7 109.01(12) . .
S7 Cu9 Au1 77.17(16) . .
S7 Cu9 Au2 100.73(17) . .
S7 Cu9 Au3 138.83(18) . .
S7 Cu9 Cu7 145.9(2) . .
S7 Cu9 Cu15 100.73(18) . .
S7 Cu9 S3 106.6(2) . .
S7 Cu9 S8 112.0(2) . .
S3 Cu9 Au1 138.36(17) . .
S3 Cu9 Au2 78.00(14) . .
S3 Cu9 Au3 105.71(15) . .
S3 Cu9 Cu7 48.88(13) . .
S3 Cu9 Cu15 151.29(18) . .
S8 Cu9 Au1 106.27(18) . .
S8 Cu9 Au2 141.35(18) . .
S8 Cu9 Au3 79.41(16) . .
S8 Cu9 Cu7 100.06(18) . .
S8 Cu9 Cu15 49.72(17) . .
S8 Cu9 S3 110.0(2) . .
Au4 Cu10 Au6 60.83(7) 2_656 .
Au4 Cu10 Cu8 56.09(8) 2_656 .
Au4 Cu10 Cu16 105.74(11) 2_656 .
Au5 Cu10 Au4 62.47(7) . 2_656
Au5 Cu10 Au6 61.39(7) . .
Au5 Cu10 Cu8 57.64(8) . .
Au5 Cu10 Cu16 55.33(8) . .
Au6 Cu10 Cu8 105.84(11) . .
Au6 Cu10 Cu16 56.39(9) . .
Cu8 Cu10 Cu16 109.69(12) . .
S9 Cu10 Au4 99.92(17) 2_656 2_656
S9 Cu10 Au5 138.17(18) 2_656 .
S9 Cu10 Au6 76.83(15) 2_656 .
S9 Cu10 Cu8 145.22(19) 2_656 .
S9 Cu10 Cu16 100.58(18) 2_656 .
S9 Cu10 S16 106.0(2) 2_656 .
S16 Cu10 Au4 78.64(15) . 2_656
S16 Cu10 Au5 106.80(16) . .
S16 Cu10 Au6 138.94(18) . .
S16 Cu10 Cu8 49.18(14) . .
S16 Cu10 Cu16 151.97(18) . .
S15 Cu10 Au4 141.2(2) . 2_656
S15 Cu10 Au5 79.00(18) . .
S15 Cu10 Au6 105.2(2) . .
S15 Cu10 Cu8 100.6(2) . .
S15 Cu10 Cu16 48.91(19) . .
S15 Cu10 S9 112.3(2) . 2_656
S15 Cu10 S16 110.8(2) . .
Au1 Cu11 Au2 61.81(7) . .
Au1 Cu11 Au6 62.64(7) . 2_656
Au1 Cu11 Cu4 79.20(10) . .
Au1 Cu11 Cu6 106.00(10) . 2_656
Au1 Cu11 Cu12 57.19(8) . .
Au2 Cu11 Cu4 136.51(13) . .
Au2 Cu11 Cu6 56.36(8) . 2_656
Au2 Cu11 Cu12 107.02(10) . .
Au6 Cu11 Au2 62.48(6) 2_656 .
Au6 Cu11 Cu4 116.93(12) 2_656 .
Au6 Cu11 Cu6 55.43(8) 2_656 2_656
Au6 Cu11 Cu12 56.47(8) 2_656 .
Cu6 Cu11 Cu4 163.39(15) 2_656 .
Cu12 Cu11 Cu4 60.83(10) . .
Cu12 Cu11 Cu6 108.20(12) . 2_656
S4 Cu11 Au1 145.69(19) . .
S4 Cu11 Au2 106.58(17) . .
S4 Cu11 Au6 83.21(17) . 2_656
S4 Cu11 Cu4 116.69(18) . .
S4 Cu11 Cu6 50.77(15) . 2_656
S4 Cu11 Cu12 102.16(19) . .
S4 Cu11 S7 133.4(2) . .
S7 Cu11 Au1 80.32(17) . .
S7 Cu11 Au2 103.80(18) . .
S7 Cu11 Au6 142.8(2) . 2_656
S7 Cu11 Cu4 47.79(17) . .
S7 Cu11 Cu6 147.9(2) . 2_656
S7 Cu11 Cu12 101.67(19) . .
Au1 Cu12 Cu4 78.25(10) . .
Au1 Cu12 Cu5 54.98(8) . .
Au1 Cu12 Cu11 55.53(8) . .
Au4 Cu12 Au1 61.93(7) . .
Au4 Cu12 Cu4 135.85(13) . .
Au4 Cu12 Cu5 56.40(8) . .
Au4 Cu12 Cu11 105.69(10) . .
Au6 Cu12 Au1 61.97(7) 2_656 .
Au6 Cu12 Au4 61.45(6) 2_656 .
Au6 Cu12 Cu4 116.58(12) 2_656 .
Au6 Cu12 Cu5 105.35(10) 2_656 .
Au6 Cu12 Cu11 56.44(8) 2_656 .
Cu5 Cu12 Cu4 86.02(11) . .
Cu11 Cu12 Cu4 60.51(10) . .
Cu11 Cu12 Cu5 106.85(12) . .
S9 Cu12 Au1 141.80(18) . .
S9 Cu12 Au4 102.49(16) . .
S9 Cu12 Au6 79.87(16) . 2_656
S9 Cu12 Cu4 121.07(18) . .
S9 Cu12 Cu5 147.37(19) . .
S9 Cu12 Cu11 102.73(18) . .
S10 Cu12 Au1 82.49(16) . .
S10 Cu12 Au4 106.66(17) . .
S10 Cu12 Au6 144.23(19) . 2_656
S10 Cu12 Cu4 46.34(16) . .
S10 Cu12 Cu5 50.69(15) . .
S10 Cu12 Cu11 101.08(18) . .
S10 Cu12 S9 135.3(2) . .
Au10 Cu13 Cu15 93.42(14) . .
Au10 Cu13 Cu16 89.54(13) . .
Cu15 Cu13 Cu16 59.83(11) . .
S8 Cu13 Au10 116.7(2) . .
S8 Cu13 Cu15 49.31(19) . .
S8 Cu13 Cu16 103.8(2) . .
S8 Cu13 S13 122.4(3) . .
S8 Cu13 S12 115.9(3) . .
S13 Cu13 Au10 111.8(2) . .
S13 Cu13 Cu15 100.2(2) . .
S13 Cu13 Cu16 47.2(2) . .
S13 Cu13 S12 118.9(3) . .
S12 Cu13 Au10 48.7(3) . .
S12 Cu13 Cu15 132.3(3) . .
S12 Cu13 Cu16 131.5(3) . .
S11 Cu14 Au10 114.6(2) . .
S11 Cu14 S15 119.0(3) . .
S11 Cu14 S14 129.7(3) . .
S15 Cu14 Au10 110.8(2) . .
S15 Cu14 S14 110.2(4) . .
S14 Cu14 Au10 50.7(3) . .
Au1 Cu15 Au5 60.87(7) . .
Au1 Cu15 Cu9 57.93(9) . .
Au1 Cu15 Cu13 140.35(14) . .
Au1 Cu15 Cu16 106.00(11) . .
Au3 Cu15 Au1 63.18(7) . .
Au3 Cu15 Au5 62.58(7) . .
Au3 Cu15 Cu9 57.79(8) . .
Au3 Cu15 Cu13 79.57(11) . .
Au3 Cu15 Cu16 58.67(9) . .
Au5 Cu15 Cu9 107.55(11) . .
Au5 Cu15 Cu13 114.36(12) . .
Au5 Cu15 Cu16 53.99(8) . .
Cu9 Cu15 Cu13 91.63(13) . .
Cu9 Cu15 Cu16 113.86(12) . .
Cu13 Cu15 Cu16 60.73(11) . .
S11 Cu15 Au1 102.47(18) . .
S11 Cu15 Au3 143.24(19) . .
S11 Cu15 Au5 80.77(17) . .
S11 Cu15 Cu9 145.45(19) . .
S11 Cu15 Cu13 116.0(2) . .
S11 Cu15 Cu16 98.31(18) . .
S11 Cu15 S8 132.8(2) . .
S8 Cu15 Au1 110.92(19) . .
S8 Cu15 Au3 82.95(17) . .
S8 Cu15 Au5 144.84(19) . .
S8 Cu15 Cu9 53.06(17) . .
S8 Cu15 Cu13 47.78(18) . .
S8 Cu15 Cu16 103.3(2) . .
Au3 Cu16 Cu10 107.13(12) . .
Au3 Cu16 Cu13 76.52(11) . .
Au3 Cu16 Cu15 53.67(8) . .
Au5 Cu16 Au3 62.20(7) . .
Au5 Cu16 Au6 62.85(7) . .
Au5 Cu16 Cu10 57.28(9) . .
Au5 Cu16 Cu13 117.14(13) . .
Au5 Cu16 Cu15 58.09(9) . .
Au6 Cu16 Au3 60.60(7) . .
Au6 Cu16 Cu10 58.15(9) . .
Au6 Cu16 Cu13 131.31(14) . .
Au6 Cu16 Cu15 105.25(11) . .
Cu10 Cu16 Cu13 167.62(15) . .
Cu10 Cu16 Cu15 112.71(13) . .
Cu15 Cu16 Cu13 59.44(11) . .
S15 Cu16 Au3 143.8(2) . .
S15 Cu16 Au5 82.2(2) . .
S15 Cu16 Au6 110.1(2) . .
S15 Cu16 Cu10 52.06(18) . .
S15 Cu16 Cu13 118.2(2) . .
S15 Cu16 Cu15 103.0(2) . .
S13 Cu16 Au3 80.5(2) . .
S13 Cu16 Au5 142.7(2) . .
S13 Cu16 Au6 100.3(2) . .
S13 Cu16 Cu10 143.9(2) . .
S13 Cu16 Cu13 47.7(2) . .
S13 Cu16 Cu15 100.3(2) . .
S13 Cu16 S15 134.7(3) . .
Cu3 S4 Cu6 126.2(3) . 2_656
Cu3 S4 Cu11 90.4(2) . .
Cu11 S4 Cu6 81.3(2) . 2_656
C22 S4 Cu3 116.3(8) . .
C22 S4 Cu6 116.4(8) . 2_656
C22 S4 Cu11 110.5(10) . .
Cu3 S9 Cu10 132.9(3) . 2_656
Cu3 S9 Cu12 88.1(2) . .
Cu12 S9 Cu10 85.6(2) . 2_656
C57 S9 Cu3 112.8(7) . .
C57 S9 Cu10 111.4(7) . 2_656
C57 S9 Cu12 117.5(9) . .
Cu4 S10 Cu5 129.7(3) . .
Cu4 S10 Cu12 86.1(2) . .
Cu12 S10 Cu5 81.79(19) . .
C64 S10 Cu4 114.3(8) . .
C64 S10 Cu5 115.3(8) . .
C64 S10 Cu12 113.4(9) . .
Cu4 S7 Cu9 135.1(3) . .
Cu4 S7 Cu11 84.0(2) . .
Cu11 S7 Cu9 84.36(19) . .
C43 S7 Cu4 112.7(7) . .
C43 S7 Cu9 111.2(7) . .
C43 S7 Cu11 116.9(9) . .
Cu1 S2 Cu6 127.1(3) . 2_656
Cu1 S2 Cu7 84.6(2) . 2_656
Cu7 S2 Cu6 89.0(2) 2_656 2_656
C8 S2 Cu1 116.8(8) . .
C8 S2 Cu6 113.2(8) . 2_656
C8 S2 Cu7 115.4(9) . 2_656
Cu2 S18 Cu5 128.7(3) . .
Cu2 S18 Cu8 83.1(2) . .
Cu8 S18 Cu5 89.1(2) . .
C120 S18 Cu2 117.3(8) . .
C120 S18 Cu5 112.4(7) . .
C120 S18 Cu8 113.0(8) . .
Cu1 S3 Cu7 88.5(2) . .
Cu1 S3 Cu9 131.5(3) . .
Cu7 S3 Cu9 77.08(18) . .
C15 S3 Cu1 107.4(6) . .
C15 S3 Cu7 111.6(7) . .
C15 S3 Cu9 121.0(6) . .
Cu2 S16 Cu8 88.7(2) 2_656 .
Cu2 S16 Cu10 130.7(3) 2_656 .
Cu8 S16 Cu10 75.93(19) . .
C106 S16 Cu2 107.9(7) . 2_656
C106 S16 Cu8 112.7(7) . .
C106 S16 Cu10 121.3(7) . .
Cu14 S11 Cu5 130.0(3) . .
Cu14 S11 Cu15 91.8(2) . .
Cu15 S11 Cu5 84.8(2) . .
C71 S11 Cu5 109.9(8) . .
C71 S11 Cu14 115.0(8) . .
C71 S11 Cu15 119.0(9) . .
Cu14 S15 Cu10 135.8(3) . .
Cu14 S15 Cu16 88.3(3) . .
Cu16 S15 Cu10 79.0(2) . .
C99 S15 Cu10 112.4(11) . .
C99 S15 Cu14 111.1(11) . .
C99 S15 Cu16 116.8(11) . .
Cu13 S8 Cu9 132.8(3) . .
Cu13 S8 Cu15 82.9(2) . .
Cu15 S8 Cu9 77.2(2) . .
C50 S8 Cu9 114.2(10) . .
C50 S8 Cu13 112.6(10) . .
C50 S8 Cu15 108.6(9) . .
Cu13 S13 Cu6 128.5(3) . .
Cu16 S13 Cu6 87.6(3) . .
Cu16 S13 Cu13 85.1(2) . .
C85 S13 Cu6 111.2(12) . .
C85 S13 Cu13 118.7(12) . .
C85 S13 Cu16 112.2(14) . .
Cu2 S17 Au8 82.7(2) . .
C113 S17 Au8 106.6(9) . .
C113 S17 Cu2 109.0(9) . .
Cu1 S1 Au7 84.0(2) . .
C1 S1 Au7 109.5(8) . .
C1 S1 Cu1 110.1(8) . .
Cu3 S5 Au9 77.6(2) . .
C29 S5 Au9 105.1(9) . .
C29 S5 Cu3 109.8(9) . .
Cu4 S6 Au9 87.7(2) . .
C36 S6 Au9 105.7(8) . .
C36 S6 Cu4 109.5(8) . .
Au10 S14 Cu14 77.8(3) . .
C92 S14 Au10 106.8(10) . .
C92 S14 Cu14 118.5(10) . .
Au10 S12 Cu13 82.3(4) . .
C78 S12 Au10 108.9(16) . .
C78 S12 Cu13 123.3(13) . .
C44 C43 S7 123.9(18) . .
C44 C43 C48 118(2) . .
C48 C43 S7 117.9(18) . .
C1 C6 C5 117(2) . .
C23 C22 S4 119.4(18) . .
C23 C22 C27 117(2) . .
C27 C22 S4 124(2) . .
C65 C64 S10 116(2) . .
C65 C64 C69 122(2) . .
C69 C64 S10 121(2) . .
C58 C57 S9 122.6(19) . .
C62 C57 S9 118.4(19) . .
C62 C57 C58 119(2) . .
C111 C106 S16 120.0(17) . .
C111 C106 C107 122(2) . .
C107 C106 S16 118.3(16) . .
C43 C44 C45 125(2) . .
C117 C116 C119 118(2) . .
C115 C116 C119 120(2) . .
C115 C116 C117 121(2) . .
C76 C71 S11 121(2) . .
C72 C71 S11 119(2) . .
C72 C71 C76 120(2) . .
C10 C9 C8 122(2) . .
F50 C119 F49 104(2) . .
F50 C119 C116 116(2) . .
F49 C119 C116 111(2) . .
F51 C119 F50 108(2) . .
F51 C119 F49 105(2) . .
F51 C119 C116 112(2) . .
C106 C111 C110 121(2) . .
C9 C8 S2 123.0(18) . .
C9 C8 C13 115(2) . .
C13 C8 S2 122(2) . .
C22 C23 C24 120(2) . .
C2 C3 C4 123(3) . .
C44 C45 C46 117(2) . .
C4 C5 C6 123(2) . .
C15 C20 C19 119(2) . .
C41 C36 S6 117.2(19) . .
C37 C36 S6 121(2) . .
C37 C36 C41 121(3) . .
C75 C76 C71 120(3) . .
C101 C102 C103 120.0 . .
C101 C102 C105 120.4(18) . .
C103 C102 C105 119.5(18) . .
C102 C101 C100 120.0 . .
C99 C100 C101 120.0 . .
C100 C99 S15 122.3(18) . .
C104 C99 S15 117.7(18) . .
C104 C99 C100 120.0 . .
C99 C104 C103 120.0 . .
C104 C103 C102 120.0 . .
C114 C113 S17 124(2) . .
C118 C113 S17 115(2) . .
C118 C113 C114 121(3) . .
C115 C114 C113 118(2) . .
C122 C121 C120 120(2) . .
C51 C50 S8 122(2) . .
C55 C50 S8 119(2) . .
C55 C50 C51 119(2) . .
C46 C47 C48 119(2) . .
C3 C4 C7 123(2) . .
C5 C4 C3 116(2) . .
C5 C4 C7 120(2) . .
C9 C10 C11 120(3) . .
C26 C27 C22 123(2) . .
C109 C110 C111 118(2) . .
C17 C16 C15 122(2) . .
C6 C1 S1 121.5(19) . .
C2 C1 S1 118.5(17) . .
C2 C1 C6 120(2) . .
C59 C58 C57 122(2) . .
C122 C123 C124 121(2) . .
C122 C123 C126 120(3) . .
C124 C123 C126 118(3) . .
C43 C48 C47 121(2) . .
C108 C107 C106 119(2) . .
C121 C120 S18 121.9(19) . .
C121 C120 C125 120(2) . .
C125 C120 S18 117.9(17) . .
C147 N2 C155 113.0(16) . .
C147 N2 C143 111.8(19) . .
C143 N2 C155 109(3) . .
C151 N2 C147 99(3) . .
C151 N2 C155 110.5(18) . .
C151 N2 C143 114.0(19) . .
C116 C117 C118 117(2) . .
C64 C65 C66 117(3) . .
C20 C15 S3 119.5(18) . .
C20 C15 C16 120(2) . .
C16 C15 S3 120.9(15) . .
C69 C68 C67 119(3) . .
C58 C59 C60 121(2) . .
C27 C26 C25 121(2) . .
C124 C125 C120 121(2) . .
C26 C25 C28 122(3) . .
C24 C25 C26 117(2) . .
C24 C25 C28 120(3) . .
C68 C67 C70 118(3) . .
C66 C67 C68 120(2) . .
C66 C67 C70 120(3) . .
C45 C46 C49 119(2) . .
C47 C46 C45 121(2) . .
C47 C46 C49 120(2) . .
C68 C69 C64 120(2) . .
C25 C24 C23 122(3) . .
C121 C122 C123 121(2) . .
C67 C66 C65 120(3) . .
C116 C115 C114 123(2) . .
C86 C85 S13 114(3) . .
C86 C85 C90 120.0 . .
C90 C85 S13 125(3) . .
C85 C86 C87 120.0 . .
C88 C87 C86 120.0 . .
C87 C88 C89 120.0 . .
C87 C88 C91 118(3) . .
C89 C88 C91 122(3) . .
C88 C89 C90 120.0 . .
C89 C90 C85 120.0 . .
C125 C124 C123 116(3) . .
C3 C2 C1 121(2) . .
C16 C17 C18 121(2) . .
C113 C118 C117 120(3) . .
C34 C29 S5 119(2) . .
C30 C29 S5 123(2) . .
C30 C29 C34 118(3) . .
C107 C108 C109 120(3) . .
C57 C62 C61 119(3) . .
C13 C12 C11 121(3) . .
C52 C51 C50 122(3) . .
C71 C72 C73 120(4) . .
C33 C32 C35 119(3) . .
C31 C32 C33 123(3) . .
C31 C32 C35 118(3) . .
C12 C13 C8 121(3) . .
C10 C11 C14 118(3) . .
C12 C11 C10 121(3) . .
C12 C11 C14 121(3) . .
F19 C49 F20 107(3) . .
F19 C49 F21 110(3) . .
F19 C49 C46 112(3) . .
F20 C49 C46 111(3) . .
F21 C49 F20 106(3) . .
F21 C49 C46 110(2) . .
C61 C60 C59 112(3) . .
C61 C60 C63 127(3) . .
C63 C60 C59 121(3) . .
C29 C34 C33 122(3) . .
C74 C75 C76 121(3) . .
C17 C18 C19 119(2) . .
C17 C18 C21 123(3) . .
C19 C18 C21 118(3) . .
C18 C19 C20 120(2) . .
C40 C41 C36 118(3) . .
C110 C109 C108 121(3) . .
C110 C109 C112 121(3) . .
C108 C109 C112 118(3) . .
C50 C55 C54 120(3) . .
C62 C61 C60 126(3) . .
C51 C52 C53 118(3) . .
F52 C126 C123 108(3) . .
F53 C126 F52 103(3) . .
F53 C126 C123 113(3) . .
F54 C126 F52 105(3) . .
F54 C126 F53 112(4) . .
F54 C126 C123 115(3) . .
C52 C53 C56 118(4) . .
C54 C53 C52 120(3) . .
C54 C53 C56 122(4) . .
C74 C73 C72 120(4) . .
F46 C112 C109 109(3) . .
F47 C112 F46 104(3) . .
F47 C112 C109 109(3) . .
F48 C112 F46 108(3) . .
F48 C112 F47 112(3) . .
F48 C112 C109 116(3) . .
C53 C54 C55 120(3) . .
C39 C40 C41 120(3) . .
C75 C74 C73 119(3) . .
C75 C74 C77 123(5) . .
C73 C74 C77 118(5) . .
C29 C30 C31 124(3) . .
C32 C33 C34 116(3) . .
F7 C21 F8 103(3) . .
F7 C21 C18 116(3) . .
F8 C21 C18 110(3) . .
F9 C21 F7 104(3) . .
F9 C21 F8 110(4) . .
F9 C21 C18 112(3) . .
F1 C7 F2 106(2) . .
F1 C7 C4 112(2) . .
F3 C7 F1 108(2) . .
F3 C7 F2 107(3) . .
F3 C7 C4 114(2) . .
F2 C7 C4 110(2) . .
F10 C28 C25 110(3) . .
F12 C28 F10 103(2) . .
F12 C28 F11 109(3) . .
F12 C28 C25 116(2) . .
F11 C28 F10 105(2) . .
F11 C28 C25 112(3) . .
C148 C147 N2 117(2) . .
F30 C70 F28 108(3) . .
F30 C70 C67 108(4) . .
F29 C70 F30 110(3) . .
F29 C70 F28 112(4) . .
F29 C70 C67 113(3) . .
F28 C70 C67 106(3) . .
C147 C148 C149 112(2) . .
C32 C31 C30 117(3) . .
C40 C39 C38 122(3) . .
C40 C39 C42 115(3) . .
C38 C39 C42 124(3) . .
C36 C37 C38 122(4) . .
C37 C38 C39 118(3) . .
F16 C42 C39 107(4) . .
F17 C42 F16 105(3) . .
F17 C42 F18 114(5) . .
F17 C42 C39 112(4) . .
F18 C42 F16 105(4) . .
F18 C42 C39 113(3) . .
F6 C14 C11 112(3) . .
F4 C14 F6 104(4) . .
F4 C14 C11 111(3) . .
F5 C14 F6 100(4) . .
F5 C14 C11 112(4) . .
F5 C14 F4 117(4) . .
C142 C141 C140 116(2) . .
C155 C157 C158 114(2) . .
C92 C93 C94 120.0 . .
C93 C92 S14 117.2(16) . .
C97 C92 S14 122.8(16) . .
C97 C92 C93 120.0 . .
C96 C97 C92 120.0 . .
C97 C96 C95 120.0 . .
C96 C95 C98 122(2) . .
C94 C95 C96 120.0 . .
C94 C95 C98 117(2) . .
C95 C94 C93 120.0 . .
F14 C35 C32 115(4) . .
F14 C35 F13 99(3) . .
F15 C35 F14 108(3) . .
F15 C35 C32 119(3) . .
F15 C35 F13 99(4) . .
F13 C35 C32 114(3) . .
C157 C158 C159 112(2) . .
C141 C140 C139 115(2) . .
F44 C105 C102 94(3) . .
F43 C105 C102 98(3) . .
F43 C105 F44 116.7(16) . .
F45 C105 C102 95(3) . .
F45 C105 F44 120.0(17) . .
F45 C105 F43 120.5(17) . .
C131 C132 C133 116(2) . .
C74 C77 F32A 113(6) . .
F33 C77 C74 117(5) . .
F33 C77 F31 106(6) . .
F33 C77 F32 109(6) . .
F33 C77 F33A 38(6) . .
F33 C77 F32A 65(5) . .
F33 C77 F31A 119(5) . .
F31 C77 C74 110(5) . .
F31 C77 F32A 135(4) . .
F32 C77 C74 116(5) . .
F32 C77 F31 96(5) . .
F32 C77 F33A 126(5) . .
F32 C77 F32A 53(4) . .
F33A C77 C74 118(6) . .
F33A C77 F31 71(6) . .
F33A C77 F32A 99(7) . .
F31A C77 C74 122(5) . .
F31A C77 F31 42(6) . .
F31A C77 F32 55(5) . .
F31A C77 F33A 99(7) . .
F31A C77 F32A 102(7) . .
C151 C152 C153 112(2) . .
C157 C155 N2 113.0(19) . .
C150 C149 C148 118(2) . .
C144 C143 N2 115(2) . .
C127 C128 C129 113(2) . .
C138 C137 C136 113(2) . .
C136 C135 N1 110.6(15) . .
C134 C133 C132 116(2) . .
C135 C136 C137 113(2) . .
C154 C153 C152 115(2) . .
C152 C151 N2 117(2) . .
C132 C131 N1 115.8(19) . .
C128 C127 N1 111.8(17) . .
C143 C144 C145 111(2) . .
C82 C83 C78 120.0 . .
C83 C82 C81 120.0 . .
C82 C81 C80 120.0 . .
C82 C81 C84 114(4) . .
C80 C81 C84 122(4) . .
C79 C80 C81 120.0 . .
C80 C79 C78 120.0 . .
C83 C78 S12 121(3) . .
C79 C78 S12 119(3) . .
C79 C78 C83 120.0 . .
F27 C63 C60 111(4) . .
F27 C63 F26 105(4) . .
F25 C63 C60 111(5) . .
F25 C63 F27 109(3) . .
F25 C63 F26 107(4) . .
F26 C63 C60 113(3) . .
F39 C91 C88 90(3) . .
F39 C91 F38 118(2) . .
F39 C91 F37 124(2) . .
F38 C91 C88 93(3) . .
F38 C91 F37 115.8(19) . .
F37 C91 C88 101(3) . .
C146 C145 C144 111(2) . .
C130 C129 C128 113(2) . .
C131 N1 C135 105.8(10) . .
C131 N1 C127 133.8(13) . .
C131 N1 C139 113.1(13) . .
C127 N1 C135 105.3(11) . .
C127 N1 C139 105.7(9) . .
C139 N1 C135 79.4(8) . .
C140 C139 N1 108.6(15) . .
F40 C98 C95 102(3) . .
F41 C98 C95 93(3) . .
F41 C98 F40 118(2) . .
F42 C98 C95 99(3) . .
F42 C98 F40 117(2) . .
F42 C98 F41 119(2) . .
F36 C84 C81 117(8) . .
F36 C84 F34 117(5) . .
F36 C84 F35 104(5) . .
F34 C84 C81 119(5) . .
F34 C84 F35 99(5) . .
F35 C84 C81 92(4) . .
F24 C56 C53 110(5) . .
F24 C56 F22A 69(5) . .
F24 C56 F24A 30(4) . .
F23 C56 C53 112(5) . .
F23 C56 F24 109(6) . .
F23 C56 F22A 144(6) . .
F23 C56 F24A 85(5) . .
F22 C56 C53 111(5) . .
F22 C56 F24 110(6) . .
F22 C56 F23 104(6) . .
F22 C56 F22A 50(4) . .
F22 C56 F24A 134(6) . .
F23A C56 C53 111(5) . .
F23A C56 F24 139(7) . .
F23A C56 F23 52(5) . .
F23A C56 F22 56(5) . .
F23A C56 F22A 105(6) . .
F23A C56 F24A 130(7) . .
F22A C56 C53 101(4) . .
F24A C56 C53 106(5) . .
F24A C56 F22A 98(6) . .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Au1 Au2 2.7613(11) .
Au1 Au3 2.7934(11) .
Au1 Au4 2.7966(11) .
Au1 Au5 2.7705(11) .
Au1 Au6 2.7943(12) 2_656
Au1 Cu5 2.672(3) .
Au1 Cu9 2.739(3) .
Au1 Cu11 2.671(3) .
Au1 Cu12 2.723(3) .
Au1 Cu15 2.699(3) .
Au2 Au2 2.8268(15) 2_656
Au2 Au3 2.7618(11) 2_656
Au2 Au3 2.8021(11) .
Au2 Au6 2.8050(11) 2_656
Au2 Cu6 2.716(3) 2_656
Au2 Cu7 2.724(3) 2_656
Au2 Cu7 2.657(3) .
Au2 Cu9 2.714(3) .
Au2 Cu11 2.704(3) .
Au3 Au2 2.7618(11) 2_656
Au3 Au5 2.8071(12) .
Au3 Au6 2.7765(11) .
Au3 Cu6 2.719(3) .
Au3 Cu7 2.703(3) .
Au3 Cu9 2.706(3) .
Au3 Cu15 2.632(3) .
Au3 Cu16 2.791(3) .
Au4 Au4 2.8336(15) 2_656
Au4 Au5 2.7619(12) .
Au4 Au5 2.7996(11) 2_656
Au4 Au6 2.7677(12) 2_656
Au4 Cu5 2.730(3) .
Au4 Cu8 2.650(3) 2_656
Au4 Cu8 2.717(3) .
Au4 Cu10 2.701(3) 2_656
Au4 Cu12 2.712(3) .
Au5 Au4 2.7996(11) 2_656
Au5 Au6 2.7894(11) .
Au5 Cu5 2.702(3) .
Au5 Cu8 2.716(3) .
Au5 Cu10 2.698(3) .
Au5 Cu15 2.768(3) .
Au5 Cu16 2.638(3) .
Au6 Au1 2.7943(12) 2_656
Au6 Au2 2.8050(12) 2_656
Au6 Au4 2.7677(12) 2_656
Au6 Cu6 2.675(3) .
Au6 Cu10 2.765(3) .
Au6 Cu11 2.704(3) 2_656
Au6 Cu12 2.705(3) 2_656
Au6 Cu16 2.711(3) .
Au7 Cu1 3.046(3) .
Au7 Cu1 3.046(3) 2_656
Au7 S1 2.286(6) .
Au7 S1 2.286(6) 2_656
Au8 Cu2 3.016(3) .
Au8 Cu2 3.016(3) 2_656
Au8 S17 2.298(6) .
Au8 S17 2.298(6) 2_656
Au9 Cu3 2.875(3) .
Au9 Cu4 3.154(4) .
Au9 S5 2.300(7) .
Au9 S6 2.290(7) .
Au10 Cu13 2.989(4) .
Au10 Cu14 2.857(5) .
Au10 S14 2.262(11) .
Au10 S12 2.265(12) .
Cu1 Cu7 3.031(4) 2_656
Cu1 S2 2.245(6) .
Cu1 S3 2.219(6) .
Cu1 S1 2.267(7) .
Cu2 Cu8 2.997(4) .
Cu2 S18 2.242(6) .
Cu2 S16 2.236(7) 2_656
Cu2 S17 2.267(7) .
Cu3 S4 2.242(6) .
Cu3 S9 2.265(6) .
Cu3 S5 2.287(6) .
Cu4 Cu11 3.046(4) .
Cu4 Cu12 3.055(4) .
Cu4 S10 2.216(6) .
Cu4 S7 2.268(7) .
Cu4 S6 2.262(6) .
Cu5 Cu12 3.034(4) .
Cu5 S10 2.372(6) .
Cu5 S18 2.323(6) .
Cu5 S11 2.363(6) .
Cu6 Au2 2.716(3) 2_656
Cu6 Cu11 3.018(4) 2_656
Cu6 S4 2.365(6) 2_656
Cu6 S2 2.332(6) 2_656
Cu6 S13 2.352(7) .
Cu7 Au2 2.724(3) 2_656
Cu7 Cu1 3.031(4) 2_656
Cu7 Cu7 2.971(6) 2_656
Cu7 Cu9 2.954(4) .
Cu7 S2 2.258(6) 2_656
Cu7 S3 2.283(6) .
Cu8 Au4 2.650(3) 2_656
Cu8 Cu8 2.931(6) 2_656
Cu8 Cu10 2.921(4) .
Cu8 S18 2.277(6) .
Cu8 S16 2.279(6) .
Cu9 Cu15 2.940(4) .
Cu9 S7 2.385(6) .
Cu9 S3 2.453(6) .
Cu9 S8 2.410(6) .
Cu10 Au4 2.701(3) 2_656
Cu10 Cu16 2.961(4) .
Cu10 S9 2.386(6) 2_656
Cu10 S16 2.463(6) .
Cu10 S15 2.379(7) .
Cu11 Au6 2.704(3) 2_656
Cu11 Cu6 3.018(4) 2_656
Cu11 Cu12 2.989(4) .
Cu11 S4 2.265(7) .
Cu11 S7 2.282(6) .
Cu12 Au6 2.705(3) 2_656
Cu12 S9 2.276(6) .
Cu12 S10 2.261(6) .
Cu13 Cu15 3.010(5) .
Cu13 Cu16 3.050(5) .
Cu13 S8 2.246(7) .
Cu13 S13 2.264(7) .
Cu13 S12 2.276(9) .
Cu14 S11 2.223(7) .
Cu14 S15 2.257(7) .
Cu14 S14 2.284(10) .
Cu15 Cu16 3.022(4) .
Cu15 S11 2.270(6) .
Cu15 S8 2.300(7) .
Cu16 S15 2.273(8) .
Cu16 S13 2.246(8) .
S4 Cu6 2.365(6) 2_656
S4 C22 1.75(2) .
S9 Cu10 2.386(6) 2_656
S9 C57 1.78(2) .
S10 C64 1.83(2) .
S7 C43 1.77(2) .
S2 Cu6 2.332(6) 2_656
S2 Cu7 2.258(6) 2_656
S2 C8 1.76(2) .
S18 C120 1.77(2) .
S3 C15 1.81(2) .
S16 Cu2 2.236(7) 2_656
S16 C106 1.81(2) .
S11 C71 1.81(2) .
S15 C99 1.77(2) .
S8 C50 1.80(2) .
S13 C85 1.79(3) .
S17 C113 1.78(3) .
S1 C1 1.80(2) .
S5 C29 1.79(3) .
S6 C36 1.83(3) .
S14 C92 1.79(2) .
S12 C78 1.76(3) .
F50 C119 1.32(3) .
F49 C119 1.38(3) .
F1 C7 1.34(3) .
F19 C49 1.31(3) .
F10 C28 1.38(4) .
F20 C49 1.33(4) .
F21 C49 1.31(4) .
F51 C119 1.32(3) .
F3 C7 1.31(4) .
C43 C44 1.36(3) .
C43 C48 1.42(3) .
F12 C28 1.27(3) .
F7 C21 1.29(4) .
F30 C70 1.33(5) .
C6 C5 1.43(3) .
C6 C1 1.38(3) .
F52 C126 1.36(4) .
C22 C23 1.36(4) .
C22 C27 1.42(3) .
F11 C28 1.33(3) .
C64 C65 1.34(4) .
C64 C69 1.37(3) .
F53 C126 1.35(4) .
F29 C70 1.31(5) .
C57 C58 1.36(3) .
C57 C62 1.36(4) .
F46 C112 1.36(4) .
C106 C111 1.36(3) .
C106 C107 1.39(3) .
F47 C112 1.33(4) .
C44 C45 1.38(3) .
F2 C7 1.35(3) .
C116 C119 1.49(4) .
C116 C117 1.40(4) .
C116 C115 1.35(3) .
C71 C76 1.39(4) .
C71 C72 1.32(4) .
C9 C8 1.42(4) .
C9 C10 1.36(4) .
F48 C112 1.24(4) .
C111 C110 1.39(4) .
C8 C13 1.45(3) .
F8 C21 1.39(4) .
C23 C24 1.42(4) .
C3 C4 1.39(4) .
C3 C2 1.33(4) .
C45 C46 1.43(3) .
C5 C4 1.33(4) .
C20 C15 1.37(3) .
C20 C19 1.40(4) .
C36 C41 1.40(4) .
C36 C37 1.32(4) .
C76 C75 1.37(4) .
C102 C101 1.3900 .
C102 C103 1.3900 .
C102 C105 1.85(6) .
C101 C100 1.3900 .
C100 C99 1.3900 .
C99 C104 1.3900 .
C104 C103 1.3900 .
C113 C114 1.41(4) .
C113 C118 1.40(4) .
C114 C115 1.36(3) .
C121 C120 1.39(3) .
C121 C122 1.38(4) .
C50 C51 1.38(4) .
C50 C55 1.37(4) .
C47 C48 1.42(3) .
C47 C46 1.40(4) .
C4 C7 1.49(3) .
C10 C11 1.38(4) .
C27 C26 1.36(4) .
C110 C109 1.38(4) .
C16 C15 1.41(3) .
C16 C17 1.32(3) .
C1 C2 1.36(3) .
C58 C59 1.35(3) .
C123 C122 1.42(4) .
C123 C124 1.43(4) .
C123 C126 1.52(4) .
C107 C108 1.37(4) .
C120 C125 1.44(3) .
N2 C147 1.492(19) .
N2 C155 1.511(19) .
N2 C143 1.49(2) .
N2 C151 1.49(2) .
C117 C118 1.44(4) .
F54 C126 1.24(4) .
C65 C66 1.43(4) .
C68 C67 1.41(4) .
C68 C69 1.33(3) .
C59 C60 1.46(4) .
C26 C25 1.41(4) .
F6 C14 1.33(5) .
C125 C124 1.42(4) .
C25 C24 1.37(4) .
C25 C28 1.47(4) .
F28 C70 1.34(4) .
C67 C66 1.32(4) .
C67 C70 1.60(4) .
C46 C49 1.52(4) .
C85 C86 1.3900 .
C85 C90 1.3900 .
C86 C87 1.3900 .
C87 C88 1.3900 .
C88 C89 1.3900 .
C88 C91 1.90(6) .
C89 C90 1.3900 .
C17 C18 1.39(4) .
F16 C42 1.41(5) .
C29 C34 1.37(4) .
C29 C30 1.35(4) .
C108 C109 1.40(4) .
F17 C42 1.25(5) .
F14 C35 1.34(4) .
C62 C61 1.36(4) .
C12 C13 1.32(4) .
C12 C11 1.35(4) .
C51 C52 1.37(4) .
F9 C21 1.27(4) .
C72 C73 1.39(4) .
C32 C33 1.39(4) .
C32 C31 1.36(4) .
C32 C35 1.45(5) .
F18 C42 1.33(5) .
C11 C14 1.56(4) .
F15 C35 1.26(4) .
C60 C61 1.36(4) .
C60 C63 1.46(5) .
C34 C33 1.42(4) .
C75 C74 1.33(6) .
C18 C19 1.40(4) .
C18 C21 1.49(4) .
C41 C40 1.38(4) .
C109 C112 1.54(5) .
C55 C54 1.41(4) .
F13 C35 1.36(5) .
C52 C53 1.43(5) .
C53 C54 1.35(5) .
C53 C56 1.60(6) .
C73 C74 1.38(6) .
C40 C39 1.37(4) .
C74 C77 1.43(5) .
F33 C77 1.24(7) .
C30 C31 1.40(4) .
F4 C14 1.23(4) .
F24 C56 1.34(9) .
F44 C105 1.37(2) .
F43 C105 1.36(2) .
F45 C105 1.35(2) .
C147 C148 1.49(2) .
C148 C149 1.50(2) .
F5 C14 1.22(5) .
C39 C38 1.37(5) .
C39 C42 1.58(5) .
C37 C38 1.36(5) .
F31 C77 1.42(9) .
F23 C56 1.29(7) .
C150 C149 1.45(2) .
F22 C56 1.24(7) .
C141 C140 1.487(16) .
C141 C142 1.47(2) .
C157 C158 1.49(2) .
C157 C155 1.49(2) .
C93 C92 1.3900 .
C93 C94 1.3900 .
C92 C97 1.3900 .
C97 C96 1.3900 .
C96 C95 1.3900 .
C95 C94 1.3900 .
C95 C98 1.75(5) .
C158 C159 1.50(2) .
C140 C139 1.491(16) .
C132 C133 1.49(2) .
C132 C131 1.45(2) .
C77 F32 1.30(7) .
C77 F33A 1.30(11) .
C77 F32A 1.65(11) .
C77 F31A 1.24(10) .
C152 C153 1.50(2) .
C152 C151 1.47(2) .
F40 C98 1.37(2) .
C143 C144 1.49(2) .
C128 C127 1.47(2) .
C128 C129 1.51(2) .
C137 C136 1.51(2) .
C137 C138 1.51(2) .
C135 C136 1.490(16) .
C135 N1 1.613(10) .
C133 C134 1.49(2) .
C130 C129 1.49(2) .
F41 C98 1.37(2) .
C153 C154 1.47(2) .
C131 N1 1.548(10) .
C127 N1 1.561(10) .
C144 C145 1.52(2) .
C83 C82 1.3900 .
C83 C78 1.3900 .
C82 C81 1.3900 .
C81 C80 1.3900 .
C81 C84 1.52(2) .
C80 C79 1.3900 .
C79 C78 1.3900 .
F27 C63 1.35(5) .
F25 C63 1.35(7) .
F26 C63 1.37(6) .
C91 F39 1.336(16) .
C91 F38 1.37(2) .
C91 F37 1.39(2) .
C145 C146 1.50(2) .
N1 C139 1.603(10) .
C98 F42 1.36(2) .
C84 F36 1.20(8) .
C84 F34 1.32(7) .
C84 F35 1.51(8) .
C56 F23A 1.17(8) .
C56 F22A 1.44(8) .
C56 F24A 1.35(9) .
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
Au1 Au2 Au3 Au2 138.55(3) . 2_656
Au1 Au2 Au3 Au5 36.49(3) . .
Au1 Au2 Au3 Au6 99.84(4) . .
Au1 Au2 Au3 Cu6 163.00(8) . .
Au1 Au2 Au3 Cu7 -150.75(8) . .
Au1 Au2 Au3 Cu9 -70.96(7) . .
Au1 Au2 Au3 Cu15 -28.56(8) . .
Au1 Au2 Au3 Cu16 56.8(2) . .
Au1 Au2 Cu7 Au2 97.07(5) . 2_656
Au1 Au2 Cu7 Au3 27.55(7) . .
Au1 Au2 Cu7 Cu1 151.49(11) . 2_656
Au1 Au2 Cu7 Cu7 161.37(7) . 2_656
Au1 Au2 Cu7 Cu9 -38.77(8) . .
Au1 Au2 Cu7 S2 93.7(3) . 2_656
Au1 Au2 Cu7 S3 -90.84(16) . .
Au1 Au2 Cu9 Au3 71.37(5) . .
Au1 Au2 Cu9 Cu7 138.47(9) . .
Au1 Au2 Cu9 Cu15 35.85(8) . .
Au1 Au2 Cu9 S7 -68.63(16) . .
Au1 Au2 Cu9 S3 -173.50(15) . .
Au1 Au2 Cu9 S8 79.4(3) . .
Au1 Au2 Cu11 Au6 -72.02(5) . 2_656
Au1 Au2 Cu11 Cu4 29.10(15) . .
Au1 Au2 Cu11 Cu6 -137.06(9) . 2_656
Au1 Au2 Cu11 Cu12 -36.19(8) . .
Au1 Au2 Cu11 S4 -144.9(2) . .
Au1 Au2 Cu11 S7 70.84(18) . .
Au1 Au3 Au5 Au4 37.72(3) . .
Au1 Au3 Au5 Au4 102.50(4) . 2_656
Au1 Au3 Au5 Au6 139.06(4) . .
Au1 Au3 Au5 Cu5 -26.72(8) . .
Au1 Au3 Au5 Cu8 80.3(2) . .
Au1 Au3 Au5 Cu10 165.48(8) . .
Au1 Au3 Au5 Cu15 -69.84(8) . .
Au1 Au3 Au5 Cu16 -151.05(8) . .
Au1 Au3 Au6 Au1 64.99(4) . 2_656
Au1 Au3 Au6 Au2 101.50(4) . 2_656
Au1 Au3 Au6 Au4 1.21(5) . 2_656
Au1 Au3 Au6 Au5 -36.29(3) . .
Au1 Au3 Au6 Cu6 171.62(8) . .
Au1 Au3 Au6 Cu10 -61.79(8) . .
Au1 Au3 Au6 Cu11 126.85(8) . 2_656
Au1 Au3 Au6 Cu12 40.5(3) . 2_656
Au1 Au3 Au6 Cu16 -102.88(8) . .
Au1 Au3 Cu6 Au2 42.0(3) . 2_656
Au1 Au3 Cu6 Au6 -30.6(3) . .
Au1 Au3 Cu6 Cu11 6.5(3) . 2_656
Au1 Au3 Cu6 S4 -29.9(5) . 2_656
Au1 Au3 Cu6 S2 116.6(3) . 2_656
Au1 Au3 Cu6 S13 -135.8(3) . .
Au1 Au3 Cu7 Au2 -99.60(5) . 2_656
Au1 Au3 Cu7 Au2 -26.70(6) . .
Au1 Au3 Cu7 Cu1 -134.21(14) . 2_656
Au1 Au3 Cu7 Cu7 -66.05(14) . 2_656
Au1 Au3 Cu7 Cu9 40.55(9) . .
Au1 Au3 Cu7 S2 -174.13(15) . 2_656
Au1 Au3 Cu7 S3 42.25(19) . .
Au1 Au3 Cu9 Au2 -69.99(5) . .
Au1 Au3 Cu9 Cu7 -135.36(9) . .
Au1 Au3 Cu9 Cu15 67.19(8) . .
Au1 Au3 Cu9 S7 3.6(3) . .
Au1 Au3 Cu9 S3 -136.90(18) . .
Au1 Au3 Cu9 S8 115.11(17) . .
Au1 Au3 Cu15 Au5 69.38(5) . .
Au1 Au3 Cu15 Cu9 -67.38(8) . .
Au1 Au3 Cu15 Cu13 -166.01(12) . .
Au1 Au3 Cu15 Cu16 132.02(10) . .
Au1 Au3 Cu15 S11 74.2(3) . .
Au1 Au3 Cu15 S8 -117.75(18) . .
Au1 Au3 Cu16 Au5 26.29(7) . .
Au1 Au3 Cu16 Au6 99.13(6) . .
Au1 Au3 Cu16 Cu10 62.97(11) . .
Au1 Au3 Cu16 Cu13 -104.76(10) . .
Au1 Au3 Cu16 Cu15 -42.98(9) . .
Au1 Au3 Cu16 S15 14.9(4) . .
Au1 Au3 Cu16 S13 -153.33(18) . .
Au1 Au4 Au5 Au3 -37.44(3) . .
Au1 Au4 Au5 Au4 -137.35(3) . 2_656
Au1 Au4 Au5 Au6 -100.67(4) . .
Au1 Au4 Au5 Cu5 68.34(8) . .
Au1 Au4 Au5 Cu8 155.58(8) . .
Au1 Au4 Au5 Cu10 -165.85(8) . .
Au1 Au4 Au5 Cu15 23.32(8) . .
Au1 Au4 Au5 Cu16 -75.5(3) . .
Au1 Au4 Cu5 Au5 -71.65(5) . .
Au1 Au4 Cu5 Cu12 66.68(8) . .
Au1 Au4 Cu5 S10 73.18(16) . .
Au1 Au4 Cu5 S18 -175.99(17) . .
Au1 Au4 Cu5 S11 -71.2(3) . .
Au1 Au4 Cu8 Au4 -95.25(6) . 2_656
Au1 Au4 Cu8 Au5 -23.20(7) . .
Au1 Au4 Cu8 Cu2 130.09(8) . .
Au1 Au4 Cu8 Cu8 -162.97(8) . 2_656
Au1 Au4 Cu8 Cu10 -56.98(12) . .
Au1 Au4 Cu8 S18 81.37(16) . .
Au1 Au4 Cu8 S16 -110.2(3) . .
Au1 Au4 Cu12 Au6 71.57(5) . 2_656
Au1 Au4 Cu12 Cu4 -28.27(15) . .
Au1 Au4 Cu12 Cu5 -64.75(8) . .
Au1 Au4 Cu12 Cu11 35.32(8) . .
Au1 Au4 Cu12 S9 142.57(19) . .
Au1 Au4 Cu12 S10 -71.69(17) . .
Au1 Au5 Au6 Au1 -62.99(4) . 2_656
Au1 Au5 Au6 Au2 -0.63(5) . 2_656
Au1 Au5 Au6 Au3 36.71(3) . .
Au1 Au5 Au6 Au4 -101.92(4) . 2_656
Au1 Au5 Au6 Cu6 63.15(8) . .
Au1 Au5 Au6 Cu10 -171.05(8) . .
Au1 Au5 Au6 Cu11 -33.6(3) . 2_656
Au1 Au5 Au6 Cu12 -126.79(8) . 2_656
Au1 Au5 Au6 Cu16 109.45(9) . .
Au1 Au5 Cu5 Au4 72.09(6) . .
Au1 Au5 Cu5 Cu12 37.25(8) . .
Au1 Au5 Cu5 S10 0.6(3) . .
Au1 Au5 Cu5 S18 146.32(19) . .
Au1 Au5 Cu5 S11 -107.60(16) . .
Au1 Au5 Cu8 Au4 23.62(7) . .
Au1 Au5 Cu8 Au4 97.02(6) . 2_656
Au1 Au5 Cu8 Cu2 -12.46(19) . .
Au1 Au5 Cu8 Cu8 57.45(15) . 2_656
Au1 Au5 Cu8 Cu10 164.54(8) . .
Au1 Au5 Cu8 S18 -51.42(18) . .
Au1 Au5 Cu8 S16 166.29(17) . .
Au1 Au5 Cu10 Au4 -32.4(3) . 2_656
Au1 Au5 Cu10 Au6 37.6(3) . .
Au1 Au5 Cu10 Cu8 -97.9(3) . .
Au1 Au5 Cu10 Cu16 104.7(3) . .
Au1 Au5 Cu10 S9 40.7(5) . 2_656
Au1 Au5 Cu10 S16 -99.5(3) . .
Au1 Au5 Cu10 S15 151.9(3) . .
Au1 Au5 Cu15 Au3 -72.97(6) . .
Au1 Au5 Cu15 Cu9 -35.54(8) . .
Au1 Au5 Cu15 Cu13 -135.67(15) . .
Au1 Au5 Cu15 Cu16 -142.66(10) . .
Au1 Au5 Cu15 S11 109.93(17) . .
Au1 Au5 Cu15 S8 -85.3(3) . .
Au1 Au5 Cu16 Au3 -27.70(7) . .
Au1 Au5 Cu16 Au6 -97.00(6) . .
Au1 Au5 Cu16 Cu10 -164.96(8) . .
Au1 Au5 Cu16 Cu13 27.80(16) . .
Au1 Au5 Cu16 Cu15 34.87(9) . .
Au1 Au5 Cu16 S15 145.52(16) . .
Au1 Au5 Cu16 S13 -27.1(4) . .
Au1 Au6 Cu6 Au2 26.98(7) 2_656 2_656
Au1 Au6 Cu6 Au3 97.00(6) 2_656 .
Au1 Au6 Cu6 Cu11 -38.66(9) 2_656 2_656
Au1 Au6 Cu6 S4 -82.59(17) 2_656 2_656
Au1 Au6 Cu6 S2 35.0(3) 2_656 2_656
Au1 Au6 Cu6 S13 171.13(17) 2_656 .
Au1 Au6 Cu10 Au4 -23.89(7) 2_656 2_656
Au1 Au6 Cu10 Au5 -96.52(6) 2_656 .
Au1 Au6 Cu10 Cu8 -58.56(11) 2_656 .
Au1 Au6 Cu10 Cu16 -161.97(8) 2_656 .
Au1 Au6 Cu10 S9 85.58(16) 2_656 2_656
Au1 Au6 Cu10 S16 -13.7(3) 2_656 .
Au1 Au6 Cu10 S15 -164.57(18) 2_656 .
Au1 Au6 Cu16 Au3 -45.4(3) 2_656 .
Au1 Au6 Cu16 Au5 26.3(3) 2_656 .
Au1 Au6 Cu16 Cu10 93.0(3) 2_656 .
Au1 Au6 Cu16 Cu13 -77.1(3) 2_656 .
Au1 Au6 Cu16 Cu15 -14.6(4) 2_656 .
Au1 Au6 Cu16 S15 95.8(3) 2_656 .
Au1 Au6 Cu16 S13 -118.3(3) 2_656 .
Au1 Cu5 Cu12 Au4 77.04(7) . .
Au1 Cu5 Cu12 Au6 38.06(8) . 2_656
Au1 Cu5 Cu12 Cu4 -78.43(9) . .
Au1 Cu5 Cu12 Cu11 -20.89(9) . .
Au1 Cu5 Cu12 S9 133.2(3) . .
Au1 Cu5 Cu12 S10 -111.6(2) . .
Au1 Cu5 S10 Cu4 -26.2(3) . .
Au1 Cu5 S10 Cu12 51.69(14) . .
Au1 Cu5 S10 C64 163.8(10) . .
Au1 Cu5 S18 Cu2 -39.0(5) . .
Au1 Cu5 S18 Cu8 41.4(4) . .
Au1 Cu5 S18 C120 156.0(8) . .
Au1 Cu5 S11 Cu14 -95.5(3) . .
Au1 Cu5 S11 Cu15 -7.47(17) . .
Au1 Cu5 S11 C71 111.5(9) . .
Au1 Cu9 Cu15 Au3 76.43(7) . .
Au1 Cu9 Cu15 Au5 36.81(8) . .
Au1 Cu9 Cu15 Cu13 153.02(12) . .
Au1 Cu9 Cu15 Cu16 94.50(13) . .
Au1 Cu9 Cu15 S11 -62.6(3) . .
Au1 Cu9 Cu15 S8 -176.6(2) . .
Au1 Cu9 S7 Cu4 24.3(4) . .
Au1 Cu9 S7 Cu11 -51.40(15) . .
Au1 Cu9 S7 C43 -168.1(9) . .
Au1 Cu9 S3 Cu1 13.0(5) . .
Au1 Cu9 S3 Cu7 -63.2(3) . .
Au1 Cu9 S3 C15 -170.8(8) . .
Au1 Cu9 S8 Cu13 70.5(4) . .
Au1 Cu9 S8 Cu15 2.98(19) . .
Au1 Cu9 S8 C50 -101.9(10) . .
Au1 Cu11 Cu12 Au4 -38.22(8) . .
Au1 Cu11 Cu12 Au6 -76.78(7) . 2_656
Au1 Cu11 Cu12 Cu4 96.00(11) . .
Au1 Cu11 Cu12 Cu5 20.75(9) . .
Au1 Cu11 Cu12 S9 -145.30(17) . .
Au1 Cu11 Cu12 S10 72.78(16) . .
Au1 Cu11 S4 Cu3 71.0(4) . .
Au1 Cu11 S4 Cu6 -55.6(4) . 2_656
Au1 Cu11 S4 C22 -170.6(9) . .
Au1 Cu11 S7 Cu4 -84.15(16) . .
Au1 Cu11 S7 Cu9 52.44(14) . .
Au1 Cu11 S7 C43 163.4(8) . .
Au1 Cu12 S9 Cu3 -78.2(3) . .
Au1 Cu12 S9 Cu10 55.1(3) . 2_656
Au1 Cu12 S9 C57 167.0(8) . .
Au1 Cu12 S10 Cu4 80.91(16) . .
Au1 Cu12 S10 Cu5 -50.20(13) . .
Au1 Cu12 S10 C64 -164.3(8) . .
Au1 Cu15 Cu16 Au3 43.61(9) . .
Au1 Cu15 Cu16 Au5 -33.45(9) . .
Au1 Cu15 Cu16 Au6 9.92(15) . .
Au1 Cu15 Cu16 Cu10 -51.47(16) . .
Au1 Cu15 Cu16 Cu13 139.25(15) . .
Au1 Cu15 Cu16 S15 -105.5(2) . .
Au1 Cu15 Cu16 S13 113.6(2) . .
Au1 Cu15 S11 Cu5 7.44(17) . .
Au1 Cu15 S11 Cu14 137.40(18) . .
Au1 Cu15 S11 C71 -102.5(9) . .
Au1 Cu15 S8 Cu9 -3.1(2) . .
Au1 Cu15 S8 Cu13 -140.02(16) . .
Au1 Cu15 S8 C50 108.5(10) . .
Au2 Au1 Au3 Au2 -37.62(3) . 2_656
Au2 Au1 Au3 Au5 -138.58(4) . .
Au2 Au1 Au3 Au6 -102.01(4) . .
Au2 Au1 Au3 Cu6 -75.0(3) . .
Au2 Au1 Au3 Cu7 26.26(7) . .
Au2 Au1 Au3 Cu9 69.78(7) . .
Au2 Au1 Au3 Cu15 149.08(9) . .
Au2 Au1 Au3 Cu16 -163.93(8) . .
Au2 Au1 Au4 Au4 63.77(5) . 2_656
Au2 Au1 Au4 Au5 1.93(5) . 2_656
Au2 Au1 Au4 Au5 101.73(4) . .
Au2 Au1 Au4 Au6 -36.79(3) . 2_656
Au2 Au1 Au4 Cu5 171.91(8) . .
Au2 Au1 Au4 Cu8 124.84(7) . .
Au2 Au1 Au4 Cu8 34.3(3) . 2_656
Au2 Au1 Au4 Cu10 -61.21(8) . 2_656
Au2 Au1 Au4 Cu12 -106.46(8) . .
Au2 Au1 Au5 Au3 37.59(3) . .
Au2 Au1 Au5 Au4 -61.84(4) . 2_656
Au2 Au1 Au5 Au4 -100.80(4) . .
Au2 Au1 Au5 Au6 1.15(5) . .
Au2 Au1 Au5 Cu5 -171.57(8) . .
Au2 Au1 Au5 Cu8 -124.10(8) . .
Au2 Au1 Au5 Cu10 -32.8(3) . .
Au2 Au1 Au5 Cu15 104.22(8) . .
Au2 Au1 Au5 Cu16 65.72(9) . .
Au2 Au1 Cu5 Au4 -34.3(3) . .
Au2 Au1 Cu5 Au5 35.8(3) . .
Au2 Au1 Cu5 Cu12 -99.9(3) . .
Au2 Au1 Cu5 S10 -143.8(3) . .
Au2 Au1 Cu5 S18 -27.9(5) . .
Au2 Au1 Cu5 S11 109.1(3) . .
Au2 Au1 Cu9 Au3 -72.24(5) . .
Au2 Au1 Cu9 Cu7 -34.63(8) . .
Au2 Au1 Cu9 Cu15 -137.52(9) . .
Au2 Au1 Cu9 S7 110.22(17) . .
Au2 Au1 Cu9 S3 9.6(2) . .
Au2 Au1 Cu9 S8 -140.24(19) . .
Au2 Au1 Cu11 Au6 71.77(5) . 2_656
Au2 Au1 Cu11 Cu4 -160.07(11) . .
Au2 Au1 Cu11 Cu6 36.16(8) . 2_656
Au2 Au1 Cu11 Cu12 137.79(9) . .
Au2 Au1 Cu11 S4 77.8(3) . .
Au2 Au1 Cu11 S7 -111.47(17) . .
Au2 Au1 Cu12 Au4 98.40(6) . .
Au2 Au1 Cu12 Au6 27.65(7) . 2_656
Au2 Au1 Cu12 Cu4 -101.30(9) . .
Au2 Au1 Cu12 Cu5 165.31(8) . .
Au2 Au1 Cu12 Cu11 -39.15(9) . .
Au2 Au1 Cu12 S9 24.7(3) . .
Au2 Au1 Cu12 S10 -148.15(14) . .
Au2 Au1 Cu15 Au3 -28.70(7) . .
Au2 Au1 Cu15 Au5 -100.70(6) . .
Au2 Au1 Cu15 Cu9 38.46(8) . .
Au2 Au1 Cu15 Cu13 -6.8(2) . .
Au2 Au1 Cu15 Cu16 -70.01(12) . .
Au2 Au1 Cu15 S11 -172.57(15) . .
Au2 Au1 Cu15 S8 41.4(2) . .
Au2 Au2 Au3 Au1 -138.55(3) 2_656 .
Au2 Au2 Au3 Au5 -102.06(3) 2_656 .
Au2 Au2 Au3 Au6 -38.72(3) 2_656 .
Au2 Au2 Au3 Cu6 24.45(7) 2_656 .
Au2 Au2 Au3 Cu7 70.69(7) 2_656 .
Au2 Au2 Au3 Cu9 150.49(7) 2_656 .
Au2 Au2 Au3 Cu15 -167.11(8) 2_656 .
Au2 Au2 Au3 Cu16 -81.7(2) 2_656 .
Au2 Au2 Cu7 Au3 -69.51(5) 2_656 .
Au2 Au2 Cu7 Cu1 54.42(11) 2_656 2_656
Au2 Au2 Cu7 Cu7 64.30(9) 2_656 2_656
Au2 Au2 Cu7 Cu9 -135.83(9) 2_656 .
Au2 Au2 Cu7 S2 -3.3(3) 2_656 2_656
Au2 Au2 Cu7 S3 172.10(17) 2_656 .
Au2 Au2 Cu9 Au1 -98.29(5) 2_656 .
Au2 Au2 Cu9 Au3 -26.92(6) 2_656 .
Au2 Au2 Cu9 Cu7 40.18(8) 2_656 .
Au2 Au2 Cu9 Cu15 -62.44(11) 2_656 .
Au2 Au2 Cu9 S7 -166.92(16) 2_656 .
Au2 Au2 Cu9 S3 88.21(14) 2_656 .
Au2 Au2 Cu9 S8 -18.9(3) 2_656 .
Au2 Au2 Cu11 Au1 34.6(3) 2_656 .
Au2 Au2 Cu11 Au6 -37.4(3) 2_656 2_656
Au2 Au2 Cu11 Cu4 63.7(4) 2_656 .
Au2 Au2 Cu11 Cu6 -102.4(3) 2_656 2_656
Au2 Au2 Cu11 Cu12 -1.6(4) 2_656 .
Au2 Au2 Cu11 S4 -110.3(3) 2_656 .
Au2 Au2 Cu11 S7 105.5(3) 2_656 .
Au2 Au3 Au5 Au1 -36.42(3) . .
Au2 Au3 Au5 Au1 -100.85(4) 2_656 .
Au2 Au3 Au5 Au4 66.08(4) . 2_656
Au2 Au3 Au5 Au4 1.29(4) . .
Au2 Au3 Au5 Au4 1.64(5) 2_656 2_656
Au2 Au3 Au5 Au4 -63.14(4) 2_656 .
Au2 Au3 Au5 Au6 38.21(3) 2_656 .
Au2 Au3 Au5 Au6 102.64(4) . .
Au2 Au3 Au5 Cu5 -63.14(8) . .
Au2 Au3 Au5 Cu5 -127.58(8) 2_656 .
Au2 Au3 Au5 Cu8 43.9(2) . .
Au2 Au3 Au5 Cu8 -20.5(2) 2_656 .
Au2 Au3 Au5 Cu10 129.06(8) . .
Au2 Au3 Au5 Cu10 64.63(8) 2_656 .
Au2 Au3 Au5 Cu15 -170.70(9) 2_656 .
Au2 Au3 Au5 Cu15 -106.26(8) . .
Au2 Au3 Au5 Cu16 108.10(8) 2_656 .
Au2 Au3 Au5 Cu16 172.53(8) . .
Au2 Au3 Au6 Au1 2.29(5) . 2_656
Au2 Au3 Au6 Au1 -36.51(3) 2_656 2_656
Au2 Au3 Au6 Au2 38.81(3) . 2_656
Au2 Au3 Au6 Au4 -100.29(4) 2_656 2_656
Au2 Au3 Au6 Au4 -61.48(4) . 2_656
Au2 Au3 Au6 Au5 -98.98(4) . .
Au2 Au3 Au6 Au5 -137.79(4) 2_656 .
Au2 Au3 Au6 Cu6 108.93(8) . .
Au2 Au3 Au6 Cu6 70.12(8) 2_656 .
Au2 Au3 Au6 Cu10 -163.29(8) 2_656 .
Au2 Au3 Au6 Cu10 -124.48(7) . .
Au2 Au3 Au6 Cu11 25.35(8) 2_656 2_656
Au2 Au3 Au6 Cu11 64.16(8) . 2_656
Au2 Au3 Au6 Cu12 -61.0(3) 2_656 2_656
Au2 Au3 Au6 Cu12 -22.2(3) . 2_656
Au2 Au3 Au6 Cu16 155.62(8) 2_656 .
Au2 Au3 Au6 Cu16 -165.57(8) . .
Au2 Au3 Cu6 Au2 -24.88(7) . 2_656
Au2 Au3 Cu6 Au6 -97.46(6) . .
Au2 Au3 Cu6 Au6 -72.57(5) 2_656 .
Au2 Au3 Cu6 Cu11 -35.48(8) 2_656 2_656
Au2 Au3 Cu6 Cu11 -60.36(12) . 2_656
Au2 Au3 Cu6 S4 -71.9(3) 2_656 2_656
Au2 Au3 Cu6 S4 -96.8(3) . 2_656
Au2 Au3 Cu6 S2 74.60(15) 2_656 2_656
Au2 Au3 Cu6 S2 49.72(17) . 2_656
Au2 Au3 Cu6 S13 157.3(2) . .
Au2 Au3 Cu6 S13 -177.8(2) 2_656 .
Au2 Au3 Cu7 Au2 72.89(5) 2_656 .
Au2 Au3 Cu7 Au2 -72.89(5) . 2_656
Au2 Au3 Cu7 Cu1 -107.51(16) . 2_656
Au2 Au3 Cu7 Cu1 -34.62(13) 2_656 2_656
Au2 Au3 Cu7 Cu7 -39.35(10) . 2_656
Au2 Au3 Cu7 Cu7 33.54(10) 2_656 2_656
Au2 Au3 Cu7 Cu9 67.25(8) . .
Au2 Au3 Cu7 Cu9 140.14(9) 2_656 .
Au2 Au3 Cu7 S2 -147.43(18) . 2_656
Au2 Au3 Cu7 S2 -74.53(16) 2_656 2_656
Au2 Au3 Cu7 S3 141.8(2) 2_656 .
Au2 Au3 Cu7 S3 68.95(17) . .
Au2 Au3 Cu9 Au1 69.99(5) . .
Au2 Au3 Cu9 Au1 98.10(6) 2_656 .
Au2 Au3 Cu9 Au2 28.12(7) 2_656 .
Au2 Au3 Cu9 Cu7 -37.26(9) 2_656 .
Au2 Au3 Cu9 Cu7 -65.38(8) . .
Au2 Au3 Cu9 Cu15 165.29(9) 2_656 .
Au2 Au3 Cu9 Cu15 137.17(10) . .
Au2 Au3 Cu9 S7 101.7(3) 2_656 .
Au2 Au3 Cu9 S7 73.6(3) . .
Au2 Au3 Cu9 S3 -38.80(17) 2_656 .
Au2 Au3 Cu9 S3 -66.92(15) . .
Au2 Au3 Cu9 S8 -146.79(16) 2_656 .
Au2 Au3 Cu9 S8 -174.91(18) . .
Au2 Au3 Cu15 Au1 28.42(7) . .
Au2 Au3 Cu15 Au1 -28.3(4) 2_656 .
Au2 Au3 Cu15 Au5 97.80(6) . .
Au2 Au3 Cu15 Au5 41.1(3) 2_656 .
Au2 Au3 Cu15 Cu9 -38.96(9) . .
Au2 Au3 Cu15 Cu9 -95.7(3) 2_656 .
Au2 Au3 Cu15 Cu13 -137.60(9) . .
Au2 Au3 Cu15 Cu13 165.7(3) 2_656 .
Au2 Au3 Cu15 Cu16 103.7(3) 2_656 .
Au2 Au3 Cu15 Cu16 160.43(8) . .
Au2 Au3 Cu15 S11 102.6(3) . .
Au2 Au3 Cu15 S11 45.9(5) 2_656 .
Au2 Au3 Cu15 S8 -146.1(3) 2_656 .
Au2 Au3 Cu15 S8 -89.34(17) . .
Au2 Au3 Cu16 Au5 -96.26(6) 2_656 .
Au2 Au3 Cu16 Au5 -23.6(3) . .
Au2 Au3 Cu16 Au6 -23.41(8) 2_656 .
Au2 Au3 Cu16 Au6 49.3(2) . .
Au2 Au3 Cu16 Cu10 -59.57(12) 2_656 .
Au2 Au3 Cu16 Cu10 13.1(3) . .
Au2 Au3 Cu16 Cu13 132.69(9) 2_656 .
Au2 Au3 Cu16 Cu13 -154.6(2) . .
Au2 Au3 Cu16 Cu15 -92.8(2) . .
Au2 Au3 Cu16 Cu15 -165.52(9) 2_656 .
Au2 Au3 Cu16 S15 -107.7(3) 2_656 .
Au2 Au3 Cu16 S15 -35.0(5) . .
Au2 Au3 Cu16 S13 84.12(19) 2_656 .
Au2 Au3 Cu16 S13 156.8(2) . .
Au2 Au6 Cu6 Au3 70.02(5) 2_656 .
Au2 Au6 Cu6 Cu11 -65.64(8) 2_656 2_656
Au2 Au6 Cu6 S4 -109.57(17) 2_656 2_656
Au2 Au6 Cu6 S2 8.0(3) 2_656 2_656
Au2 Au6 Cu6 S13 144.15(19) 2_656 .
Au2 Au6 Cu10 Au4 38.9(3) 2_656 2_656
Au2 Au6 Cu10 Au5 -33.7(3) 2_656 .
Au2 Au6 Cu10 Cu8 4.3(3) 2_656 .
Au2 Au6 Cu10 Cu16 -99.1(2) 2_656 .
Au2 Au6 Cu10 S9 148.4(2) 2_656 2_656
Au2 Au6 Cu10 S16 49.1(4) 2_656 .
Au2 Au6 Cu10 S15 -101.7(3) 2_656 .
Au2 Au6 Cu16 Au3 23.28(7) 2_656 .
Au2 Au6 Cu16 Au5 95.06(7) 2_656 .
Au2 Au6 Cu16 Cu10 161.69(8) 2_656 .
Au2 Au6 Cu16 Cu13 -8.4(2) 2_656 .
Au2 Au6 Cu16 Cu15 54.13(13) 2_656 .
Au2 Au6 Cu16 S15 164.48(19) 2_656 .
Au2 Au6 Cu16 S13 -49.6(2) 2_656 .
Au2 Cu6 S13 Cu13 -34.4(7) 2_656 .
Au2 Cu6 S13 Cu16 47.3(4) 2_656 .
Au2 Cu6 S13 C85 160.2(15) 2_656 .
Au2 Cu7 Cu9 Au1 36.91(8) . .
Au2 Cu7 Cu9 Au1 -3.86(14) 2_656 .
Au2 Cu7 Cu9 Au2 -40.77(8) 2_656 .
Au2 Cu7 Cu9 Au3 36.07(8) 2_656 .
Au2 Cu7 Cu9 Au3 76.84(7) . .
Au2 Cu7 Cu9 Cu15 96.34(12) . .
Au2 Cu7 Cu9 Cu15 55.57(15) 2_656 .
Au2 Cu7 Cu9 S7 -93.6(3) 2_656 .
Au2 Cu7 Cu9 S7 -52.9(3) . .
Au2 Cu7 Cu9 S3 -105.13(19) . .
Au2 Cu7 Cu9 S3 -145.9(2) 2_656 .
Au2 Cu7 Cu9 S8 147.04(19) . .
Au2 Cu7 Cu9 S8 106.26(18) 2_656 .
Au2 Cu7 S3 Cu1 -65.7(4) 2_656 .
Au2 Cu7 S3 Cu1 -77.93(16) . .
Au2 Cu7 S3 Cu9 55.34(12) . .
Au2 Cu7 S3 Cu9 67.6(3) 2_656 .
Au2 Cu7 S3 C15 173.9(7) . .
Au2 Cu7 S3 C15 -173.8(6) 2_656 .
Au2 Cu9 Cu15 Au1 -37.76(8) . .
Au2 Cu9 Cu15 Au3 38.67(8) . .
Au2 Cu9 Cu15 Au5 -0.95(14) . .
Au2 Cu9 Cu15 Cu13 115.26(12) . .
Au2 Cu9 Cu15 Cu16 56.74(15) . .
Au2 Cu9 Cu15 S11 -100.3(3) . .
Au2 Cu9 Cu15 S8 145.7(2) . .
Au2 Cu9 S7 Cu4 80.8(4) . .
Au2 Cu9 S7 Cu11 5.11(19) . .
Au2 Cu9 S7 C43 -111.6(9) . .
Au2 Cu9 S3 Cu1 21.6(3) . .
Au2 Cu9 S3 Cu7 -54.64(13) . .
Au2 Cu9 S3 C15 -162.2(8) . .
Au2 Cu9 S8 Cu13 7.1(6) . .
Au2 Cu9 S8 Cu15 -60.4(3) . .
Au2 Cu9 S8 C50 -165.3(10) . .
Au2 Cu11 Cu12 Au1 38.27(8) . .
Au2 Cu11 Cu12 Au4 0.05(15) . .
Au2 Cu11 Cu12 Au6 -38.51(8) . 2_656
Au2 Cu11 Cu12 Cu4 134.27(14) . .
Au2 Cu11 Cu12 Cu5 59.01(14) . .
Au2 Cu11 Cu12 S9 -107.03(17) . .
Au2 Cu11 Cu12 S10 111.05(17) . .
Au2 Cu11 S4 Cu3 135.03(16) . .
Au2 Cu11 S4 Cu6 8.44(19) . 2_656
Au2 Cu11 S4 C22 -106.6(9) . .
Au2 Cu11 S7 Cu4 -141.78(16) . .
Au2 Cu11 S7 Cu9 -5.2(2) . .
Au2 Cu11 S7 C43 105.8(8) . .
Au3 Au1 Au2 Au2 36.38(4) . 2_656
Au3 Au1 Au2 Au3 99.92(4) . 2_656
Au3 Au1 Au2 Au6 137.07(3) . 2_656
Au3 Au1 Au2 Cu6 163.65(7) . 2_656
Au3 Au1 Au2 Cu7 60.6(2) . 2_656
Au3 Au1 Au2 Cu7 -27.25(7) . .
Au3 Au1 Au2 Cu9 -68.85(7) . .
Au3 Au1 Au2 Cu11 -153.45(8) . .
Au3 Au1 Au4 Au4 -0.45(5) . 2_656
Au3 Au1 Au4 Au5 37.51(3) . .
Au3 Au1 Au4 Au5 -62.29(4) . 2_656
Au3 Au1 Au4 Au6 -101.02(4) . 2_656
Au3 Au1 Au4 Cu5 107.69(8) . .
Au3 Au1 Au4 Cu8 60.61(8) . .
Au3 Au1 Au4 Cu8 -29.9(3) . 2_656
Au3 Au1 Au4 Cu10 -125.43(8) . 2_656
Au3 Au1 Au4 Cu12 -170.68(8) . .
Au3 Au1 Au5 Au4 -99.44(4) . 2_656
Au3 Au1 Au5 Au4 -138.39(4) . .
Au3 Au1 Au5 Au6 -36.44(3) . .
Au3 Au1 Au5 Cu5 150.84(8) . .
Au3 Au1 Au5 Cu8 -161.70(8) . .
Au3 Au1 Au5 Cu10 -70.4(3) . .
Au3 Au1 Au5 Cu15 66.63(8) . .
Au3 Au1 Au5 Cu16 28.13(8) . .
Au3 Au1 Cu5 Au4 -97.84(6) . .
Au3 Au1 Cu5 Au5 -27.68(7) . .
Au3 Au1 Cu5 Cu12 -163.41(8) . .
Au3 Au1 Cu5 S10 152.70(15) . .
Au3 Au1 Cu5 S18 -91.4(3) . .
Au3 Au1 Cu5 S11 45.52(16) . .
Au3 Au1 Cu9 Au2 72.24(5) . .
Au3 Au1 Cu9 Cu7 37.61(8) . .
Au3 Au1 Cu9 Cu15 -65.29(8) . .
Au3 Au1 Cu9 S7 -177.54(18) . .
Au3 Au1 Cu9 S3 81.8(2) . .
Au3 Au1 Cu9 S8 -68.01(17) . .
Au3 Au1 Cu11 Au2 25.47(8) . .
Au3 Au1 Cu11 Au6 97.24(6) . 2_656
Au3 Au1 Cu11 Cu4 -134.60(8) . .
Au3 Au1 Cu11 Cu6 61.63(12) . 2_656
Au3 Au1 Cu11 Cu12 163.26(8) . .
Au3 Au1 Cu11 S4 103.3(3) . .
Au3 Au1 Cu11 S7 -86.00(16) . .
Au3 Au1 Cu12 Au4 35.2(3) . .
Au3 Au1 Cu12 Au6 -35.5(3) . 2_656
Au3 Au1 Cu12 Cu4 -164.5(2) . .
Au3 Au1 Cu12 Cu5 102.1(3) . .
Au3 Au1 Cu12 Cu11 -102.3(3) . .
Au3 Au1 Cu12 S9 -38.5(5) . .
Au3 Au1 Cu12 S10 148.7(3) . .
Au3 Au1 Cu15 Au5 -72.00(5) . .
Au3 Au1 Cu15 Cu9 67.16(8) . .
Au3 Au1 Cu15 Cu13 21.87(18) . .
Au3 Au1 Cu15 Cu16 -41.31(9) . .
Au3 Au1 Cu15 S11 -143.87(19) . .
Au3 Au1 Cu15 S8 70.09(19) . .
Au3 Au2 Au3 Au1 -101.47(4) 2_656 .
Au3 Au2 Au3 Au2 37.08(4) 2_656 2_656
Au3 Au2 Au3 Au5 -64.98(4) 2_656 .
Au3 Au2 Au3 Au6 -1.63(5) 2_656 .
Au3 Au2 Au3 Cu6 61.53(9) 2_656 .
Au3 Au2 Au3 Cu7 107.78(8) 2_656 .
Au3 Au2 Au3 Cu9 -172.43(8) 2_656 .
Au3 Au2 Au3 Cu15 -130.03(8) 2_656 .
Au3 Au2 Au3 Cu16 -44.6(2) 2_656 .
Au3 Au2 Cu7 Au2 -27.16(7) 2_656 2_656
Au3 Au2 Cu7 Au2 69.51(5) . 2_656
Au3 Au2 Cu7 Au3 -96.67(6) 2_656 .
Au3 Au2 Cu7 Cu1 27.27(15) 2_656 2_656
Au3 Au2 Cu7 Cu1 123.94(14) . 2_656
Au3 Au2 Cu7 Cu7 133.82(10) . 2_656
Au3 Au2 Cu7 Cu7 37.15(8) 2_656 2_656
Au3 Au2 Cu7 Cu9 -66.32(8) . .
Au3 Au2 Cu7 Cu9 -162.99(8) 2_656 .
Au3 Au2 Cu7 S2 -30.5(3) 2_656 2_656
Au3 Au2 Cu7 S2 66.2(3) . 2_656
Au3 Au2 Cu7 S3 -118.39(16) . .
Au3 Au2 Cu7 S3 144.94(15) 2_656 .
Au3 Au2 Cu9 Au1 -43.5(3) 2_656 .
Au3 Au2 Cu9 Au1 -71.37(5) . .
Au3 Au2 Cu9 Au3 27.9(3) 2_656 .
Au3 Au2 Cu9 Cu7 67.10(8) . .
Au3 Au2 Cu9 Cu7 95.0(3) 2_656 .
Au3 Au2 Cu9 Cu15 -35.52(8) . .
Au3 Au2 Cu9 Cu15 -7.6(3) 2_656 .
Au3 Au2 Cu9 S7 -112.1(3) 2_656 .
Au3 Au2 Cu9 S7 -140.00(18) . .
Au3 Au2 Cu9 S3 115.13(15) . .
Au3 Au2 Cu9 S3 143.0(3) 2_656 .
Au3 Au2 Cu9 S8 8.0(3) . .
Au3 Au2 Cu9 S8 35.9(5) 2_656 .
Au3 Au2 Cu11 Au1 -25.10(7) . .
Au3 Au2 Cu11 Au1 97.76(6) 2_656 .
Au3 Au2 Cu11 Au6 -97.11(6) . 2_656
Au3 Au2 Cu11 Au6 25.75(7) 2_656 2_656
Au3 Au2 Cu11 Cu4 4.0(2) . .
Au3 Au2 Cu11 Cu4 126.87(16) 2_656 .
Au3 Au2 Cu11 Cu6 -39.30(8) 2_656 2_656
Au3 Au2 Cu11 Cu6 -162.16(8) . 2_656
Au3 Au2 Cu11 Cu12 -61.29(12) . .
Au3 Au2 Cu11 Cu12 61.57(12) 2_656 .
Au3 Au2 Cu11 S4 -170.01(16) . .
Au3 Au2 Cu11 S4 -47.15(19) 2_656 .
Au3 Au2 Cu11 S7 45.7(2) . .
Au3 Au2 Cu11 S7 168.61(17) 2_656 .
Au3 Au5 Au6 Au1 -99.70(4) . 2_656
Au3 Au5 Au6 Au2 -37.33(3) . 2_656
Au3 Au5 Au6 Au4 -138.62(4) . 2_656
Au3 Au5 Au6 Cu6 26.44(8) . .
Au3 Au5 Au6 Cu10 152.25(8) . .
Au3 Au5 Au6 Cu11 -70.3(3) . 2_656
Au3 Au5 Au6 Cu12 -163.49(8) . 2_656
Au3 Au5 Au6 Cu16 72.74(8) . .
Au3 Au5 Cu5 Au1 27.23(7) . .
Au3 Au5 Cu5 Au4 99.32(6) . .
Au3 Au5 Cu5 Cu12 64.47(11) . .
Au3 Au5 Cu5 S10 27.9(3) . .
Au3 Au5 Cu5 S18 173.55(16) . .
Au3 Au5 Cu5 S11 -80.38(16) . .
Au3 Au5 Cu8 Au4 25.3(3) . 2_656
Au3 Au5 Cu8 Au4 -48.1(3) . .
Au3 Au5 Cu8 Cu2 -84.2(3) . .
Au3 Au5 Cu8 Cu8 -14.3(4) . 2_656
Au3 Au5 Cu8 Cu10 92.8(2) . .
Au3 Au5 Cu8 S18 -123.1(2) . .
Au3 Au5 Cu8 S16 94.6(3) . .
Au3 Au5 Cu10 Au4 -96.15(6) . 2_656
Au3 Au5 Cu10 Au6 -26.14(7) . .
Au3 Au5 Cu10 Cu8 -161.67(8) . .
Au3 Au5 Cu10 Cu16 40.95(10) . .
Au3 Au5 Cu10 S9 -23.1(3) . 2_656
Au3 Au5 Cu10 S16 -163.24(15) . .
Au3 Au5 Cu10 S15 88.13(19) . .
Au3 Au5 Cu15 Au1 72.97(6) . .
Au3 Au5 Cu15 Cu9 37.44(8) . .
Au3 Au5 Cu15 Cu13 -62.70(12) . .
Au3 Au5 Cu15 Cu16 -69.69(9) . .
Au3 Au5 Cu15 S11 -177.10(18) . .
Au3 Au5 Cu15 S8 -12.4(3) . .
Au3 Au5 Cu16 Au6 -69.31(5) . .
Au3 Au5 Cu16 Cu10 -137.27(9) . .
Au3 Au5 Cu16 Cu13 55.50(12) . .
Au3 Au5 Cu16 Cu15 62.57(8) . .
Au3 Au5 Cu16 S15 173.22(18) . .
Au3 Au5 Cu16 S13 0.6(3) . .
Au3 Au6 Cu6 Au2 -70.02(5) . 2_656
Au3 Au6 Cu6 Cu11 -135.66(9) . 2_656
Au3 Au6 Cu6 S4 -179.59(18) . 2_656
Au3 Au6 Cu6 S2 -62.0(3) . 2_656
Au3 Au6 Cu6 S13 74.12(18) . .
Au3 Au6 Cu10 Au4 98.83(6) . 2_656
Au3 Au6 Cu10 Au5 26.20(7) . .
Au3 Au6 Cu10 Cu8 64.16(12) . .
Au3 Au6 Cu10 Cu16 -39.25(9) . .
Au3 Au6 Cu10 S9 -151.70(15) . 2_656
Au3 Au6 Cu10 S16 109.0(2) . .
Au3 Au6 Cu10 S15 -41.9(2) . .
Au3 Au6 Cu16 Au5 71.78(5) . .
Au3 Au6 Cu16 Cu10 138.41(9) . .
Au3 Au6 Cu16 Cu13 -31.63(15) . .
Au3 Au6 Cu16 Cu15 30.85(9) . .
Au3 Au6 Cu16 S15 141.2(2) . .
Au3 Au6 Cu16 S13 -72.9(2) . .
Au3 Cu6 S13 Cu13 -31.3(4) . .
Au3 Cu6 S13 Cu16 50.46(17) . .
Au3 Cu6 S13 C85 163.3(15) . .
Au3 Cu7 Cu9 Au1 -39.93(8) . .
Au3 Cu7 Cu9 Au2 -76.84(7) . .
Au3 Cu7 Cu9 Cu15 19.50(10) . .
Au3 Cu7 Cu9 S7 -129.7(3) . .
Au3 Cu7 Cu9 S3 178.0(2) . .
Au3 Cu7 Cu9 S8 70.20(17) . .
Au3 Cu7 S3 Cu1 -135.03(16) . .
Au3 Cu7 S3 Cu9 -1.77(18) . .
Au3 Cu7 S3 C15 116.8(7) . .
Au3 Cu9 Cu15 Au1 -76.43(7) . .
Au3 Cu9 Cu15 Au5 -39.63(8) . .
Au3 Cu9 Cu15 Cu13 76.59(10) . .
Au3 Cu9 Cu15 Cu16 18.07(11) . .
Au3 Cu9 Cu15 S11 -139.0(4) . .
Au3 Cu9 Cu15 S8 107.0(2) . .
Au3 Cu9 S7 Cu4 21.0(6) . .
Au3 Cu9 S7 Cu11 -54.7(3) . .
Au3 Cu9 S7 C43 -171.4(9) . .
Au3 Cu9 S3 Cu1 77.9(3) . .
Au3 Cu9 S3 Cu7 1.71(18) . .
Au3 Cu9 S3 C15 -105.9(8) . .
Au3 Cu9 S8 Cu13 14.3(4) . .
Au3 Cu9 S8 Cu15 -53.20(13) . .
Au3 Cu9 S8 C50 -158.0(10) . .
Au3 Cu15 Cu16 Au5 -77.05(8) . .
Au3 Cu15 Cu16 Au6 -33.68(9) . .
Au3 Cu15 Cu16 Cu10 -95.08(13) . .
Au3 Cu15 Cu16 Cu13 95.64(12) . .
Au3 Cu15 Cu16 S15 -149.1(2) . .
Au3 Cu15 Cu16 S13 70.03(19) . .
Au3 Cu15 S11 Cu5 -54.1(3) . .
Au3 Cu15 S11 Cu14 75.8(4) . .
Au3 Cu15 S11 C71 -164.0(9) . .
Au3 Cu15 S8 Cu9 54.62(13) . .
Au3 Cu15 S8 Cu13 -82.30(17) . .
Au3 Cu15 S8 C50 166.2(10) . .
Au3 Cu16 S15 Cu10 64.4(4) . .
Au3 Cu16 S15 Cu14 -73.0(4) . .
Au3 Cu16 S15 C99 174.1(12) . .
Au3 Cu16 S13 Cu6 -48.66(16) . .
Au3 Cu16 S13 Cu13 80.37(19) . .
Au3 Cu16 S13 C85 -160.6(13) . .
Au4 Au1 Au2 Au2 -64.45(5) . 2_656
Au4 Au1 Au2 Au3 -0.92(5) . 2_656
Au4 Au1 Au2 Au3 -100.84(4) . .
Au4 Au1 Au2 Au6 36.24(3) . 2_656
Au4 Au1 Au2 Cu6 62.81(8) . 2_656
Au4 Au1 Au2 Cu7 -40.3(2) . 2_656
Au4 Au1 Au2 Cu7 -128.09(7) . .
Au4 Au1 Au2 Cu9 -169.69(8) . .
Au4 Au1 Au2 Cu11 105.71(8) . .
Au4 Au1 Au3 Au2 63.95(4) . 2_656
Au4 Au1 Au3 Au2 101.56(4) . .
Au4 Au1 Au3 Au5 -37.02(3) . .
Au4 Au1 Au3 Au6 -0.45(5) . .
Au4 Au1 Au3 Cu6 26.6(3) . .
Au4 Au1 Au3 Cu7 127.82(7) . .
Au4 Au1 Au3 Cu9 171.34(8) . .
Au4 Au1 Au3 Cu15 -109.35(9) . .
Au4 Au1 Au3 Cu16 -62.37(8) . .
Au4 Au1 Au5 Au3 138.39(4) . .
Au4 Au1 Au5 Au4 38.96(3) . 2_656
Au4 Au1 Au5 Au6 101.96(4) . .
Au4 Au1 Au5 Cu5 -70.77(8) . .
Au4 Au1 Au5 Cu8 -23.30(7) . .
Au4 Au1 Au5 Cu10 68.0(3) . .
Au4 Au1 Au5 Cu15 -154.98(8) . .
Au4 Au1 Au5 Cu16 166.53(9) . .
Au4 Au1 Cu5 Au5 70.16(5) . .
Au4 Au1 Cu5 Cu12 -65.56(8) . .
Au4 Au1 Cu5 S10 -109.46(16) . .
Au4 Au1 Cu5 S18 6.4(3) . .
Au4 Au1 Cu5 S11 143.37(17) . .
Au4 Au1 Cu9 Au2 39.7(3) . .
Au4 Au1 Cu9 Au3 -32.6(3) . .
Au4 Au1 Cu9 Cu7 5.1(3) . .
Au4 Au1 Cu9 Cu15 -97.8(3) . .
Au4 Au1 Cu9 S7 149.9(3) . .
Au4 Au1 Cu9 S3 49.3(4) . .
Au4 Au1 Cu9 S8 -100.6(3) . .
Au4 Au1 Cu11 Au2 -99.08(6) . .
Au4 Au1 Cu11 Au6 -27.32(7) . 2_656
Au4 Au1 Cu11 Cu4 100.84(9) . .
Au4 Au1 Cu11 Cu6 -62.93(11) . 2_656
Au4 Au1 Cu11 Cu12 38.70(8) . .
Au4 Au1 Cu11 S4 -21.3(4) . .
Au4 Au1 Cu11 S7 149.44(15) . .
Au4 Au1 Cu12 Au6 -70.75(5) . 2_656
Au4 Au1 Cu12 Cu4 160.31(11) . .
Au4 Au1 Cu12 Cu5 66.91(8) . .
Au4 Au1 Cu12 Cu11 -137.54(9) . .
Au4 Au1 Cu12 S9 -73.7(3) . .
Au4 Au1 Cu12 S10 113.45(16) . .
Au4 Au1 Cu15 Au3 95.85(6) . .
Au4 Au1 Cu15 Au5 23.85(7) . .
Au4 Au1 Cu15 Cu9 163.01(7) . .
Au4 Au1 Cu15 Cu13 117.7(2) . .
Au4 Au1 Cu15 Cu16 54.54(13) . .
Au4 Au1 Cu15 S11 -48.02(18) . .
Au4 Au1 Cu15 S8 165.94(17) . .
Au4 Au4 Au5 Au1 137.35(3) 2_656 .
Au4 Au4 Au5 Au3 99.90(3) 2_656 .
Au4 Au4 Au5 Au6 36.68(3) 2_656 .
Au4 Au4 Au5 Cu5 -154.31(8) 2_656 .
Au4 Au4 Au5 Cu8 -67.07(7) 2_656 .
Au4 Au4 Au5 Cu10 -28.51(7) 2_656 .
Au4 Au4 Au5 Cu15 160.67(8) 2_656 .
Au4 Au4 Au5 Cu16 61.8(3) 2_656 .
Au4 Au4 Cu5 Au1 95.97(5) 2_656 .
Au4 Au4 Cu5 Au5 24.32(7) 2_656 .
Au4 Au4 Cu5 Cu12 162.65(7) 2_656 .
Au4 Au4 Cu5 S10 169.15(14) 2_656 .
Au4 Au4 Cu5 S18 -80.03(15) 2_656 .
Au4 Au4 Cu5 S11 24.8(3) 2_656 .
Au4 Au4 Cu8 Au5 72.05(5) 2_656 .
Au4 Au4 Cu8 Cu2 -134.66(11) 2_656 .
Au4 Au4 Cu8 Cu8 -67.72(10) 2_656 2_656
Au4 Au4 Cu8 Cu10 38.27(8) 2_656 .
Au4 Au4 Cu8 S18 176.62(18) 2_656 .
Au4 Au4 Cu8 S16 -15.0(3) 2_656 .
Au4 Au4 Cu12 Au1 -35.8(3) 2_656 .
Au4 Au4 Cu12 Au6 35.7(3) 2_656 2_656
Au4 Au4 Cu12 Cu4 -64.1(4) 2_656 .
Au4 Au4 Cu12 Cu5 -100.6(3) 2_656 .
Au4 Au4 Cu12 Cu11 -0.5(4) 2_656 .
Au4 Au4 Cu12 S9 106.7(3) 2_656 .
Au4 Au4 Cu12 S10 -107.5(3) 2_656 .
Au4 Au5 Au6 Au1 1.43(5) . 2_656
Au4 Au5 Au6 Au1 38.92(3) 2_656 2_656
Au4 Au5 Au6 Au2 63.79(4) . 2_656
Au4 Au5 Au6 Au2 101.29(4) 2_656 2_656
Au4 Au5 Au6 Au3 101.13(4) . .
Au4 Au5 Au6 Au3 138.62(4) 2_656 .
Au4 Au5 Au6 Au4 -37.50(3) . 2_656
Au4 Au5 Au6 Cu6 165.07(8) 2_656 .
Au4 Au5 Au6 Cu6 127.57(8) . .
Au4 Au5 Au6 Cu10 -69.13(8) 2_656 .
Au4 Au5 Au6 Cu10 -106.62(8) . .
Au4 Au5 Au6 Cu11 30.8(3) . 2_656
Au4 Au5 Au6 Cu11 68.3(3) 2_656 2_656
Au4 Au5 Au6 Cu12 -62.37(8) . 2_656
Au4 Au5 Au6 Cu12 -24.87(8) 2_656 2_656
Au4 Au5 Au6 Cu16 -148.64(9) 2_656 .
Au4 Au5 Au6 Cu16 173.87(9) . .
Au4 Au5 Cu5 Au1 -72.09(6) . .
Au4 Au5 Cu5 Au1 -97.17(6) 2_656 .
Au4 Au5 Cu5 Au4 -25.08(7) 2_656 .
Au4 Au5 Cu5 Cu12 -59.93(12) 2_656 .
Au4 Au5 Cu5 Cu12 -34.85(8) . .
Au4 Au5 Cu5 S10 -71.5(3) . .
Au4 Au5 Cu5 S10 -96.5(3) 2_656 .
Au4 Au5 Cu5 S18 74.23(17) . .
Au4 Au5 Cu5 S18 49.14(18) 2_656 .
Au4 Au5 Cu5 S11 155.22(15) 2_656 .
Au4 Au5 Cu5 S11 -179.70(17) . .
Au4 Au5 Cu8 Au4 73.41(6) . 2_656
Au4 Au5 Cu8 Au4 -73.41(6) 2_656 .
Au4 Au5 Cu8 Cu2 -109.48(18) 2_656 .
Au4 Au5 Cu8 Cu2 -36.07(14) . .
Au4 Au5 Cu8 Cu8 -39.58(11) 2_656 2_656
Au4 Au5 Cu8 Cu8 33.83(11) . 2_656
Au4 Au5 Cu8 Cu10 140.92(10) . .
Au4 Au5 Cu8 Cu10 67.52(8) 2_656 .
Au4 Au5 Cu8 S18 -148.44(19) 2_656 .
Au4 Au5 Cu8 S18 -75.04(17) . .
Au4 Au5 Cu8 S16 142.7(2) . .
Au4 Au5 Cu8 S16 69.27(17) 2_656 .
Au4 Au5 Cu10 Au4 29.28(7) . 2_656
Au4 Au5 Cu10 Au6 99.30(6) . .
Au4 Au5 Cu10 Au6 70.01(5) 2_656 .
Au4 Au5 Cu10 Cu8 -36.23(9) . .
Au4 Au5 Cu10 Cu8 -65.52(8) 2_656 .
Au4 Au5 Cu10 Cu16 137.10(10) 2_656 .
Au4 Au5 Cu10 Cu16 166.39(9) . .
Au4 Au5 Cu10 S9 73.1(3) 2_656 2_656
Au4 Au5 Cu10 S9 102.4(3) . 2_656
Au4 Au5 Cu10 S16 -37.80(18) . .
Au4 Au5 Cu10 S16 -67.08(16) 2_656 .
Au4 Au5 Cu10 S15 -175.7(2) 2_656 .
Au4 Au5 Cu10 S15 -146.44(18) . .
Au4 Au5 Cu15 Au1 48.3(3) 2_656 .
Au4 Au5 Cu15 Au1 -23.94(7) . .
Au4 Au5 Cu15 Au3 -24.7(3) 2_656 .
Au4 Au5 Cu15 Au3 -96.91(6) . .
Au4 Au5 Cu15 Cu9 12.8(3) 2_656 .
Au4 Au5 Cu15 Cu9 -59.47(12) . .
Au4 Au5 Cu15 Cu13 -159.61(11) . .
Au4 Au5 Cu15 Cu13 -87.4(3) 2_656 .
Au4 Au5 Cu15 Cu16 -166.60(9) . .
Au4 Au5 Cu15 Cu16 -94.4(2) 2_656 .
Au4 Au5 Cu15 S11 158.2(2) 2_656 .
Au4 Au5 Cu15 S11 85.99(16) . .
Au4 Au5 Cu15 S8 -109.3(3) . .
Au4 Au5 Cu15 S8 -37.0(5) 2_656 .
Au4 Au5 Cu16 Au3 41.6(4) . .
Au4 Au5 Cu16 Au3 98.26(6) 2_656 .
Au4 Au5 Cu16 Au6 -27.7(4) . .
Au4 Au5 Cu16 Au6 28.95(7) 2_656 .
Au4 Au5 Cu16 Cu10 -39.01(9) 2_656 .
Au4 Au5 Cu16 Cu10 -95.7(3) . .
Au4 Au5 Cu16 Cu13 153.76(12) 2_656 .
Au4 Au5 Cu16 Cu13 97.1(4) . .
Au4 Au5 Cu16 Cu15 104.2(3) . .
Au4 Au5 Cu16 Cu15 160.83(8) 2_656 .
Au4 Au5 Cu16 S15 -145.2(3) . .
Au4 Au5 Cu16 S15 -88.52(17) 2_656 .
Au4 Au5 Cu16 S13 42.2(6) . .
Au4 Au5 Cu16 S13 98.9(3) 2_656 .
Au4 Au6 Cu6 Au2 -29.8(3) 2_656 2_656
Au4 Au6 Cu6 Au3 40.2(3) 2_656 .
Au4 Au6 Cu6 Cu11 -95.4(3) 2_656 2_656
Au4 Au6 Cu6 S4 -139.4(3) 2_656 2_656
Au4 Au6 Cu6 S2 -21.8(5) 2_656 2_656
Au4 Au6 Cu6 S13 114.3(3) 2_656 .
Au4 Au6 Cu10 Au5 -72.63(5) 2_656 .
Au4 Au6 Cu10 Cu8 -34.67(8) 2_656 .
Au4 Au6 Cu10 Cu16 -138.08(9) 2_656 .
Au4 Au6 Cu10 S9 109.47(16) 2_656 2_656
Au4 Au6 Cu10 S16 10.2(2) 2_656 .
Au4 Au6 Cu10 S15 -140.7(2) 2_656 .
Au4 Au6 Cu16 Au3 -100.82(6) 2_656 .
Au4 Au6 Cu16 Au5 -29.04(7) 2_656 .
Au4 Au6 Cu16 Cu10 37.59(8) 2_656 .
Au4 Au6 Cu16 Cu13 -132.45(16) 2_656 .
Au4 Au6 Cu16 Cu15 -69.97(12) 2_656 .
Au4 Au6 Cu16 S15 40.4(2) 2_656 .
Au4 Au6 Cu16 S13 -173.71(19) 2_656 .
Au4 Cu5 Cu12 Au1 -77.04(7) . .
Au4 Cu5 Cu12 Au6 -38.98(8) . 2_656
Au4 Cu5 Cu12 Cu4 -155.47(12) . .
Au4 Cu5 Cu12 Cu11 -97.93(11) . .
Au4 Cu5 Cu12 S9 56.2(3) . .
Au4 Cu5 Cu12 S10 171.4(2) . .
Au4 Cu5 S10 Cu4 -85.2(3) . .
Au4 Cu5 S10 Cu12 -7.29(18) . .
Au4 Cu5 S10 C64 104.8(10) . .
Au4 Cu5 S18 Cu2 -33.2(3) . .
Au4 Cu5 S18 Cu8 47.17(16) . .
Au4 Cu5 S18 C120 161.8(9) . .
Au4 Cu5 S11 Cu14 -36.9(5) . .
Au4 Cu5 S11 Cu15 51.1(3) . .
Au4 Cu5 S11 C71 170.1(9) . .
Au4 Cu8 Cu10 Au4 -41.04(9) . 2_656
Au4 Cu8 Cu10 Au5 35.46(8) . .
Au4 Cu8 Cu10 Au5 76.50(8) 2_656 .
Au4 Cu8 Cu10 Au6 -4.28(14) . .
Au4 Cu8 Cu10 Au6 36.76(8) 2_656 .
Au4 Cu8 Cu10 Cu16 96.13(13) 2_656 .
Au4 Cu8 Cu10 Cu16 55.09(15) . .
Au4 Cu8 Cu10 S9 -93.9(3) . 2_656
Au4 Cu8 Cu10 S9 -52.9(3) 2_656 2_656
Au4 Cu8 Cu10 S16 -146.5(2) . .
Au4 Cu8 Cu10 S16 -105.49(19) 2_656 .
Au4 Cu8 Cu10 S15 105.1(2) . .
Au4 Cu8 Cu10 S15 146.1(2) 2_656 .
Au4 Cu8 S18 Cu2 81.88(16) . .
Au4 Cu8 S18 Cu2 87.1(3) 2_656 .
Au4 Cu8 S18 Cu5 -42.0(4) 2_656 .
Au4 Cu8 S18 Cu5 -47.28(16) . .
Au4 Cu8 S18 C120 -161.3(8) . .
Au4 Cu8 S18 C120 -156.1(8) 2_656 .
Au4 Cu8 S16 Cu2 -77.47(16) 2_656 2_656
Au4 Cu8 S16 Cu2 -64.0(4) . 2_656
Au4 Cu8 S16 Cu10 55.21(12) 2_656 .
Au4 Cu8 S16 Cu10 68.7(4) . .
Au4 Cu8 S16 C106 -172.9(8) . .
Au4 Cu8 S16 C106 173.6(8) 2_656 .
Au4 Cu10 Cu16 Au3 -0.07(14) 2_656 .
Au4 Cu10 Cu16 Au5 38.84(8) 2_656 .
Au4 Cu10 Cu16 Au6 -37.31(8) 2_656 .
Au4 Cu10 Cu16 Cu13 105.4(7) 2_656 .
Au4 Cu10 Cu16 Cu15 57.03(15) 2_656 .
Au4 Cu10 Cu16 S15 146.0(2) 2_656 .
Au4 Cu10 Cu16 S13 -97.5(4) 2_656 .
Au4 Cu10 S16 Cu2 21.1(3) 2_656 2_656
Au4 Cu10 S16 Cu8 -54.66(13) 2_656 .
Au4 Cu10 S16 C106 -162.9(8) 2_656 .
Au4 Cu10 S15 Cu14 16.8(7) 2_656 .
Au4 Cu10 S15 Cu16 -59.2(4) 2_656 .
Au4 Cu10 S15 C99 -173.9(12) 2_656 .
Au4 Cu12 S9 Cu3 -138.31(15) . .
Au4 Cu12 S9 Cu10 -5.05(18) . 2_656
Au4 Cu12 S9 C57 106.8(8) . .
Au4 Cu12 S10 Cu4 138.57(16) . .
Au4 Cu12 S10 Cu5 7.47(19) . .
Au4 Cu12 S10 C64 -106.6(8) . .
Au5 Au1 Au2 Au2 -1.22(5) . 2_656
Au5 Au1 Au2 Au3 -37.60(3) . .
Au5 Au1 Au2 Au3 62.32(4) . 2_656
Au5 Au1 Au2 Au6 99.48(4) . 2_656
Au5 Au1 Au2 Cu6 126.05(7) . 2_656
Au5 Au1 Au2 Cu7 23.0(3) . 2_656
Au5 Au1 Au2 Cu7 -64.85(8) . .
Au5 Au1 Au2 Cu9 -106.45(8) . .
Au5 Au1 Au2 Cu11 168.95(9) . .
Au5 Au1 Au3 Au2 100.96(4) . 2_656
Au5 Au1 Au3 Au2 138.58(4) . .
Au5 Au1 Au3 Au6 36.57(3) . .
Au5 Au1 Au3 Cu6 63.6(3) . .
Au5 Au1 Au3 Cu7 164.84(7) . .
Au5 Au1 Au3 Cu9 -151.64(8) . .
Au5 Au1 Au3 Cu15 -72.34(8) . .
Au5 Au1 Au3 Cu16 -25.35(7) . .
Au5 Au1 Au4 Au4 -37.96(4) . 2_656
Au5 Au1 Au4 Au5 -99.80(4) . 2_656
Au5 Au1 Au4 Au6 -138.52(4) . 2_656
Au5 Au1 Au4 Cu5 70.18(7) . .
Au5 Au1 Au4 Cu8 23.11(7) . .
Au5 Au1 Au4 Cu8 -67.4(3) . 2_656
Au5 Au1 Au4 Cu10 -162.94(8) . 2_656
Au5 Au1 Au4 Cu12 151.81(8) . .
Au5 Au1 Cu5 Au4 -70.16(5) . .
Au5 Au1 Cu5 Cu12 -135.72(9) . .
Au5 Au1 Cu5 S10 -179.62(17) . .
Au5 Au1 Cu5 S18 -63.7(3) . .
Au5 Au1 Cu5 S11 73.21(15) . .
Au5 Au1 Cu9 Au2 99.05(6) . .
Au5 Au1 Cu9 Au3 26.81(7) . .
Au5 Au1 Cu9 Cu7 64.42(11) . .
Au5 Au1 Cu9 Cu15 -38.47(9) . .
Au5 Au1 Cu9 S7 -150.73(16) . .
Au5 Au1 Cu9 S3 108.6(2) . .
Au5 Au1 Cu9 S8 -41.19(18) . .
Au5 Au1 Cu11 Au2 -44.4(3) . .
Au5 Au1 Cu11 Au6 27.4(3) . 2_656
Au5 Au1 Cu11 Cu4 155.5(3) . .
Au5 Au1 Cu11 Cu6 -8.2(4) . 2_656
Au5 Au1 Cu11 Cu12 93.4(3) . .
Au5 Au1 Cu11 S4 33.4(5) . .
Au5 Au1 Cu11 S7 -155.9(3) . .
Au5 Au1 Cu12 Au4 -26.19(7) . .
Au5 Au1 Cu12 Au6 -96.94(6) . 2_656
Au5 Au1 Cu12 Cu4 134.12(8) . .
Au5 Au1 Cu12 Cu5 40.72(8) . .
Au5 Au1 Cu12 Cu11 -163.73(8) . .
Au5 Au1 Cu12 S9 -99.9(3) . .
Au5 Au1 Cu12 S10 87.26(15) . .
Au5 Au1 Cu15 Au3 72.00(5) . .
Au5 Au1 Cu15 Cu9 139.16(9) . .
Au5 Au1 Cu15 Cu13 93.9(2) . .
Au5 Au1 Cu15 Cu16 30.69(9) . .
Au5 Au1 Cu15 S11 -71.87(16) . .
Au5 Au1 Cu15 S8 142.1(2) . .
Au5 Au3 Au6 Au1 101.28(4) . 2_656
Au5 Au3 Au6 Au2 137.79(4) . 2_656
Au5 Au3 Au6 Au4 37.50(3) . 2_656
Au5 Au3 Au6 Cu6 -152.09(8) . .
Au5 Au3 Au6 Cu10 -25.50(7) . .
Au5 Au3 Au6 Cu11 163.14(8) . 2_656
Au5 Au3 Au6 Cu12 76.8(3) . 2_656
Au5 Au3 Au6 Cu16 -66.59(8) . .
Au5 Au3 Cu6 Au2 98.63(6) . 2_656
Au5 Au3 Cu6 Au6 26.06(7) . .
Au5 Au3 Cu6 Cu11 63.16(11) . 2_656
Au5 Au3 Cu6 S4 26.7(3) . 2_656
Au5 Au3 Cu6 S2 173.24(15) . 2_656
Au5 Au3 Cu6 S13 -79.1(2) . .
Au5 Au3 Cu7 Au2 24.8(3) . .
Au5 Au3 Cu7 Au2 -48.1(2) . 2_656
Au5 Au3 Cu7 Cu1 -82.7(3) . 2_656
Au5 Au3 Cu7 Cu7 -14.5(3) . 2_656
Au5 Au3 Cu7 Cu9 92.1(2) . .
Au5 Au3 Cu7 S2 -122.6(2) . 2_656
Au5 Au3 Cu7 S3 93.8(3) . .
Au5 Au3 Cu9 Au1 -26.41(7) . .
Au5 Au3 Cu9 Au2 -96.40(6) . .
Au5 Au3 Cu9 Cu7 -161.78(8) . .
Au5 Au3 Cu9 Cu15 40.77(9) . .
Au5 Au3 Cu9 S7 -22.8(3) . .
Au5 Au3 Cu9 S3 -163.31(15) . .
Au5 Au3 Cu9 S8 88.69(17) . .
Au5 Au3 Cu15 Au1 -69.38(5) . .
Au5 Au3 Cu15 Cu9 -136.76(9) . .
Au5 Au3 Cu15 Cu13 124.61(11) . .
Au5 Au3 Cu15 Cu16 62.64(8) . .
Au5 Au3 Cu15 S11 4.8(3) . .
Au5 Au3 Cu15 S8 172.87(19) . .
Au5 Au3 Cu16 Au6 72.84(6) . .
Au5 Au3 Cu16 Cu10 36.68(8) . .
Au5 Au3 Cu16 Cu13 -131.05(11) . .
Au5 Au3 Cu16 Cu15 -69.27(9) . .
Au5 Au3 Cu16 S15 -11.4(3) . .
Au5 Au3 Cu16 S13 -179.6(2) . .
Au5 Au4 Au5 Au1 100.67(4) 2_656 .
Au5 Au4 Au5 Au3 63.23(4) 2_656 .
Au5 Au4 Au5 Au4 -36.68(4) 2_656 2_656
Au5 Au4 Au5 Au6 0.01(5) 2_656 .
Au5 Au4 Au5 Cu5 169.01(8) 2_656 .
Au5 Au4 Au5 Cu8 -103.75(8) 2_656 .
Au5 Au4 Au5 Cu10 -65.18(9) 2_656 .
Au5 Au4 Au5 Cu15 123.99(7) 2_656 .
Au5 Au4 Au5 Cu16 25.2(4) 2_656 .
Au5 Au4 Cu5 Au1 71.65(5) . .
Au5 Au4 Cu5 Au1 33.9(3) 2_656 .
Au5 Au4 Cu5 Au5 -37.8(3) 2_656 .
Au5 Au4 Cu5 Cu12 138.33(9) . .
Au5 Au4 Cu5 Cu12 100.6(2) 2_656 .
Au5 Au4 Cu5 S10 144.83(18) . .
Au5 Au4 Cu5 S10 107.1(3) 2_656 .
Au5 Au4 Cu5 S18 -142.1(2) 2_656 .
Au5 Au4 Cu5 S18 -104.35(16) . .
Au5 Au4 Cu5 S11 -37.3(5) 2_656 .
Au5 Au4 Cu5 S11 0.5(3) . .
Au5 Au4 Cu8 Au4 26.21(8) 2_656 2_656
Au5 Au4 Cu8 Au4 -72.05(5) . 2_656
Au5 Au4 Cu8 Au5 98.26(6) 2_656 .
Au5 Au4 Cu8 Cu2 -108.45(8) 2_656 .
Au5 Au4 Cu8 Cu2 153.29(10) . .
Au5 Au4 Cu8 Cu8 -139.78(11) . 2_656
Au5 Au4 Cu8 Cu8 -41.52(8) 2_656 2_656
Au5 Au4 Cu8 Cu10 -33.78(9) . .
Au5 Au4 Cu8 Cu10 64.48(12) 2_656 .
Au5 Au4 Cu8 S18 104.57(16) . .
Au5 Au4 Cu8 S18 -157.17(15) 2_656 .
Au5 Au4 Cu8 S16 -87.0(4) . .
Au5 Au4 Cu8 S16 11.3(4) 2_656 .
Au5 Au4 Cu12 Au1 -96.51(6) 2_656 .
Au5 Au4 Cu12 Au1 26.41(7) . .
Au5 Au4 Cu12 Au6 97.97(6) . 2_656
Au5 Au4 Cu12 Au6 -24.94(7) 2_656 2_656
Au5 Au4 Cu12 Cu4 -124.78(16) 2_656 .
Au5 Au4 Cu12 Cu4 -1.9(2) . .
Au5 Au4 Cu12 Cu5 -38.35(9) . .
Au5 Au4 Cu12 Cu5 -161.26(8) 2_656 .
Au5 Au4 Cu12 Cu11 61.72(12) . .
Au5 Au4 Cu12 Cu11 -61.19(12) 2_656 .
Au5 Au4 Cu12 S9 46.06(18) 2_656 .
Au5 Au4 Cu12 S9 168.97(16) . .
Au5 Au4 Cu12 S10 -45.28(19) . .
Au5 Au4 Cu12 S10 -168.20(16) 2_656 .
Au5 Au6 Cu6 Au2 -96.69(6) . 2_656
Au5 Au6 Cu6 Au3 -26.67(7) . .
Au5 Au6 Cu6 Cu11 -162.32(8) . 2_656
Au5 Au6 Cu6 S4 153.74(16) . 2_656
Au5 Au6 Cu6 S2 -88.7(3) . 2_656
Au5 Au6 Cu6 S13 47.46(19) . .
Au5 Au6 Cu10 Au4 72.63(5) . 2_656
Au5 Au6 Cu10 Cu8 37.96(8) . .
Au5 Au6 Cu10 Cu16 -65.45(8) . .
Au5 Au6 Cu10 S9 -177.90(17) . 2_656
Au5 Au6 Cu10 S16 82.8(2) . .
Au5 Au6 Cu10 S15 -68.05(18) . .
Au5 Au6 Cu16 Au3 -71.78(5) . .
Au5 Au6 Cu16 Cu10 66.63(8) . .
Au5 Au6 Cu16 Cu13 -103.41(18) . .
Au5 Au6 Cu16 Cu15 -40.93(9) . .
Au5 Au6 Cu16 S15 69.4(2) . .
Au5 Au6 Cu16 S13 -144.7(2) . .
Au5 Cu5 Cu12 Au1 -39.84(8) . .
Au5 Cu5 Cu12 Au4 37.20(8) . .
Au5 Cu5 Cu12 Au6 -1.78(14) . 2_656
Au5 Cu5 Cu12 Cu4 -118.27(11) . .
Au5 Cu5 Cu12 Cu11 -60.73(13) . .
Au5 Cu5 Cu12 S9 93.4(3) . .
Au5 Cu5 Cu12 S10 -151.4(2) . .
Au5 Cu5 S10 Cu4 -26.8(6) . .
Au5 Cu5 S10 Cu12 51.1(4) . .
Au5 Cu5 S10 C64 163.2(10) . .
Au5 Cu5 S18 Cu2 -92.1(3) . .
Au5 Cu5 S18 Cu8 -11.65(19) . .
Au5 Cu5 S18 C120 103.0(9) . .
Au5 Cu5 S11 Cu14 -36.4(3) . .
Au5 Cu5 S11 Cu15 51.55(14) . .
Au5 Cu5 S11 C71 170.5(9) . .
Au5 Cu8 Cu10 Au4 -76.50(7) . 2_656
Au5 Cu8 Cu10 Au6 -39.74(8) . .
Au5 Cu8 Cu10 Cu16 19.63(10) . .
Au5 Cu8 Cu10 S9 -129.4(3) . 2_656
Au5 Cu8 Cu10 S16 178.0(2) . .
Au5 Cu8 Cu10 S15 69.6(2) . .
Au5 Cu8 S18 Cu2 140.78(16) . .
Au5 Cu8 S18 Cu5 11.61(19) . .
Au5 Cu8 S18 C120 -102.5(8) . .
Au5 Cu8 S16 Cu2 -134.47(16) . 2_656
Au5 Cu8 S16 Cu10 -1.80(18) . .
Au5 Cu8 S16 C106 116.6(8) . .
Au5 Cu10 Cu16 Au3 -38.91(8) . .
Au5 Cu10 Cu16 Au6 -76.15(8) . .
Au5 Cu10 Cu16 Cu13 66.5(7) . .
Au5 Cu10 Cu16 Cu15 18.19(10) . .
Au5 Cu10 Cu16 S15 107.2(2) . .
Au5 Cu10 Cu16 S13 -136.4(4) . .
Au5 Cu10 S16 Cu2 77.5(3) . 2_656
Au5 Cu10 S16 Cu8 1.75(18) . .
Au5 Cu10 S16 C106 -106.5(8) . .
Au5 Cu10 S15 Cu14 22.9(5) . .
Au5 Cu10 S15 Cu16 -53.18(15) . .
Au5 Cu10 S15 C99 -167.9(12) . .
Au5 Cu15 Cu16 Au3 77.05(8) . .
Au5 Cu15 Cu16 Au6 43.37(9) . .
Au5 Cu15 Cu16 Cu10 -18.02(10) . .
Au5 Cu15 Cu16 Cu13 172.70(14) . .
Au5 Cu15 Cu16 S15 -72.0(2) . .
Au5 Cu15 Cu16 S13 147.1(2) . .
Au5 Cu15 S11 Cu5 -49.82(13) . .
Au5 Cu15 S11 Cu14 80.15(18) . .
Au5 Cu15 S11 C71 -159.7(9) . .
Au5 Cu15 S8 Cu9 65.7(4) . .
Au5 Cu15 S8 Cu13 -71.3(4) . .
Au5 Cu15 S8 C50 177.2(10) . .
Au5 Cu16 S15 Cu10 54.23(15) . .
Au5 Cu16 S15 Cu14 -83.2(2) . .
Au5 Cu16 S15 C99 163.9(12) . .
Au5 Cu16 S13 Cu6 -49.2(4) . .
Au5 Cu16 S13 Cu13 79.8(4) . .
Au5 Cu16 S13 C85 -161.1(13) . .
Au6 Au1 Au2 Au2 -100.69(4) 2_656 2_656
Au6 Au1 Au2 Au3 -137.07(3) 2_656 .
Au6 Au1 Au2 Au3 -37.16(3) 2_656 2_656
Au6 Au1 Au2 Cu6 26.57(7) 2_656 2_656
Au6 Au1 Au2 Cu7 -164.33(8) 2_656 .
Au6 Au1 Au2 Cu7 -76.5(2) 2_656 2_656
Au6 Au1 Au2 Cu9 154.08(8) 2_656 .
Au6 Au1 Au2 Cu11 69.48(8) 2_656 .
Au6 Au1 Au3 Au2 38.72(3) 2_656 .
Au6 Au1 Au3 Au2 1.10(5) 2_656 2_656
Au6 Au1 Au3 Au5 -99.86(4) 2_656 .
Au6 Au1 Au3 Au6 -63.29(4) 2_656 .
Au6 Au1 Au3 Cu6 -36.3(3) 2_656 .
Au6 Au1 Au3 Cu7 64.97(8) 2_656 .
Au6 Au1 Au3 Cu9 108.50(8) 2_656 .
Au6 Au1 Au3 Cu15 -172.20(9) 2_656 .
Au6 Au1 Au3 Cu16 -125.21(8) 2_656 .
Au6 Au1 Au4 Au4 100.56(4) 2_656 2_656
Au6 Au1 Au4 Au5 138.52(4) 2_656 .
Au6 Au1 Au4 Au5 38.73(3) 2_656 2_656
Au6 Au1 Au4 Cu5 -151.29(8) 2_656 .
Au6 Au1 Au4 Cu8 161.63(8) 2_656 .
Au6 Au1 Au4 Cu8 71.1(3) 2_656 2_656
Au6 Au1 Au4 Cu10 -24.41(7) 2_656 2_656
Au6 Au1 Au4 Cu12 -69.66(8) 2_656 .
Au6 Au1 Au5 Au3 101.77(4) 2_656 .
Au6 Au1 Au5 Au4 -36.62(3) 2_656 .
Au6 Au1 Au5 Au4 2.33(5) 2_656 2_656
Au6 Au1 Au5 Au6 65.33(4) 2_656 .
Au6 Au1 Au5 Cu5 -107.39(8) 2_656 .
Au6 Au1 Au5 Cu8 -59.92(8) 2_656 .
Au6 Au1 Au5 Cu10 31.3(3) 2_656 .
Au6 Au1 Au5 Cu15 168.40(8) 2_656 .
Au6 Au1 Au5 Cu16 129.90(8) 2_656 .
Au6 Au1 Cu5 Au4 26.75(7) 2_656 .
Au6 Au1 Cu5 Au5 96.91(6) 2_656 .
Au6 Au1 Cu5 Cu12 -38.81(8) 2_656 .
Au6 Au1 Cu5 S10 -82.71(16) 2_656 .
Au6 Au1 Cu5 S18 33.2(3) 2_656 .
Au6 Au1 Cu5 S11 170.12(14) 2_656 .
Au6 Au1 Cu9 Au2 -24.85(7) 2_656 .
Au6 Au1 Cu9 Au3 -97.08(6) 2_656 .
Au6 Au1 Cu9 Cu7 -59.48(11) 2_656 .
Au6 Au1 Cu9 Cu15 -162.37(8) 2_656 .
Au6 Au1 Cu9 S7 85.38(16) 2_656 .
Au6 Au1 Cu9 S3 -15.3(3) 2_656 .
Au6 Au1 Cu9 S8 -165.09(16) 2_656 .
Au6 Au1 Cu11 Au2 -71.77(5) 2_656 .
Au6 Au1 Cu11 Cu4 128.16(10) 2_656 .
Au6 Au1 Cu11 Cu6 -35.61(8) 2_656 2_656
Au6 Au1 Cu11 Cu12 66.02(8) 2_656 .
Au6 Au1 Cu11 S4 6.0(3) 2_656 .
Au6 Au1 Cu11 S7 176.76(18) 2_656 .
Au6 Au1 Cu12 Au4 70.75(5) 2_656 .
Au6 Au1 Cu12 Cu4 -128.94(10) 2_656 .
Au6 Au1 Cu12 Cu5 137.66(9) 2_656 .
Au6 Au1 Cu12 Cu11 -66.79(8) 2_656 .
Au6 Au1 Cu12 S9 -2.9(3) 2_656 .
Au6 Au1 Cu12 S10 -175.80(17) 2_656 .
Au6 Au1 Cu15 Au3 27.9(3) 2_656 .
Au6 Au1 Cu15 Au5 -44.1(3) 2_656 .
Au6 Au1 Cu15 Cu9 95.0(3) 2_656 .
Au6 Au1 Cu15 Cu13 49.7(4) 2_656 .
Au6 Au1 Cu15 Cu16 -13.5(4) 2_656 .
Au6 Au1 Cu15 S11 -116.0(3) 2_656 .
Au6 Au1 Cu15 S8 98.0(3) 2_656 .
Au6 Au2 Au3 Au1 -38.40(3) 2_656 .
Au6 Au2 Au3 Au2 100.15(3) 2_656 2_656
Au6 Au2 Au3 Au5 -1.91(4) 2_656 .
Au6 Au2 Au3 Au6 61.44(4) 2_656 .
Au6 Au2 Au3 Cu6 124.60(8) 2_656 .
Au6 Au2 Au3 Cu7 170.85(8) 2_656 .
Au6 Au2 Au3 Cu9 -109.36(8) 2_656 .
Au6 Au2 Au3 Cu15 -66.96(8) 2_656 .
Au6 Au2 Au3 Cu16 18.4(2) 2_656 .
Au6 Au2 Cu7 Au2 34.6(3) 2_656 2_656
Au6 Au2 Cu7 Au3 -34.9(3) 2_656 .
Au6 Au2 Cu7 Cu1 89.0(3) 2_656 2_656
Au6 Au2 Cu7 Cu7 98.9(2) 2_656 2_656
Au6 Au2 Cu7 Cu9 -101.2(3) 2_656 .
Au6 Au2 Cu7 S2 31.3(5) 2_656 2_656
Au6 Au2 Cu7 S3 -153.3(3) 2_656 .
Au6 Au2 Cu9 Au1 24.84(7) 2_656 .
Au6 Au2 Cu9 Au3 96.21(6) 2_656 .
Au6 Au2 Cu9 Cu7 163.31(8) 2_656 .
Au6 Au2 Cu9 Cu15 60.69(12) 2_656 .
Au6 Au2 Cu9 S7 -43.78(18) 2_656 .
Au6 Au2 Cu9 S3 -148.66(13) 2_656 .
Au6 Au2 Cu9 S8 104.2(3) 2_656 .
Au6 Au2 Cu11 Au1 72.02(5) 2_656 .
Au6 Au2 Cu11 Cu4 101.12(18) 2_656 .
Au6 Au2 Cu11 Cu6 -65.05(8) 2_656 2_656
Au6 Au2 Cu11 Cu12 35.82(8) 2_656 .
Au6 Au2 Cu11 S4 -72.90(18) 2_656 .
Au6 Au2 Cu11 S7 142.9(2) 2_656 .
Au6 Au3 Au5 Au1 -139.06(4) . .
Au6 Au3 Au5 Au4 -101.35(4) . .
Au6 Au3 Au5 Au4 -36.56(3) . 2_656
Au6 Au3 Au5 Cu5 -165.78(8) . .
Au6 Au3 Au5 Cu8 -58.7(2) . .
Au6 Au3 Au5 Cu10 26.42(8) . .
Au6 Au3 Au5 Cu15 151.10(8) . .
Au6 Au3 Au5 Cu16 69.89(8) . .
Au6 Au3 Cu6 Au2 72.57(5) . 2_656
Au6 Au3 Cu6 Cu11 37.10(8) . 2_656
Au6 Au3 Cu6 S4 0.7(3) . 2_656
Au6 Au3 Cu6 S2 147.18(18) . 2_656
Au6 Au3 Cu6 S13 -105.2(2) . .
Au6 Au3 Cu7 Au2 96.95(6) . .
Au6 Au3 Cu7 Au2 24.06(7) . 2_656
Au6 Au3 Cu7 Cu1 -10.56(18) . 2_656
Au6 Au3 Cu7 Cu7 57.60(15) . 2_656
Au6 Au3 Cu7 Cu9 164.20(8) . .
Au6 Au3 Cu7 S2 -50.47(18) . 2_656
Au6 Au3 Cu7 S3 165.90(16) . .
Au6 Au3 Cu9 Au1 32.9(3) . .
Au6 Au3 Cu9 Au2 -37.1(3) . .
Au6 Au3 Cu9 Cu7 -102.5(3) . .
Au6 Au3 Cu9 Cu15 100.1(3) . .
Au6 Au3 Cu9 S7 36.5(5) . .
Au6 Au3 Cu9 S3 -104.0(3) . .
Au6 Au3 Cu9 S8 148.0(3) . .
Au6 Au3 Cu15 Au1 -96.85(6) . .
Au6 Au3 Cu15 Au5 -27.47(7) . .
Au6 Au3 Cu15 Cu9 -164.23(8) . .
Au6 Au3 Cu15 Cu13 97.14(10) . .
Au6 Au3 Cu15 Cu16 35.17(10) . .
Au6 Au3 Cu15 S11 -22.7(3) . .
Au6 Au3 Cu15 S8 145.40(16) . .
Au6 Au3 Cu16 Au5 -72.84(6) . .
Au6 Au3 Cu16 Cu10 -36.16(8) . .
Au6 Au3 Cu16 Cu13 156.11(12) . .
Au6 Au3 Cu16 Cu15 -142.11(10) . .
Au6 Au3 Cu16 S15 -84.3(3) . .
Au6 Au3 Cu16 S13 107.54(19) . .
Au6 Au4 Au5 Au1 37.27(3) 2_656 .
Au6 Au4 Au5 Au3 -0.17(4) 2_656 .
Au6 Au4 Au5 Au4 -100.07(4) 2_656 2_656
Au6 Au4 Au5 Au6 -63.39(4) 2_656 .
Au6 Au4 Au5 Cu5 105.61(8) 2_656 .
Au6 Au4 Au5 Cu8 -167.14(8) 2_656 .
Au6 Au4 Au5 Cu10 -128.58(8) 2_656 .
Au6 Au4 Au5 Cu15 60.60(8) 2_656 .
Au6 Au4 Au5 Cu16 -38.2(4) 2_656 .
Au6 Au4 Cu5 Au1 -26.81(7) 2_656 .
Au6 Au4 Cu5 Au5 -98.46(6) 2_656 .
Au6 Au4 Cu5 Cu12 39.87(9) 2_656 .
Au6 Au4 Cu5 S10 46.37(17) 2_656 .
Au6 Au4 Cu5 S18 157.19(14) 2_656 .
Au6 Au4 Cu5 S11 -98.0(3) 2_656 .
Au6 Au4 Cu8 Au4 -25.7(3) 2_656 2_656
Au6 Au4 Cu8 Au5 46.3(3) 2_656 .
Au6 Au4 Cu8 Cu2 -160.4(2) 2_656 .
Au6 Au4 Cu8 Cu8 -93.4(2) 2_656 2_656
Au6 Au4 Cu8 Cu10 12.6(3) 2_656 .
Au6 Au4 Cu8 S18 150.9(2) 2_656 .
Au6 Au4 Cu8 S16 -40.7(5) 2_656 .
Au6 Au4 Cu12 Au1 -71.57(5) 2_656 .
Au6 Au4 Cu12 Cu4 -99.84(18) 2_656 .
Au6 Au4 Cu12 Cu5 -136.32(9) 2_656 .
Au6 Au4 Cu12 Cu11 -36.25(8) 2_656 .
Au6 Au4 Cu12 S9 71.00(17) 2_656 .
Au6 Au4 Cu12 S10 -143.26(19) 2_656 .
Au6 Au5 Cu5 Au1 -27.8(3) . .
Au6 Au5 Cu5 Au4 44.3(3) . .
Au6 Au5 Cu5 Cu12 9.5(4) . .
Au6 Au5 Cu5 S10 -27.1(5) . .
Au6 Au5 Cu5 S18 118.5(3) . .
Au6 Au5 Cu5 S11 -135.4(3) . .
Au6 Au5 Cu8 Au4 -100.16(5) . .
Au6 Au5 Cu8 Au4 -26.75(7) . 2_656
Au6 Au5 Cu8 Cu2 -136.23(14) . .
Au6 Au5 Cu8 Cu8 -66.33(15) . 2_656
Au6 Au5 Cu8 Cu10 40.76(9) . .
Au6 Au5 Cu8 S18 -175.20(16) . .
Au6 Au5 Cu8 S16 42.51(19) . .
Au6 Au5 Cu10 Au4 -70.01(5) . 2_656
Au6 Au5 Cu10 Cu8 -135.53(10) . .
Au6 Au5 Cu10 Cu16 67.09(9) . .
Au6 Au5 Cu10 S9 3.1(3) . 2_656
Au6 Au5 Cu10 S16 -137.10(18) . .
Au6 Au5 Cu10 S15 114.26(19) . .
Au6 Au5 Cu15 Au1 99.32(6) . .
Au6 Au5 Cu15 Au3 26.35(7) . .
Au6 Au5 Cu15 Cu9 63.79(12) . .
Au6 Au5 Cu15 Cu13 -36.35(15) . .
Au6 Au5 Cu15 Cu16 -43.34(9) . .
Au6 Au5 Cu15 S11 -150.75(15) . .
Au6 Au5 Cu15 S8 14.0(4) . .
Au6 Au5 Cu16 Au3 69.31(5) . .
Au6 Au5 Cu16 Cu10 -67.96(8) . .
Au6 Au5 Cu16 Cu13 124.81(16) . .
Au6 Au5 Cu16 Cu15 131.88(10) . .
Au6 Au5 Cu16 S15 -117.47(18) . .
Au6 Au5 Cu16 S13 69.9(3) . .
Au6 Cu6 S13 Cu13 -90.8(4) . .
Au6 Cu6 S13 Cu16 -9.0(2) . .
Au6 Cu6 S13 C85 103.9(15) . .
Au6 Cu10 Cu16 Au3 37.24(8) . .
Au6 Cu10 Cu16 Au5 76.15(8) . .
Au6 Cu10 Cu16 Cu13 142.7(7) . .
Au6 Cu10 Cu16 Cu15 94.34(13) . .
Au6 Cu10 Cu16 S15 -176.7(2) . .
Au6 Cu10 Cu16 S13 -60.2(4) . .
Au6 Cu10 S16 Cu2 12.0(5) . 2_656
Au6 Cu10 S16 Cu8 -63.7(3) . .
Au6 Cu10 S16 C106 -172.0(8) . .
Au6 Cu10 S15 Cu14 78.9(5) . .
Au6 Cu10 S15 Cu16 2.9(2) . .
Au6 Cu10 S15 C99 -111.8(12) . .
Au6 Cu11 Cu12 Au1 76.78(7) 2_656 .
Au6 Cu11 Cu12 Au4 38.56(8) 2_656 .
Au6 Cu11 Cu12 Cu4 172.78(13) 2_656 .
Au6 Cu11 Cu12 Cu5 97.52(11) 2_656 .
Au6 Cu11 Cu12 S9 -68.52(16) 2_656 .
Au6 Cu11 Cu12 S10 149.56(18) 2_656 .
Au6 Cu11 S4 Cu3 76.42(16) 2_656 .
Au6 Cu11 S4 Cu6 -50.17(13) 2_656 2_656
Au6 Cu11 S4 C22 -165.2(9) 2_656 .
Au6 Cu11 S7 Cu4 -79.4(3) 2_656 .
Au6 Cu11 S7 Cu9 57.2(4) 2_656 .
Au6 Cu11 S7 C43 168.2(8) 2_656 .
Au6 Cu12 S9 Cu3 -80.78(16) 2_656 .
Au6 Cu12 S9 Cu10 52.48(14) 2_656 2_656
Au6 Cu12 S9 C57 164.4(8) 2_656 .
Au6 Cu12 S10 Cu4 74.6(3) 2_656 .
Au6 Cu12 S10 Cu5 -56.5(3) 2_656 .
Au6 Cu12 S10 C64 -170.7(8) 2_656 .
Au6 Cu16 S15 Cu10 -3.0(2) . .
Au6 Cu16 S15 Cu14 -140.39(19) . .
Au6 Cu16 S15 C99 106.7(12) . .
Au6 Cu16 S13 Cu6 8.9(2) . .
Au6 Cu16 S13 Cu13 137.95(18) . .
Au6 Cu16 S13 C85 -103.0(13) . .
Au7 Cu1 S2 Cu6 150.3(2) . 2_656
Au7 Cu1 S2 Cu7 65.7(2) . 2_656
Au7 Cu1 S2 C8 -50.2(10) . .
Au7 Cu1 S3 Cu7 -71.20(19) . .
Au7 Cu1 S3 Cu9 -142.5(3) . .
Au7 Cu1 S3 C15 41.0(8) . .
Au7 Cu1 S1 C1 -108.6(9) . .
Au7 S1 C1 C6 16(2) . .
Au7 S1 C1 C2 -168.9(16) . .
Au8 Cu2 Cu8 Au4 96.20(13) . 2_656
Au8 Cu2 Cu8 Au4 144.72(9) . .
Au8 Cu2 Cu8 Au5 176.53(13) . .
Au8 Cu2 Cu8 Cu8 87.10(10) . 2_656
Au8 Cu2 Cu8 Cu10 12.7(9) . .
Au8 Cu2 Cu8 S18 -126.5(2) . .
Au8 Cu2 Cu8 S16 -2.2(2) . .
Au8 Cu2 S18 Cu5 148.3(2) . .
Au8 Cu2 S18 Cu8 65.0(2) . .
Au8 Cu2 S18 C120 -47.3(9) . .
Au8 Cu2 S17 C113 -105.1(10) . .
Au8 S17 C113 C114 18(2) . .
Au8 S17 C113 C118 -164.7(19) . .
Au9 Cu3 S4 Cu6 152.0(3) . 2_656
Au9 Cu3 S4 Cu11 72.46(19) . .
Au9 Cu3 S4 C22 -40.7(11) . .
Au9 Cu3 S9 Cu10 -150.4(3) . 2_656
Au9 Cu3 S9 Cu12 -68.29(19) . .
Au9 Cu3 S9 C57 50.8(9) . .
Au9 Cu3 S5 C29 101.8(10) . .
Au9 Cu4 Cu11 Au1 -146.21(9) . .
Au9 Cu4 Cu11 Au2 -172.09(16) . .
Au9 Cu4 Cu11 Au6 -94.65(12) . 2_656
Au9 Cu4 Cu11 Cu6 -36.2(5) . 2_656
Au9 Cu4 Cu11 Cu12 -87.90(10) . .
Au9 Cu4 Cu11 S4 1.5(2) . .
Au9 Cu4 Cu11 S7 127.1(2) . .
Au9 Cu4 Cu12 Au1 147.34(9) . .
Au9 Cu4 Cu12 Au4 172.61(16) . .
Au9 Cu4 Cu12 Au6 97.19(12) . 2_656
Au9 Cu4 Cu12 Cu5 -157.63(10) . .
Au9 Cu4 Cu12 Cu11 90.47(10) . .
Au9 Cu4 Cu12 S9 3.1(2) . .
Au9 Cu4 Cu12 S10 -121.9(2) . .
Au9 Cu4 S10 Cu5 141.6(3) . .
Au9 Cu4 S10 Cu12 65.67(19) . .
Au9 Cu4 S10 C64 -48.3(10) . .
Au9 Cu4 S7 Cu9 -138.5(3) . .
Au9 Cu4 S7 Cu11 -62.7(2) . .
Au9 Cu4 S7 C43 54.0(10) . .
Au9 Cu4 S6 C36 105.8(9) . .
Au9 S5 C29 C34 -62(2) . .
Au9 S5 C29 C30 113(2) . .
Au9 S6 C36 C41 128.0(19) . .
Au9 S6 C36 C37 -58(3) . .
Au10 Cu13 Cu15 Au1 -167.04(17) . .
Au10 Cu13 Cu15 Au3 -147.28(11) . .
Au10 Cu13 Cu15 Au5 -93.96(13) . .
Au10 Cu13 Cu15 Cu9 155.92(11) . .
Au10 Cu13 Cu15 Cu16 -87.48(12) . .
Au10 Cu13 Cu15 S11 -2.5(2) . .
Au10 Cu13 Cu15 S8 122.8(2) . .
Au10 Cu13 Cu16 Au3 149.75(11) . .
Au10 Cu13 Cu16 Au5 101.19(14) . .
Au10 Cu13 Cu16 Au6 177.77(14) . .
Au10 Cu13 Cu16 Cu10 41.1(7) . .
Au10 Cu13 Cu16 Cu15 94.23(12) . .
Au10 Cu13 Cu16 S15 5.4(3) . .
Au10 Cu13 Cu16 S13 -120.9(3) . .
Au10 Cu13 S8 Cu9 -135.1(3) . .
Au10 Cu13 S8 Cu15 -69.9(2) . .
Au10 Cu13 S8 C50 37.3(10) . .
Au10 Cu13 S13 Cu6 150.5(3) . .
Au10 Cu13 S13 Cu16 67.5(2) . .
Au10 Cu13 S13 C85 -45.1(16) . .
Au10 Cu13 S12 C78 108(2) . .
Au10 Cu14 S11 Cu5 149.8(3) . .
Au10 Cu14 S11 Cu15 65.1(2) . .
Au10 Cu14 S11 C71 -58.3(9) . .
Au10 Cu14 S15 Cu10 -140.7(4) . .
Au10 Cu14 S15 Cu16 -68.4(3) . .
Au10 Cu14 S15 C99 49.9(12) . .
Au10 Cu14 S14 C92 102.7(12) . .
Au10 S14 C92 C93 -160.2(13) . .
Au10 S14 C92 C97 17.5(18) . .
Au10 S12 C78 C83 178.2(16) . .
Au10 S12 C78 C79 6(2) . .
Cu1 Au7 Cu1 Cu7 -29.29(6) 2_656 2_656
Cu1 Au7 Cu1 S2 -71.81(18) 2_656 .
Cu1 Au7 Cu1 S3 71.61(16) 2_656 .
Cu1 Au7 Cu1 S1 -166.4(2) 2_656 .
Cu1 Au7 S1 Cu1 17.8(3) 2_656 .
Cu1 Au7 S1 C1 127.0(8) 2_656 .
Cu1 Au7 S1 C1 109.2(8) . .
Cu1 Cu7 Cu9 Au1 114.3(8) 2_656 .
Cu1 Cu7 Cu9 Au2 77.3(9) 2_656 .
Cu1 Cu7 Cu9 Au3 154.2(9) 2_656 .
Cu1 Cu7 Cu9 Cu15 173.7(8) 2_656 .
Cu1 Cu7 Cu9 S7 24.5(10) 2_656 .
Cu1 Cu7 Cu9 S3 -27.8(9) 2_656 .
Cu1 Cu7 Cu9 S8 -135.6(8) 2_656 .
Cu1 Cu7 S3 Cu1 42.0(2) 2_656 .
Cu1 Cu7 S3 Cu9 175.22(15) 2_656 .
Cu1 Cu7 S3 C15 -66.2(7) 2_656 .
Cu1 S2 C8 C9 -45(2) . .
Cu1 S2 C8 C13 137.5(18) . .
Cu1 S3 C15 C20 111.8(19) . .
Cu1 S3 C15 C16 -68.3(18) . .
Cu1 S1 C1 C6 106.2(18) . .
Cu1 S1 C1 C2 -78.3(19) . .
Cu2 Au8 Cu2 Cu8 -29.18(6) 2_656 .
Cu2 Au8 Cu2 S18 -72.34(19) 2_656 .
Cu2 Au8 Cu2 S16 71.15(17) 2_656 2_656
Cu2 Au8 Cu2 S17 -164.4(2) 2_656 .
Cu2 Au8 S17 Cu2 20.5(3) 2_656 .
Cu2 Au8 S17 C113 107.7(10) . .
Cu2 Au8 S17 C113 128.3(10) 2_656 .
Cu2 Cu8 Cu10 Au4 89.1(9) . 2_656
Cu2 Cu8 Cu10 Au5 165.6(9) . .
Cu2 Cu8 Cu10 Au6 125.9(9) . .
Cu2 Cu8 Cu10 Cu16 -174.7(9) . .
Cu2 Cu8 Cu10 S9 36.3(11) . 2_656
Cu2 Cu8 Cu10 S16 -16.4(9) . .
Cu2 Cu8 Cu10 S15 -124.8(9) . .
Cu2 Cu8 S18 Cu5 -129.2(3) . .
Cu2 Cu8 S18 C120 116.8(8) . .
Cu2 Cu8 S16 Cu2 44.5(2) . 2_656
Cu2 Cu8 S16 Cu10 177.16(16) . .
Cu2 Cu8 S16 C106 -64.4(8) . .
Cu2 S18 C120 C121 -53(2) . .
Cu2 S18 C120 C125 130.1(16) . .
Cu2 S16 C106 C111 -69.1(19) 2_656 .
Cu2 S16 C106 C107 111(2) 2_656 .
Cu2 S17 C113 C114 106(2) . .
Cu2 S17 C113 C118 -77(2) . .
Cu3 Au9 Cu4 Cu11 28.81(10) . .
Cu3 Au9 Cu4 Cu12 -29.86(10) . .
Cu3 Au9 Cu4 S10 -72.17(19) . .
Cu3 Au9 Cu4 S7 70.3(2) . .
Cu3 Au9 Cu4 S6 166.9(3) . .
Cu3 Au9 S5 C29 -107.4(9) . .
Cu3 Au9 S6 Cu4 -16.9(3) . .
Cu3 Au9 S6 C36 -126.5(8) . .
Cu3 S4 C22 C23 -141(2) . .
Cu3 S4 C22 C27 42(3) . .
Cu3 S9 C57 C58 -128.2(18) . .
Cu3 S9 C57 C62 52(2) . .
Cu3 S5 C29 C34 -144(2) . .
Cu3 S5 C29 C30 31(3) . .
Cu4 Au9 Cu3 S4 -69.83(19) . .
Cu4 Au9 Cu3 S9 70.9(2) . .
Cu4 Au9 Cu3 S5 171.2(2) . .
Cu4 Au9 S5 Cu3 -12.4(3) . .
Cu4 Au9 S5 C29 -119.8(9) . .
Cu4 Au9 S6 C36 -109.7(9) . .
Cu4 Cu11 Cu12 Au1 -96.00(11) . .
Cu4 Cu11 Cu12 Au4 -134.22(13) . .
Cu4 Cu11 Cu12 Au6 -172.78(13) . 2_656
Cu4 Cu11 Cu12 Cu5 -75.26(12) . .
Cu4 Cu11 Cu12 S9 118.70(18) . .
Cu4 Cu11 Cu12 S10 -23.22(16) . .
Cu4 Cu11 S4 Cu3 -40.4(2) . .
Cu4 Cu11 S4 Cu6 -166.95(15) . 2_656
Cu4 Cu11 S4 C22 78.0(9) . .
Cu4 Cu11 S7 Cu9 136.6(3) . .
Cu4 Cu11 S7 C43 -112.4(8) . .
Cu4 Cu12 S9 Cu3 34.2(2) . .
Cu4 Cu12 S9 Cu10 167.51(16) . 2_656
Cu4 Cu12 S9 C57 -80.6(8) . .
Cu4 Cu12 S10 Cu5 -131.1(2) . .
Cu4 Cu12 S10 C64 114.8(9) . .
Cu4 S10 C64 C65 -133.9(18) . .
Cu4 S10 C64 C69 43(2) . .
Cu4 S7 C43 C44 -131.5(19) . .
Cu4 S7 C43 C48 56(2) . .
Cu4 S6 C36 C41 35(2) . .
Cu4 S6 C36 C37 -151(3) . .
Cu5 Au1 Au2 Au2 -33.5(3) . 2_656
Cu5 Au1 Au2 Au3 -69.9(3) . .
Cu5 Au1 Au2 Au3 30.0(3) . 2_656
Cu5 Au1 Au2 Au6 67.2(3) . 2_656
Cu5 Au1 Au2 Cu6 93.8(3) . 2_656
Cu5 Au1 Au2 Cu7 -9.3(4) . 2_656
Cu5 Au1 Au2 Cu7 -97.1(3) . .
Cu5 Au1 Au2 Cu9 -138.7(3) . .
Cu5 Au1 Au2 Cu11 136.7(3) . .
Cu5 Au1 Au3 Au2 165.93(8) . .
Cu5 Au1 Au3 Au2 128.32(8) . 2_656
Cu5 Au1 Au3 Au5 27.35(7) . .
Cu5 Au1 Au3 Au6 63.92(8) . .
Cu5 Au1 Au3 Cu6 91.0(3) . .
Cu5 Au1 Au3 Cu7 -167.81(10) . .
Cu5 Au1 Au3 Cu9 -124.28(10) . .
Cu5 Au1 Au3 Cu15 -44.98(11) . .
Cu5 Au1 Au3 Cu16 2.00(11) . .
Cu5 Au1 Au4 Au4 -108.14(8) . 2_656
Cu5 Au1 Au4 Au5 -70.18(7) . .
Cu5 Au1 Au4 Au5 -169.98(8) . 2_656
Cu5 Au1 Au4 Au6 151.29(8) . 2_656
Cu5 Au1 Au4 Cu8 -137.6(3) . 2_656
Cu5 Au1 Au4 Cu8 -47.08(10) . .
Cu5 Au1 Au4 Cu10 126.88(10) . 2_656
Cu5 Au1 Au4 Cu12 81.63(10) . .
Cu5 Au1 Au5 Au3 -150.84(8) . .
Cu5 Au1 Au5 Au4 70.77(8) . .
Cu5 Au1 Au5 Au4 109.73(8) . 2_656
Cu5 Au1 Au5 Au6 172.72(8) . .
Cu5 Au1 Au5 Cu8 47.47(11) . .
Cu5 Au1 Au5 Cu10 138.7(3) . .
Cu5 Au1 Au5 Cu15 -84.21(11) . .
Cu5 Au1 Au5 Cu16 -122.71(11) . .
Cu5 Au1 Cu9 Au2 168.14(9) . .
Cu5 Au1 Cu9 Au3 95.90(11) . .
Cu5 Au1 Cu9 Cu7 133.51(12) . .
Cu5 Au1 Cu9 Cu15 30.62(13) . .
Cu5 Au1 Cu9 S7 -81.64(19) . .
Cu5 Au1 Cu9 S3 177.7(2) . .
Cu5 Au1 Cu9 S8 27.9(2) . .
Cu5 Au1 Cu11 Au2 -167.82(10) . .
Cu5 Au1 Cu11 Au6 -96.05(11) . 2_656
Cu5 Au1 Cu11 Cu4 32.10(15) . .
Cu5 Au1 Cu11 Cu6 -131.67(12) . 2_656
Cu5 Au1 Cu11 Cu12 -30.03(13) . .
Cu5 Au1 Cu11 S4 -90.0(3) . .
Cu5 Au1 Cu11 S7 80.71(19) . .
Cu5 Au1 Cu12 Au4 -66.91(8) . .
Cu5 Au1 Cu12 Au6 -137.66(9) . 2_656
Cu5 Au1 Cu12 Cu4 93.40(11) . .
Cu5 Au1 Cu12 Cu11 155.55(11) . .
Cu5 Au1 Cu12 S9 -140.6(3) . .
Cu5 Au1 Cu12 S10 46.54(16) . .
Cu5 Au1 Cu15 Au3 136.95(9) . .
Cu5 Au1 Cu15 Au5 64.95(7) . .
Cu5 Au1 Cu15 Cu9 -155.89(10) . .
Cu5 Au1 Cu15 Cu13 158.8(2) . .
Cu5 Au1 Cu15 Cu16 95.64(13) . .
Cu5 Au1 Cu15 S11 -6.92(16) . .
Cu5 Au1 Cu15 S8 -153.0(2) . .
Cu5 Au4 Au5 Au1 -68.34(8) . .
Cu5 Au4 Au5 Au3 -105.78(8) . .
Cu5 Au4 Au5 Au4 154.31(8) . 2_656
Cu5 Au4 Au5 Au6 -169.00(8) . .
Cu5 Au4 Au5 Cu8 87.24(10) . .
Cu5 Au4 Au5 Cu10 125.81(11) . .
Cu5 Au4 Au5 Cu15 -45.02(10) . .
Cu5 Au4 Au5 Cu16 -143.8(4) . .
Cu5 Au4 Cu8 Au4 -135.73(9) . 2_656
Cu5 Au4 Cu8 Au5 -63.67(8) . .
Cu5 Au4 Cu8 Cu2 89.62(10) . .
Cu5 Au4 Cu8 Cu8 156.55(11) . 2_656
Cu5 Au4 Cu8 Cu10 -97.46(13) . .
Cu5 Au4 Cu8 S18 40.90(16) . .
Cu5 Au4 Cu8 S16 -150.7(4) . .
Cu5 Au4 Cu12 Au1 64.75(8) . .
Cu5 Au4 Cu12 Au6 136.32(9) . 2_656
Cu5 Au4 Cu12 Cu4 36.48(17) . .
Cu5 Au4 Cu12 Cu11 100.07(13) . .
Cu5 Au4 Cu12 S9 -152.68(19) . .
Cu5 Au4 Cu12 S10 -6.94(17) . .
Cu5 Au5 Au6 Au1 -38.3(3) . 2_656
Cu5 Au5 Au6 Au2 24.1(3) . 2_656
Cu5 Au5 Au6 Au3 61.4(3) . .
Cu5 Au5 Au6 Au4 -77.2(3) . 2_656
Cu5 Au5 Au6 Cu6 87.8(3) . .
Cu5 Au5 Au6 Cu10 -146.4(3) . .
Cu5 Au5 Au6 Cu11 -8.9(4) . 2_656
Cu5 Au5 Au6 Cu12 -102.1(3) . 2_656
Cu5 Au5 Au6 Cu16 134.1(3) . .
Cu5 Au5 Cu8 Au4 138.02(9) . 2_656
Cu5 Au5 Cu8 Au4 64.62(8) . .
Cu5 Au5 Cu8 Cu2 28.54(16) . .
Cu5 Au5 Cu8 Cu8 98.45(15) . 2_656
Cu5 Au5 Cu8 Cu10 -154.46(11) . .
Cu5 Au5 Cu8 S18 -10.42(18) . .
Cu5 Au5 Cu8 S16 -152.7(2) . .
Cu5 Au5 Cu10 Au4 98.96(12) . 2_656
Cu5 Au5 Cu10 Au6 168.98(10) . .
Cu5 Au5 Cu10 Cu8 33.45(14) . .
Cu5 Au5 Cu10 Cu16 -123.94(13) . .
Cu5 Au5 Cu10 S9 172.0(3) . 2_656
Cu5 Au5 Cu10 S16 31.9(2) . .
Cu5 Au5 Cu10 S15 -76.8(2) . .
Cu5 Au5 Cu15 Au1 -64.71(8) . .
Cu5 Au5 Cu15 Au3 -137.68(10) . .
Cu5 Au5 Cu15 Cu9 -100.25(13) . .
Cu5 Au5 Cu15 Cu13 159.62(16) . .
Cu5 Au5 Cu15 Cu16 152.63(12) . .
Cu5 Au5 Cu15 S11 45.22(16) . .
Cu5 Au5 Cu15 S8 -150.0(4) . .
Cu5 Au5 Cu16 Au3 -96.72(12) . .
Cu5 Au5 Cu16 Au6 -166.03(10) . .
Cu5 Au5 Cu16 Cu10 126.01(13) . .
Cu5 Au5 Cu16 Cu13 -41.2(2) . .
Cu5 Au5 Cu16 Cu15 -34.15(14) . .
Cu5 Au5 Cu16 S15 76.5(2) . .
Cu5 Au5 Cu16 S13 -96.1(4) . .
Cu5 Cu12 S9 Cu3 176.5(3) . .
Cu5 Cu12 S9 Cu10 -50.2(4) . 2_656
Cu5 Cu12 S9 C57 61.7(9) . .
Cu5 Cu12 S10 Cu4 131.1(2) . .
Cu5 Cu12 S10 C64 -114.1(8) . .
Cu5 S10 C64 C65 38(2) . .
Cu5 S10 C64 C69 -145.3(17) . .
Cu5 S18 C120 C121 114.2(19) . .
Cu5 S18 C120 C125 -63.1(18) . .
Cu5 S11 C71 C76 -71(2) . .
Cu5 S11 C71 C72 106(2) . .
Cu6 Au2 Au3 Au1 -66.8(2) 2_656 .
Cu6 Au2 Au3 Au2 71.7(2) 2_656 2_656
Cu6 Au2 Au3 Au5 -30.3(3) 2_656 .
Cu6 Au2 Au3 Au6 33.0(3) 2_656 .
Cu6 Au2 Au3 Cu6 96.2(2) 2_656 .
Cu6 Au2 Au3 Cu7 142.4(3) 2_656 .
Cu6 Au2 Au3 Cu9 -137.8(3) 2_656 .
Cu6 Au2 Au3 Cu15 -95.4(3) 2_656 .
Cu6 Au2 Au3 Cu16 -10.0(4) 2_656 .
Cu6 Au2 Cu7 Au2 -96.80(11) 2_656 2_656
Cu6 Au2 Cu7 Au3 -166.31(10) 2_656 .
Cu6 Au2 Cu7 Cu1 -42.38(18) 2_656 2_656
Cu6 Au2 Cu7 Cu7 -32.50(14) 2_656 2_656
Cu6 Au2 Cu7 Cu9 127.37(12) 2_656 .
Cu6 Au2 Cu7 S2 -100.1(3) 2_656 2_656
Cu6 Au2 Cu7 S3 75.30(18) 2_656 .
Cu6 Au2 Cu9 Au1 93.63(11) 2_656 .
Cu6 Au2 Cu9 Au3 165.00(10) 2_656 .
Cu6 Au2 Cu9 Cu7 -127.90(13) 2_656 .
Cu6 Au2 Cu9 Cu15 129.48(12) 2_656 .
Cu6 Au2 Cu9 S7 25.0(2) 2_656 .
Cu6 Au2 Cu9 S3 -79.87(17) 2_656 .
Cu6 Au2 Cu9 S8 173.0(3) 2_656 .
Cu6 Au2 Cu11 Au1 137.06(9) 2_656 .
Cu6 Au2 Cu11 Au6 65.05(8) 2_656 2_656
Cu6 Au2 Cu11 Cu4 166.2(2) 2_656 .
Cu6 Au2 Cu11 Cu12 100.87(13) 2_656 .
Cu6 Au2 Cu11 S4 -7.85(18) 2_656 .
Cu6 Au2 Cu11 S7 -152.1(2) 2_656 .
Cu6 Au3 Au5 Au1 -164.63(8) . .
Cu6 Au3 Au5 Au4 -62.13(8) . 2_656
Cu6 Au3 Au5 Au4 -126.92(7) . .
Cu6 Au3 Au5 Au6 -25.57(7) . .
Cu6 Au3 Au5 Cu5 168.65(10) . .
Cu6 Au3 Au5 Cu8 -84.3(3) . .
Cu6 Au3 Au5 Cu10 0.85(11) . .
Cu6 Au3 Au5 Cu15 125.53(11) . .
Cu6 Au3 Au5 Cu16 44.32(10) . .
Cu6 Au3 Au6 Au1 -106.63(8) . 2_656
Cu6 Au3 Au6 Au2 -70.12(8) . 2_656
Cu6 Au3 Au6 Au4 -170.41(8) . 2_656
Cu6 Au3 Au6 Au5 152.09(8) . .
Cu6 Au3 Au6 Cu10 126.60(10) . .
Cu6 Au3 Au6 Cu11 -44.77(10) . 2_656
Cu6 Au3 Au6 Cu12 -131.1(3) . 2_656
Cu6 Au3 Au6 Cu16 85.50(11) . .
Cu6 Au3 Cu7 Au2 64.14(8) . 2_656
Cu6 Au3 Cu7 Au2 137.03(9) . .
Cu6 Au3 Cu7 Cu1 29.52(15) . 2_656
Cu6 Au3 Cu7 Cu7 97.68(14) . 2_656
Cu6 Au3 Cu7 Cu9 -155.72(11) . .
Cu6 Au3 Cu7 S2 -10.39(17) . 2_656
Cu6 Au3 Cu7 S3 -154.0(2) . .
Cu6 Au3 Cu9 Au1 167.64(10) . .
Cu6 Au3 Cu9 Au2 97.66(12) . .
Cu6 Au3 Cu9 Cu7 32.28(14) . .
Cu6 Au3 Cu9 Cu15 -125.17(13) . .
Cu6 Au3 Cu9 S7 171.3(3) . .
Cu6 Au3 Cu9 S3 30.7(2) . .
Cu6 Au3 Cu9 S8 -77.3(2) . .
Cu6 Au3 Cu15 Au1 -165.44(10) . .
Cu6 Au3 Cu15 Au5 -96.05(12) . .
Cu6 Au3 Cu15 Cu9 127.19(13) . .
Cu6 Au3 Cu15 Cu13 28.55(16) . .
Cu6 Au3 Cu15 Cu16 -33.42(14) . .
Cu6 Au3 Cu15 S11 -91.3(3) . .
Cu6 Au3 Cu15 S8 76.8(2) . .
Cu6 Au3 Cu16 Au5 -136.89(9) . .
Cu6 Au3 Cu16 Au6 -64.05(8) . .
Cu6 Au3 Cu16 Cu10 -100.21(12) . .
Cu6 Au3 Cu16 Cu13 92.05(12) . .
Cu6 Au3 Cu16 Cu15 153.84(11) . .
Cu6 Au3 Cu16 S15 -148.3(4) . .
Cu6 Au3 Cu16 S13 43.48(19) . .
Cu6 Au6 Cu10 Au4 168.40(10) . 2_656
Cu6 Au6 Cu10 Au5 95.77(11) . .
Cu6 Au6 Cu10 Cu8 133.73(12) . .
Cu6 Au6 Cu10 Cu16 30.32(13) . .
Cu6 Au6 Cu10 S9 -82.14(19) . 2_656
Cu6 Au6 Cu10 S16 178.6(2) . .
Cu6 Au6 Cu10 S15 27.7(2) . .
Cu6 Au6 Cu16 Au3 64.67(8) . .
Cu6 Au6 Cu16 Au5 136.45(9) . .
Cu6 Au6 Cu16 Cu10 -156.92(10) . .
Cu6 Au6 Cu16 Cu13 33.05(17) . .
Cu6 Au6 Cu16 Cu15 95.53(13) . .
Cu6 Au6 Cu16 S15 -154.1(2) . .
Cu6 Au6 Cu16 S13 -8.2(2) . .
Cu6 Cu11 Cu12 Au1 97.66(11) 2_656 .
Cu6 Cu11 Cu12 Au4 59.44(14) 2_656 .
Cu6 Cu11 Cu12 Au6 20.88(9) 2_656 2_656
Cu6 Cu11 Cu12 Cu4 -166.34(14) 2_656 .
Cu6 Cu11 Cu12 Cu5 118.40(12) 2_656 .
Cu6 Cu11 Cu12 S9 -47.65(19) 2_656 .
Cu6 Cu11 Cu12 S10 170.44(17) 2_656 .
Cu6 Cu11 S4 Cu3 126.6(2) 2_656 .
Cu6 Cu11 S4 C22 -115.0(9) 2_656 .
Cu6 Cu11 S7 Cu4 171.1(3) 2_656 .
Cu6 Cu11 S7 Cu9 -52.3(4) 2_656 .
Cu6 Cu11 S7 C43 58.7(9) 2_656 .
Cu6 S4 C22 C23 28(3) 2_656 .
Cu6 S4 C22 C27 -150(2) 2_656 .
Cu6 S2 C8 C9 116.9(19) 2_656 .
Cu6 S2 C8 C13 -60(2) 2_656 .
Cu6 S13 C85 C86 -77.4(18) . .
Cu6 S13 C85 C90 99(2) . .
Cu7 Au2 Au3 Au1 150.75(7) . .
Cu7 Au2 Au3 Au1 -164.13(7) 2_656 .
Cu7 Au2 Au3 Au2 -25.58(7) 2_656 2_656
Cu7 Au2 Au3 Au2 -70.69(7) . 2_656
Cu7 Au2 Au3 Au5 -172.76(8) . .
Cu7 Au2 Au3 Au5 -127.64(7) 2_656 .
Cu7 Au2 Au3 Au6 -109.41(8) . .
Cu7 Au2 Au3 Au6 -64.29(8) 2_656 .
Cu7 Au2 Au3 Cu6 -46.25(10) . .
Cu7 Au2 Au3 Cu6 -1.13(10) 2_656 .
Cu7 Au2 Au3 Cu7 45.12(11) 2_656 .
Cu7 Au2 Au3 Cu9 124.91(10) 2_656 .
Cu7 Au2 Au3 Cu9 79.79(10) . .
Cu7 Au2 Au3 Cu15 167.31(10) 2_656 .
Cu7 Au2 Au3 Cu15 122.19(11) . .
Cu7 Au2 Au3 Cu16 -107.3(2) 2_656 .
Cu7 Au2 Au3 Cu16 -152.4(2) . .
Cu7 Au2 Cu7 Au2 -64.30(9) 2_656 2_656
Cu7 Au2 Cu7 Au3 -133.82(10) 2_656 .
Cu7 Au2 Cu7 Cu1 -9.88(12) 2_656 2_656
Cu7 Au2 Cu7 Cu9 159.87(11) 2_656 .
Cu7 Au2 Cu7 S2 -67.6(3) 2_656 2_656
Cu7 Au2 Cu7 S3 107.79(16) 2_656 .
Cu7 Au2 Cu9 Au1 -162.80(9) 2_656 .
Cu7 Au2 Cu9 Au1 -138.47(9) . .
Cu7 Au2 Cu9 Au3 -67.10(8) . .
Cu7 Au2 Cu9 Au3 -91.43(11) 2_656 .
Cu7 Au2 Cu9 Cu7 -24.33(14) 2_656 .
Cu7 Au2 Cu9 Cu15 -102.62(12) . .
Cu7 Au2 Cu9 Cu15 -126.95(12) 2_656 .
Cu7 Au2 Cu9 S7 128.57(18) 2_656 .
Cu7 Au2 Cu9 S7 152.90(19) . .
Cu7 Au2 Cu9 S3 48.03(15) . .
Cu7 Au2 Cu9 S3 23.70(18) 2_656 .
Cu7 Au2 Cu9 S8 -59.1(3) . .
Cu7 Au2 Cu9 S8 -83.4(3) 2_656 .
Cu7 Au2 Cu11 Au1 166.53(11) 2_656 .
Cu7 Au2 Cu11 Au1 -94.36(12) . .
Cu7 Au2 Cu11 Au6 94.51(12) 2_656 2_656
Cu7 Au2 Cu11 Au6 -166.38(10) . 2_656
Cu7 Au2 Cu11 Cu4 -164.37(15) 2_656 .
Cu7 Au2 Cu11 Cu4 -65.3(2) . .
Cu7 Au2 Cu11 Cu6 29.47(14) 2_656 2_656
Cu7 Au2 Cu11 Cu6 128.58(13) . 2_656
Cu7 Au2 Cu11 Cu12 130.34(13) 2_656 .
Cu7 Au2 Cu11 Cu12 -130.55(13) . .
Cu7 Au2 Cu11 S4 120.73(19) . .
Cu7 Au2 Cu11 S4 21.6(2) 2_656 .
Cu7 Au2 Cu11 S7 -122.6(2) 2_656 .
Cu7 Au2 Cu11 S7 -23.5(2) . .
Cu7 Au3 Au5 Au1 -58.2(2) . .
Cu7 Au3 Au5 Au4 -20.5(2) . .
Cu7 Au3 Au5 Au4 44.3(2) . 2_656
Cu7 Au3 Au5 Au6 80.9(2) . .
Cu7 Au3 Au5 Cu5 -84.9(2) . .
Cu7 Au3 Au5 Cu8 22.1(4) . .
Cu7 Au3 Au5 Cu10 107.3(2) . .
Cu7 Au3 Au5 Cu15 -128.0(2) . .
Cu7 Au3 Au5 Cu16 150.8(2) . .
Cu7 Au3 Au6 Au1 -60.30(8) . 2_656
Cu7 Au3 Au6 Au2 -23.79(8) . 2_656
Cu7 Au3 Au6 Au4 -124.08(8) . 2_656
Cu7 Au3 Au6 Au5 -161.58(8) . .
Cu7 Au3 Au6 Cu6 46.33(10) . .
Cu7 Au3 Au6 Cu10 172.93(10) . .
Cu7 Au3 Au6 Cu11 1.56(11) . 2_656
Cu7 Au3 Au6 Cu12 -84.8(3) . 2_656
Cu7 Au3 Au6 Cu16 131.83(11) . .
Cu7 Au3 Cu6 Au2 -64.60(7) . 2_656
Cu7 Au3 Cu6 Au6 -137.17(9) . .
Cu7 Au3 Cu6 Cu11 -100.08(12) . 2_656
Cu7 Au3 Cu6 S4 -136.5(3) . 2_656
Cu7 Au3 Cu6 S2 10.00(16) . 2_656
Cu7 Au3 Cu6 S13 117.6(2) . .
Cu7 Au3 Cu9 Au1 135.36(9) . .
Cu7 Au3 Cu9 Au2 65.38(8) . .
Cu7 Au3 Cu9 Cu15 -157.45(11) . .
Cu7 Au3 Cu9 S7 139.0(3) . .
Cu7 Au3 Cu9 S3 -1.54(16) . .
Cu7 Au3 Cu9 S8 -109.53(18) . .
Cu7 Au3 Cu15 Au1 93.88(11) . .
Cu7 Au3 Cu15 Au5 163.27(9) . .
Cu7 Au3 Cu15 Cu9 26.51(13) . .
Cu7 Au3 Cu15 Cu13 -72.13(14) . .
Cu7 Au3 Cu15 Cu16 -134.10(12) . .
Cu7 Au3 Cu15 S11 168.1(3) . .
Cu7 Au3 Cu15 S8 -23.9(2) . .
Cu7 Au3 Cu16 Au5 -167.94(11) . .
Cu7 Au3 Cu16 Au6 -95.10(13) . .
Cu7 Au3 Cu16 Cu10 -131.26(13) . .
Cu7 Au3 Cu16 Cu13 61.01(16) . .
Cu7 Au3 Cu16 Cu15 122.79(14) . .
Cu7 Au3 Cu16 S15 -179.4(3) . .
Cu7 Au3 Cu16 S13 12.4(2) . .
Cu7 Cu1 S2 Cu6 84.7(3) 2_656 2_656
Cu7 Cu1 S2 C8 -115.8(10) 2_656 .
Cu7 Cu1 S3 Cu7 22.59(19) 2_656 .
Cu7 Cu1 S3 Cu9 -48.7(3) 2_656 .
Cu7 Cu1 S3 C15 134.8(7) 2_656 .
Cu7 Cu1 S1 Au7 -54.9(2) 2_656 .
Cu7 Cu1 S1 C1 -163.5(8) 2_656 .
Cu7 Cu7 Cu9 Au1 55.23(13) 2_656 .
Cu7 Cu7 Cu9 Au2 18.32(8) 2_656 .
Cu7 Cu7 Cu9 Au3 95.16(9) 2_656 .
Cu7 Cu7 Cu9 Cu15 114.66(12) 2_656 .
Cu7 Cu7 Cu9 S7 -34.5(4) 2_656 .
Cu7 Cu7 Cu9 S3 -86.8(2) 2_656 .
Cu7 Cu7 Cu9 S8 165.36(17) 2_656 .
Cu7 Cu7 S3 Cu1 -23.10(18) 2_656 .
Cu7 Cu7 S3 Cu9 110.17(13) 2_656 .
Cu7 Cu7 S3 C15 -131.3(7) 2_656 .
Cu7 Cu9 Cu15 Au1 -96.29(11) . .
Cu7 Cu9 Cu15 Au3 -19.85(10) . .
Cu7 Cu9 Cu15 Au5 -59.48(14) . .
Cu7 Cu9 Cu15 Cu13 56.74(14) . .
Cu7 Cu9 Cu15 Cu16 -1.79(17) . .
Cu7 Cu9 Cu15 S11 -158.9(3) . .
Cu7 Cu9 Cu15 S8 87.1(2) . .
Cu7 Cu9 S7 Cu4 122.9(4) . .
Cu7 Cu9 S7 Cu11 47.2(4) . .
Cu7 Cu9 S7 C43 -69.5(10) . .
Cu7 Cu9 S3 Cu1 76.2(3) . .
Cu7 Cu9 S3 C15 -107.6(9) . .
Cu7 Cu9 S8 Cu13 -39.0(4) . .
Cu7 Cu9 S8 Cu15 -106.47(17) . .
Cu7 Cu9 S8 C50 148.7(10) . .
Cu7 S2 C8 C9 -142.5(18) 2_656 .
Cu7 S2 C8 C13 40(2) 2_656 .
Cu7 S3 C15 C20 -152.8(19) . .
Cu7 S3 C15 C16 27.1(19) . .
Cu8 Au4 Au5 Au1 164.37(8) 2_656 .
Cu8 Au4 Au5 Au1 -155.58(8) . .
Cu8 Au4 Au5 Au3 166.97(8) . .
Cu8 Au4 Au5 Au3 126.93(8) 2_656 .
Cu8 Au4 Au5 Au4 67.07(7) . 2_656
Cu8 Au4 Au5 Au4 27.02(8) 2_656 2_656
Cu8 Au4 Au5 Au6 103.75(8) . .
Cu8 Au4 Au5 Au6 63.70(9) 2_656 .
Cu8 Au4 Au5 Cu5 -87.24(10) . .
Cu8 Au4 Au5 Cu5 -127.29(11) 2_656 .
Cu8 Au4 Au5 Cu8 -40.05(12) 2_656 .
Cu8 Au4 Au5 Cu10 -1.48(11) 2_656 .
Cu8 Au4 Au5 Cu10 38.56(10) . .
Cu8 Au4 Au5 Cu15 -132.26(10) . .
Cu8 Au4 Au5 Cu15 -172.31(10) 2_656 .
Cu8 Au4 Au5 Cu16 88.9(4) 2_656 .
Cu8 Au4 Au5 Cu16 128.9(4) . .
Cu8 Au4 Cu5 Au1 135.92(9) . .
Cu8 Au4 Cu5 Au1 165.73(10) 2_656 .
Cu8 Au4 Cu5 Au5 94.08(12) 2_656 .
Cu8 Au4 Cu5 Au5 64.27(8) . .
Cu8 Au4 Cu5 Cu12 -157.40(11) . .
Cu8 Au4 Cu5 Cu12 -127.59(13) 2_656 .
Cu8 Au4 Cu5 S10 -150.90(18) . .
Cu8 Au4 Cu5 S10 -121.09(18) 2_656 .
Cu8 Au4 Cu5 S18 -10.3(2) 2_656 .
Cu8 Au4 Cu5 S18 -40.07(16) . .
Cu8 Au4 Cu5 S11 64.8(3) . .
Cu8 Au4 Cu5 S11 94.6(3) 2_656 .
Cu8 Au4 Cu8 Au4 67.72(10) 2_656 2_656
Cu8 Au4 Cu8 Au5 139.78(11) 2_656 .
Cu8 Au4 Cu8 Cu2 -66.94(9) 2_656 .
Cu8 Au4 Cu8 Cu10 105.99(15) 2_656 .
Cu8 Au4 Cu8 S18 -115.65(16) 2_656 .
Cu8 Au4 Cu8 S16 52.8(4) 2_656 .
Cu8 Au4 Cu12 Au1 -166.78(11) 2_656 .
Cu8 Au4 Cu12 Au1 95.80(13) . .
Cu8 Au4 Cu12 Au6 167.37(11) . 2_656
Cu8 Au4 Cu12 Au6 -95.21(12) 2_656 2_656
Cu8 Au4 Cu12 Cu4 67.5(2) . .
Cu8 Au4 Cu12 Cu4 164.95(16) 2_656 .
Cu8 Au4 Cu12 Cu5 31.05(15) . .
Cu8 Au4 Cu12 Cu5 128.47(13) 2_656 .
Cu8 Au4 Cu12 Cu11 -131.46(13) 2_656 .
Cu8 Au4 Cu12 Cu11 131.12(14) . .
Cu8 Au4 Cu12 S9 -24.2(2) 2_656 .
Cu8 Au4 Cu12 S9 -121.63(19) . .
Cu8 Au4 Cu12 S10 121.53(19) 2_656 .
Cu8 Au4 Cu12 S10 24.1(2) . .
Cu8 Au5 Au6 Au1 65.08(8) . 2_656
Cu8 Au5 Au6 Au2 127.45(8) . 2_656
Cu8 Au5 Au6 Au3 164.78(8) . .
Cu8 Au5 Au6 Au4 26.16(8) . 2_656
Cu8 Au5 Au6 Cu6 -168.78(10) . .
Cu8 Au5 Au6 Cu10 -42.97(10) . .
Cu8 Au5 Au6 Cu11 94.5(3) . 2_656
Cu8 Au5 Au6 Cu12 1.29(11) . 2_656
Cu8 Au5 Au6 Cu16 -122.48(11) . .
Cu8 Au5 Cu5 Au1 -136.12(9) . .
Cu8 Au5 Cu5 Au4 -64.03(8) . .
Cu8 Au5 Cu5 Cu12 -98.88(12) . .
Cu8 Au5 Cu5 S10 -135.5(3) . .
Cu8 Au5 Cu5 S18 10.19(17) . .
Cu8 Au5 Cu5 S11 116.27(17) . .
Cu8 Au5 Cu10 Au4 65.52(8) . 2_656
Cu8 Au5 Cu10 Au6 135.53(10) . .
Cu8 Au5 Cu10 Cu16 -157.38(12) . .
Cu8 Au5 Cu10 S9 138.6(3) . 2_656
Cu8 Au5 Cu10 S16 -1.57(16) . .
Cu8 Au5 Cu10 S15 -110.2(2) . .
Cu8 Au5 Cu15 Au1 -94.82(13) . .
Cu8 Au5 Cu15 Au3 -167.79(11) . .
Cu8 Au5 Cu15 Cu9 -130.36(14) . .
Cu8 Au5 Cu15 Cu13 129.51(15) . .
Cu8 Au5 Cu15 Cu16 122.52(15) . .
Cu8 Au5 Cu15 S11 15.1(2) . .
Cu8 Au5 Cu15 S8 179.8(3) . .
Cu8 Au5 Cu16 Au3 163.52(9) . .
Cu8 Au5 Cu16 Au6 94.21(11) . .
Cu8 Au5 Cu16 Cu10 26.26(13) . .
Cu8 Au5 Cu16 Cu13 -140.98(14) . .
Cu8 Au5 Cu16 Cu15 -133.91(12) . .
Cu8 Au5 Cu16 S15 -23.3(2) . .
Cu8 Au5 Cu16 S13 164.1(3) . .
Cu8 Cu2 S18 Cu5 83.3(3) . .
Cu8 Cu2 S18 C120 -112.4(9) . .
Cu8 Cu2 S17 Au8 -57.6(3) . .
Cu8 Cu2 S17 C113 -162.7(9) . .
Cu8 Cu8 Cu10 Au4 18.67(8) 2_656 2_656
Cu8 Cu8 Cu10 Au5 95.17(9) 2_656 .
Cu8 Cu8 Cu10 Au6 55.43(13) 2_656 .
Cu8 Cu8 Cu10 Cu16 114.80(13) 2_656 .
Cu8 Cu8 Cu10 S9 -34.2(4) 2_656 2_656
Cu8 Cu8 Cu10 S16 -86.8(2) 2_656 .
Cu8 Cu8 Cu10 S15 164.8(2) 2_656 .
Cu8 Cu8 S18 Cu2 31.19(18) 2_656 .
Cu8 Cu8 S18 Cu5 -97.97(16) 2_656 .
Cu8 Cu8 S18 C120 148.0(8) 2_656 .
Cu8 Cu8 S16 Cu2 -21.93(18) 2_656 2_656
Cu8 Cu8 S16 Cu10 110.75(13) 2_656 .
Cu8 Cu8 S16 C106 -130.8(8) 2_656 .
Cu8 Cu10 Cu16 Au3 -59.10(15) . .
Cu8 Cu10 Cu16 Au5 -20.18(10) . .
Cu8 Cu10 Cu16 Au6 -96.33(12) . .
Cu8 Cu10 Cu16 Cu13 46.4(7) . .
Cu8 Cu10 Cu16 Cu15 -1.99(18) . .
Cu8 Cu10 Cu16 S15 87.0(2) . .
Cu8 Cu10 Cu16 S13 -156.6(4) . .
Cu8 Cu10 S16 Cu2 75.7(3) . 2_656
Cu8 Cu10 S16 C106 -108.3(8) . .
Cu8 Cu10 S15 Cu14 -30.9(5) . .
Cu8 Cu10 S15 Cu16 -106.94(18) . .
Cu8 Cu10 S15 C99 138.4(12) . .
Cu8 S18 C120 C121 -146.8(17) . .
Cu8 S18 C120 C125 36.0(19) . .
Cu8 S16 C106 C111 27(2) . .
Cu8 S16 C106 C107 -153(2) . .
Cu9 Au1 Au2 Au2 105.23(8) . 2_656
Cu9 Au1 Au2 Au3 168.77(8) . 2_656
Cu9 Au1 Au2 Au3 68.85(7) . .
Cu9 Au1 Au2 Au6 -154.08(8) . 2_656
Cu9 Au1 Au2 Cu6 -127.50(10) . 2_656
Cu9 Au1 Au2 Cu7 41.60(10) . .
Cu9 Au1 Au2 Cu7 129.4(3) . 2_656
Cu9 Au1 Au2 Cu11 -84.60(11) . .
Cu9 Au1 Au3 Au2 -107.40(8) . 2_656
Cu9 Au1 Au3 Au2 -69.78(7) . .
Cu9 Au1 Au3 Au5 151.64(8) . .
Cu9 Au1 Au3 Au6 -171.79(8) . .
Cu9 Au1 Au3 Cu6 -144.8(3) . .
Cu9 Au1 Au3 Cu7 -43.53(10) . .
Cu9 Au1 Au3 Cu15 79.30(11) . .
Cu9 Au1 Au3 Cu16 126.29(10) . .
Cu9 Au1 Au4 Au4 28.4(3) . 2_656
Cu9 Au1 Au4 Au5 -33.4(3) . 2_656
Cu9 Au1 Au4 Au5 66.4(3) . .
Cu9 Au1 Au4 Au6 -72.1(3) . 2_656
Cu9 Au1 Au4 Cu5 136.6(3) . .
Cu9 Au1 Au4 Cu8 89.5(3) . .
Cu9 Au1 Au4 Cu8 -1.0(4) . 2_656
Cu9 Au1 Au4 Cu10 -96.5(3) . 2_656
Cu9 Au1 Au4 Cu12 -141.8(3) . .
Cu9 Au1 Au5 Au3 -26.21(7) . .
Cu9 Au1 Au5 Au4 -125.65(7) . 2_656
Cu9 Au1 Au5 Au4 -164.61(7) . .
Cu9 Au1 Au5 Au6 -62.65(8) . .
Cu9 Au1 Au5 Cu5 124.62(11) . .
Cu9 Au1 Au5 Cu8 172.09(10) . .
Cu9 Au1 Au5 Cu10 -96.7(3) . .
Cu9 Au1 Au5 Cu15 40.42(10) . .
Cu9 Au1 Au5 Cu16 1.92(11) . .
Cu9 Au1 Cu5 Au4 -166.07(9) . .
Cu9 Au1 Cu5 Au5 -95.91(11) . .
Cu9 Au1 Cu5 Cu12 128.36(12) . .
Cu9 Au1 Cu5 S10 84.47(18) . .
Cu9 Au1 Cu5 S18 -159.6(3) . .
Cu9 Au1 Cu5 S11 -22.7(2) . .
Cu9 Au1 Cu11 Au2 64.80(7) . .
Cu9 Au1 Cu11 Au6 136.57(9) . 2_656
Cu9 Au1 Cu11 Cu4 -95.28(10) . .
Cu9 Au1 Cu11 Cu6 100.95(12) . 2_656
Cu9 Au1 Cu11 Cu12 -157.41(10) . .
Cu9 Au1 Cu11 S4 142.6(3) . .
Cu9 Au1 Cu11 S7 -46.67(16) . .
Cu9 Au1 Cu12 Au4 167.09(10) . .
Cu9 Au1 Cu12 Au6 96.34(11) . 2_656
Cu9 Au1 Cu12 Cu4 -32.60(15) . .
Cu9 Au1 Cu12 Cu5 -126.00(12) . .
Cu9 Au1 Cu12 Cu11 29.55(13) . .
Cu9 Au1 Cu12 S9 93.4(3) . .
Cu9 Au1 Cu12 S10 -79.46(19) . .
Cu9 Au1 Cu15 Au3 -67.16(8) . .
Cu9 Au1 Cu15 Au5 -139.16(9) . .
Cu9 Au1 Cu15 Cu13 -45.3(2) . .
Cu9 Au1 Cu15 Cu16 -108.47(13) . .
Cu9 Au1 Cu15 S11 148.97(19) . .
Cu9 Au1 Cu15 S8 2.93(19) . .
Cu9 Au2 Au3 Au1 70.96(7) . .
Cu9 Au2 Au3 Au2 -150.49(7) . 2_656
Cu9 Au2 Au3 Au5 107.45(8) . .
Cu9 Au2 Au3 Au6 170.80(8) . .
Cu9 Au2 Au3 Cu6 -126.04(11) . .
Cu9 Au2 Au3 Cu7 -79.79(10) . .
Cu9 Au2 Au3 Cu15 42.40(10) . .
Cu9 Au2 Au3 Cu16 127.8(2) . .
Cu9 Au2 Cu7 Au2 135.83(9) . 2_656
Cu9 Au2 Cu7 Au3 66.32(8) . .
Cu9 Au2 Cu7 Cu1 -169.75(15) . 2_656
Cu9 Au2 Cu7 Cu7 -159.87(11) . 2_656
Cu9 Au2 Cu7 S2 132.5(3) . 2_656
Cu9 Au2 Cu7 S3 -52.07(16) . .
Cu9 Au2 Cu11 Au1 -66.03(8) . .
Cu9 Au2 Cu11 Au6 -138.05(9) . 2_656
Cu9 Au2 Cu11 Cu4 -36.93(18) . .
Cu9 Au2 Cu11 Cu6 156.90(10) . 2_656
Cu9 Au2 Cu11 Cu12 -102.23(13) . .
Cu9 Au2 Cu11 S4 149.1(2) . .
Cu9 Au2 Cu11 S7 4.81(18) . .
Cu9 Au3 Au5 Au1 26.54(7) . .
Cu9 Au3 Au5 Au4 64.25(8) . .
Cu9 Au3 Au5 Au4 129.03(8) . 2_656
Cu9 Au3 Au5 Au6 165.60(8) . .
Cu9 Au3 Au5 Cu5 -0.18(11) . .
Cu9 Au3 Au5 Cu8 106.9(2) . .
Cu9 Au3 Au5 Cu10 -167.98(10) . .
Cu9 Au3 Au5 Cu15 -43.31(11) . .
Cu9 Au3 Au5 Cu16 -124.51(11) . .
Cu9 Au3 Au6 Au1 35.5(3) . 2_656
Cu9 Au3 Au6 Au2 72.0(3) . 2_656
Cu9 Au3 Au6 Au4 -28.3(3) . 2_656
Cu9 Au3 Au6 Au5 -65.8(3) . .
Cu9 Au3 Au6 Cu6 142.1(3) . .
Cu9 Au3 Au6 Cu10 -91.3(3) . .
Cu9 Au3 Au6 Cu11 97.4(3) . 2_656
Cu9 Au3 Au6 Cu12 11.0(4) . 2_656
Cu9 Au3 Au6 Cu16 -132.4(3) . .
Cu9 Au3 Cu6 Au2 -95.36(12) . 2_656
Cu9 Au3 Cu6 Au6 -167.93(10) . .
Cu9 Au3 Cu6 Cu11 -130.84(12) . 2_656
Cu9 Au3 Cu6 S4 -167.2(3) . 2_656
Cu9 Au3 Cu6 S2 -20.8(2) . 2_656
Cu9 Au3 Cu6 S13 86.9(2) . .
Cu9 Au3 Cu7 Au2 -67.25(8) . .
Cu9 Au3 Cu7 Au2 -140.14(9) . 2_656
Cu9 Au3 Cu7 Cu1 -174.76(18) . 2_656
Cu9 Au3 Cu7 Cu7 -106.60(15) . 2_656
Cu9 Au3 Cu7 S2 145.33(19) . 2_656
Cu9 Au3 Cu7 S3 1.71(18) . .
Cu9 Au3 Cu15 Au1 67.38(8) . .
Cu9 Au3 Cu15 Au5 136.76(9) . .
Cu9 Au3 Cu15 Cu13 -98.63(12) . .
Cu9 Au3 Cu15 Cu16 -160.60(12) . .
Cu9 Au3 Cu15 S11 141.6(3) . .
Cu9 Au3 Cu15 S8 -50.37(18) . .
Cu9 Au3 Cu16 Au5 93.03(12) . .
Cu9 Au3 Cu16 Au6 165.87(10) . .
Cu9 Au3 Cu16 Cu10 129.71(12) . .
Cu9 Au3 Cu16 Cu13 -38.02(15) . .
Cu9 Au3 Cu16 Cu15 23.76(14) . .
Cu9 Au3 Cu16 S15 81.6(4) . .
Cu9 Au3 Cu16 S13 -86.6(2) . .
Cu9 Cu7 S3 Cu1 -133.3(2) . .
Cu9 Cu7 S3 C15 118.6(7) . .
Cu9 Cu15 Cu16 Au3 -17.89(10) . .
Cu9 Cu15 Cu16 Au5 -94.94(13) . .
Cu9 Cu15 Cu16 Au6 -51.57(16) . .
Cu9 Cu15 Cu16 Cu10 -112.97(15) . .
Cu9 Cu15 Cu16 Cu13 77.75(15) . .
Cu9 Cu15 Cu16 S15 -167.0(2) . .
Cu9 Cu15 Cu16 S13 52.1(2) . .
Cu9 Cu15 S11 Cu5 57.8(4) . .
Cu9 Cu15 S11 Cu14 -172.2(3) . .
Cu9 Cu15 S11 C71 -52.1(10) . .
Cu9 Cu15 S8 Cu13 -136.9(2) . .
Cu9 Cu15 S8 C50 111.6(11) . .
Cu9 S7 C43 C44 58(2) . .
Cu9 S7 C43 C48 -114.9(18) . .
Cu9 S3 C15 C20 -65(2) . .
Cu9 S3 C15 C16 114.7(16) . .
Cu9 S8 C50 C51 142(2) . .
Cu9 S8 C50 C55 -41(3) . .
Cu10 Au4 Au5 Au1 79.7(3) 2_656 .
Cu10 Au4 Au5 Au3 42.3(3) 2_656 .
Cu10 Au4 Au5 Au4 -57.7(3) 2_656 2_656
Cu10 Au4 Au5 Au6 -21.0(3) 2_656 .
Cu10 Au4 Au5 Cu5 148.0(3) 2_656 .
Cu10 Au4 Au5 Cu8 -124.7(3) 2_656 .
Cu10 Au4 Au5 Cu10 -86.2(2) 2_656 .
Cu10 Au4 Au5 Cu15 103.0(3) 2_656 .
Cu10 Au4 Au5 Cu16 4.2(5) 2_656 .
Cu10 Au4 Cu5 Au1 -97.05(12) 2_656 .
Cu10 Au4 Cu5 Au5 -168.70(11) 2_656 .
Cu10 Au4 Cu5 Cu12 -30.37(14) 2_656 .
Cu10 Au4 Cu5 S10 -23.9(2) 2_656 .
Cu10 Au4 Cu5 S18 86.95(19) 2_656 .
Cu10 Au4 Cu5 S11 -168.2(3) 2_656 .
Cu10 Au4 Cu8 Au4 91.66(11) 2_656 2_656
Cu10 Au4 Cu8 Au5 163.72(9) 2_656 .
Cu10 Au4 Cu8 Cu2 -42.99(13) 2_656 .
Cu10 Au4 Cu8 Cu8 23.94(14) 2_656 2_656
Cu10 Au4 Cu8 Cu10 129.93(9) 2_656 .
Cu10 Au4 Cu8 S18 -91.71(18) 2_656 .
Cu10 Au4 Cu8 S16 76.7(4) 2_656 .
Cu10 Au4 Cu12 Au1 -137.88(9) 2_656 .
Cu10 Au4 Cu12 Au6 -66.31(8) 2_656 2_656
Cu10 Au4 Cu12 Cu4 -166.2(2) 2_656 .
Cu10 Au4 Cu12 Cu5 157.37(11) 2_656 .
Cu10 Au4 Cu12 Cu11 -102.56(13) 2_656 .
Cu10 Au4 Cu12 S9 4.69(17) 2_656 .
Cu10 Au4 Cu12 S10 150.4(2) 2_656 .
Cu10 Au5 Au6 Au1 108.05(8) . 2_656
Cu10 Au5 Au6 Au2 170.42(8) . 2_656
Cu10 Au5 Au6 Au3 -152.25(8) . .
Cu10 Au5 Au6 Au4 69.13(8) . 2_656
Cu10 Au5 Au6 Cu6 -125.80(11) . .
Cu10 Au5 Au6 Cu11 137.5(3) . 2_656
Cu10 Au5 Au6 Cu12 44.26(10) . 2_656
Cu10 Au5 Au6 Cu16 -79.51(11) . .
Cu10 Au5 Cu5 Au1 -167.67(10) . .
Cu10 Au5 Cu5 Au4 -95.58(12) . .
Cu10 Au5 Cu5 Cu12 -130.43(12) . .
Cu10 Au5 Cu5 S10 -167.0(3) . .
Cu10 Au5 Cu5 S18 -21.4(2) . .
Cu10 Au5 Cu5 S11 84.72(19) . .
Cu10 Au5 Cu8 Au4 -67.52(8) . 2_656
Cu10 Au5 Cu8 Au4 -140.92(10) . .
Cu10 Au5 Cu8 Cu2 -177.00(19) . .
Cu10 Au5 Cu8 Cu8 -107.09(16) . 2_656
Cu10 Au5 Cu8 S18 144.0(2) . .
Cu10 Au5 Cu8 S16 1.75(18) . .
Cu10 Au5 Cu15 Au1 167.31(10) . .
Cu10 Au5 Cu15 Au3 94.34(12) . .
Cu10 Au5 Cu15 Cu9 131.77(12) . .
Cu10 Au5 Cu15 Cu13 31.64(19) . .
Cu10 Au5 Cu15 Cu16 24.65(14) . .
Cu10 Au5 Cu15 S11 -82.76(19) . .
Cu10 Au5 Cu15 S8 82.0(4) . .
Cu10 Au5 Cu16 Au3 137.27(9) . .
Cu10 Au5 Cu16 Au6 67.96(8) . .
Cu10 Au5 Cu16 Cu13 -167.23(17) . .
Cu10 Au5 Cu16 Cu15 -160.17(12) . .
Cu10 Au5 Cu16 S15 -49.52(18) . .
Cu10 Au5 Cu16 S13 137.9(4) . .
Cu10 Au6 Cu6 Au2 -165.14(9) . 2_656
Cu10 Au6 Cu6 Au3 -95.11(11) . .
Cu10 Au6 Cu6 Cu11 129.23(12) . 2_656
Cu10 Au6 Cu6 S4 85.29(19) . 2_656
Cu10 Au6 Cu6 S2 -157.1(3) . 2_656
Cu10 Au6 Cu6 S13 -21.0(2) . .
Cu10 Au6 Cu16 Au3 -138.41(9) . .
Cu10 Au6 Cu16 Au5 -66.63(8) . .
Cu10 Au6 Cu16 Cu13 -170.0(2) . .
Cu10 Au6 Cu16 Cu15 -107.56(13) . .
Cu10 Au6 Cu16 S15 2.8(2) . .
Cu10 Au6 Cu16 S13 148.7(2) . .
Cu10 Cu8 S18 Cu2 -171.0(2) . .
Cu10 Cu8 S18 Cu5 59.8(3) . .
Cu10 Cu8 S18 C120 -54.3(9) . .
Cu10 Cu8 S16 Cu2 -132.7(2) . 2_656
Cu10 Cu8 S16 C106 118.4(8) . .
Cu10 Cu16 S15 Cu14 -137.4(3) . .
Cu10 Cu16 S15 C99 109.7(12) . .
Cu10 Cu16 S13 Cu6 57.5(4) . .
Cu10 Cu16 S13 Cu13 -173.5(3) . .
Cu10 Cu16 S13 C85 -54.4(14) . .
Cu10 S9 C57 C58 68(2) 2_656 .
Cu10 S9 C57 C62 -111(2) 2_656 .
Cu10 S16 C106 C111 114.1(17) . .
Cu10 S16 C106 C107 -66(2) . .
Cu10 S15 C99 C100 140.2(14) . .
Cu10 S15 C99 C104 -41.2(17) . .
Cu11 Au1 Au2 Au2 -170.17(9) . 2_656
Cu11 Au1 Au2 Au3 153.45(8) . .
Cu11 Au1 Au2 Au3 -106.63(8) . 2_656
Cu11 Au1 Au2 Au6 -69.48(8) . 2_656
Cu11 Au1 Au2 Cu6 -42.90(10) . 2_656
Cu11 Au1 Au2 Cu7 126.20(11) . .
Cu11 Au1 Au2 Cu7 -146.0(3) . 2_656
Cu11 Au1 Au2 Cu9 84.60(11) . .
Cu11 Au1 Au3 Au2 -62.84(8) . 2_656
Cu11 Au1 Au3 Au2 -25.23(8) . .
Cu11 Au1 Au3 Au5 -163.81(8) . .
Cu11 Au1 Au3 Au6 -127.24(8) . .
Cu11 Au1 Au3 Cu6 -100.2(3) . .
Cu11 Au1 Au3 Cu7 1.03(11) . .
Cu11 Au1 Au3 Cu9 44.55(10) . .
Cu11 Au1 Au3 Cu15 123.86(11) . .
Cu11 Au1 Au3 Cu16 170.84(10) . .
Cu11 Au1 Au4 Au4 127.85(8) . 2_656
Cu11 Au1 Au4 Au5 66.02(8) . 2_656
Cu11 Au1 Au4 Au5 165.81(8) . .
Cu11 Au1 Au4 Au6 27.29(7) . 2_656
Cu11 Au1 Au4 Cu5 -124.00(10) . .
Cu11 Au1 Au4 Cu8 -171.08(10) . .
Cu11 Au1 Au4 Cu8 98.4(3) . 2_656
Cu11 Au1 Au4 Cu10 2.88(11) . 2_656
Cu11 Au1 Au4 Cu12 -42.37(10) . .
Cu11 Au1 Au5 Au3 77.3(3) . .
Cu11 Au1 Au5 Au4 -61.1(3) . .
Cu11 Au1 Au5 Au4 -22.1(3) . 2_656
Cu11 Au1 Au5 Au6 40.9(3) . .
Cu11 Au1 Au5 Cu5 -131.8(3) . .
Cu11 Au1 Au5 Cu8 -84.4(3) . .
Cu11 Au1 Au5 Cu10 6.9(5) . .
Cu11 Au1 Au5 Cu15 144.0(3) . .
Cu11 Au1 Au5 Cu16 105.5(3) . .
Cu11 Au1 Cu5 Au4 95.32(11) . .
Cu11 Au1 Cu5 Au5 165.48(10) . .
Cu11 Au1 Cu5 Cu12 29.76(13) . .
Cu11 Au1 Cu5 S10 -14.1(2) . .
Cu11 Au1 Cu5 S18 101.8(3) . .
Cu11 Au1 Cu5 S11 -121.31(17) . .
Cu11 Au1 Cu9 Au2 -65.50(8) . .
Cu11 Au1 Cu9 Au3 -137.74(9) . .
Cu11 Au1 Cu9 Cu7 -100.13(12) . .
Cu11 Au1 Cu9 Cu15 156.97(11) . .
Cu11 Au1 Cu9 S7 44.72(17) . .
Cu11 Au1 Cu9 S3 -55.9(2) . .
Cu11 Au1 Cu9 S8 154.25(19) . .
Cu11 Au1 Cu12 Au4 137.54(9) . .
Cu11 Au1 Cu12 Au6 66.79(8) . 2_656
Cu11 Au1 Cu12 Cu4 -62.15(11) . .
Cu11 Au1 Cu12 Cu5 -155.55(11) . .
Cu11 Au1 Cu12 S9 63.9(3) . .
Cu11 Au1 Cu12 S10 -109.01(17) . .
Cu11 Au1 Cu15 Au3 -96.40(11) . .
Cu11 Au1 Cu15 Au5 -168.39(10) . .
Cu11 Au1 Cu15 Cu9 -29.23(13) . .
Cu11 Au1 Cu15 Cu13 -74.5(2) . .
Cu11 Au1 Cu15 Cu16 -137.71(12) . .
Cu11 Au1 Cu15 S11 119.74(18) . .
Cu11 Au1 Cu15 S8 -26.3(2) . .
Cu11 Au2 Au3 Au1 24.61(8) . .
Cu11 Au2 Au3 Au2 163.17(7) . 2_656
Cu11 Au2 Au3 Au5 61.10(8) . .
Cu11 Au2 Au3 Au6 124.45(8) . .
Cu11 Au2 Au3 Cu6 -172.38(10) . .
Cu11 Au2 Au3 Cu7 -126.14(10) . .
Cu11 Au2 Au3 Cu9 -46.35(10) . .
Cu11 Au2 Au3 Cu15 -3.95(11) . .
Cu11 Au2 Au3 Cu16 81.4(2) . .
Cu11 Au2 Cu7 Au2 165.01(10) . 2_656
Cu11 Au2 Cu7 Au3 95.49(12) . .
Cu11 Au2 Cu7 Cu1 -140.57(13) . 2_656
Cu11 Au2 Cu7 Cu7 -130.69(14) . 2_656
Cu11 Au2 Cu7 Cu9 29.18(14) . .
Cu11 Au2 Cu7 S2 161.7(3) . 2_656
Cu11 Au2 Cu7 S3 -22.9(2) . .
Cu11 Au2 Cu9 Au1 64.08(8) . .
Cu11 Au2 Cu9 Au3 135.45(9) . .
Cu11 Au2 Cu9 Cu7 -157.45(11) . .
Cu11 Au2 Cu9 Cu15 99.93(12) . .
Cu11 Au2 Cu9 S7 -4.55(17) . .
Cu11 Au2 Cu9 S3 -109.42(15) . .
Cu11 Au2 Cu9 S8 143.5(3) . .
Cu11 Au6 Cu6 Au2 65.64(8) 2_656 2_656
Cu11 Au6 Cu6 Au3 135.66(9) 2_656 .
Cu11 Au6 Cu6 S4 -43.93(17) 2_656 2_656
Cu11 Au6 Cu6 S2 73.6(3) 2_656 2_656
Cu11 Au6 Cu6 S13 -150.2(2) 2_656 .
Cu11 Au6 Cu10 Au4 -92.11(12) 2_656 2_656
Cu11 Au6 Cu10 Au5 -164.74(11) 2_656 .
Cu11 Au6 Cu10 Cu8 -126.78(13) 2_656 .
Cu11 Au6 Cu10 Cu16 129.81(13) 2_656 .
Cu11 Au6 Cu10 S9 17.4(2) 2_656 2_656
Cu11 Au6 Cu10 S16 -81.9(3) 2_656 .
Cu11 Au6 Cu10 S15 127.2(2) 2_656 .
Cu11 Au6 Cu16 Au3 94.20(12) 2_656 .
Cu11 Au6 Cu16 Au5 165.99(11) 2_656 .
Cu11 Au6 Cu16 Cu10 -127.38(13) 2_656 .
Cu11 Au6 Cu16 Cu13 62.6(2) 2_656 .
Cu11 Au6 Cu16 Cu15 125.06(13) 2_656 .
Cu11 Au6 Cu16 S15 -124.6(2) 2_656 .
Cu11 Au6 Cu16 S13 21.3(3) 2_656 .
Cu11 Cu4 Cu12 Au1 56.87(9) . .
Cu11 Cu4 Cu12 Au4 82.14(18) . .
Cu11 Cu4 Cu12 Au6 6.73(12) . 2_656
Cu11 Cu4 Cu12 Cu5 111.91(12) . .
Cu11 Cu4 Cu12 S9 -87.4(2) . .
Cu11 Cu4 Cu12 S10 147.7(2) . .
Cu11 Cu4 S10 Cu5 48.2(4) . .
Cu11 Cu4 S10 Cu12 -27.68(19) . .
Cu11 Cu4 S10 C64 -141.7(10) . .
Cu11 Cu4 S7 Cu9 -75.8(4) . .
Cu11 Cu4 S7 C43 116.7(10) . .
Cu11 Cu4 S6 Au9 52.1(3) . .
Cu11 Cu4 S6 C36 157.9(9) . .
Cu11 Cu6 S13 Cu13 -133.9(4) 2_656 .
Cu11 Cu6 S13 Cu16 -52.2(4) 2_656 .
Cu11 Cu6 S13 C85 60.7(16) 2_656 .
Cu11 Cu12 S9 Cu3 -28.81(19) . .
Cu11 Cu12 S9 Cu10 104.46(16) . 2_656
Cu11 Cu12 S9 C57 -143.7(8) . .
Cu11 Cu12 S10 Cu4 28.32(19) . .
Cu11 Cu12 S10 Cu5 -102.79(16) . .
Cu11 Cu12 S10 C64 143.1(8) . .
Cu11 S4 C22 C23 118(2) . .
Cu11 S4 C22 C27 -60(2) . .
Cu11 S7 C43 C44 -37(2) . .
Cu11 S7 C43 C48 150.6(18) . .
Cu12 Au1 Au2 Au2 -127.75(8) . 2_656
Cu12 Au1 Au2 Au3 -64.21(8) . 2_656
Cu12 Au1 Au2 Au3 -164.13(8) . .
Cu12 Au1 Au2 Au6 -27.06(7) . 2_656
Cu12 Au1 Au2 Cu6 -0.48(10) . 2_656
Cu12 Au1 Au2 Cu7 -103.6(2) . 2_656
Cu12 Au1 Au2 Cu7 168.62(10) . .
Cu12 Au1 Au2 Cu9 127.02(10) . .
Cu12 Au1 Au2 Cu11 42.42(10) . .
Cu12 Au1 Au3 Au2 32.7(3) . 2_656
Cu12 Au1 Au3 Au2 70.3(3) . .
Cu12 Au1 Au3 Au5 -68.3(3) . .
Cu12 Au1 Au3 Au6 -31.7(3) . .
Cu12 Au1 Au3 Cu6 -4.7(4) . .
Cu12 Au1 Au3 Cu7 96.5(3) . .
Cu12 Au1 Au3 Cu9 140.1(3) . .
Cu12 Au1 Au3 Cu15 -140.6(3) . .
Cu12 Au1 Au3 Cu16 -93.6(3) . .
Cu12 Au1 Au4 Au4 170.23(9) . 2_656
Cu12 Au1 Au4 Au5 108.39(8) . 2_656
Cu12 Au1 Au4 Au5 -151.81(8) . .
Cu12 Au1 Au4 Au6 69.66(8) . 2_656
Cu12 Au1 Au4 Cu5 -81.63(10) . .
Cu12 Au1 Au4 Cu8 140.7(3) . 2_656
Cu12 Au1 Au4 Cu8 -128.71(10) . .
Cu12 Au1 Au4 Cu10 45.25(10) . 2_656
Cu12 Au1 Au5 Au3 164.40(8) . .
Cu12 Au1 Au5 Au4 64.96(8) . 2_656
Cu12 Au1 Au5 Au4 26.01(7) . .
Cu12 Au1 Au5 Au6 127.96(8) . .
Cu12 Au1 Au5 Cu5 -44.76(10) . .
Cu12 Au1 Au5 Cu8 2.70(11) . .
Cu12 Au1 Au5 Cu10 94.0(3) . .
Cu12 Au1 Au5 Cu15 -128.97(11) . .
Cu12 Au1 Au5 Cu16 -167.47(11) . .
Cu12 Au1 Cu5 Au4 65.56(8) . .
Cu12 Au1 Cu5 Au5 135.72(9) . .
Cu12 Au1 Cu5 S10 -43.90(16) . .
Cu12 Au1 Cu5 S18 72.0(3) . .
Cu12 Au1 Cu5 S11 -151.07(17) . .
Cu12 Au1 Cu9 Au2 -94.30(11) . .
Cu12 Au1 Cu9 Au3 -166.53(10) . .
Cu12 Au1 Cu9 Cu7 -128.93(12) . .
Cu12 Au1 Cu9 Cu15 128.18(13) . .
Cu12 Au1 Cu9 S7 15.9(2) . .
Cu12 Au1 Cu9 S3 -84.7(3) . .
Cu12 Au1 Cu9 S8 125.46(19) . .
Cu12 Au1 Cu11 Au2 -137.79(9) . .
Cu12 Au1 Cu11 Au6 -66.02(8) . 2_656
Cu12 Au1 Cu11 Cu4 62.14(10) . .
Cu12 Au1 Cu11 Cu6 -101.63(13) . 2_656
Cu12 Au1 Cu11 S4 -60.0(3) . .
Cu12 Au1 Cu11 S7 110.74(17) . .
Cu12 Au1 Cu15 Au3 166.38(10) . .
Cu12 Au1 Cu15 Au5 94.38(12) . .
Cu12 Au1 Cu15 Cu9 -126.46(13) . .
Cu12 Au1 Cu15 Cu13 -171.74(18) . .
Cu12 Au1 Cu15 Cu16 125.07(13) . .
Cu12 Au1 Cu15 S11 22.5(2) . .
Cu12 Au1 Cu15 S8 -123.5(2) . .
Cu12 Au4 Au5 Au1 -26.24(8) . .
Cu12 Au4 Au5 Au3 -63.68(8) . .
Cu12 Au4 Au5 Au4 -163.59(7) . 2_656
Cu12 Au4 Au5 Au6 -126.91(8) . .
Cu12 Au4 Au5 Cu5 42.10(10) . .
Cu12 Au4 Au5 Cu8 129.34(10) . .
Cu12 Au4 Au5 Cu10 167.90(10) . .
Cu12 Au4 Au5 Cu15 -2.92(11) . .
Cu12 Au4 Au5 Cu16 -101.8(4) . .
Cu12 Au4 Cu5 Au1 -66.68(8) . .
Cu12 Au4 Cu5 Au5 -138.33(9) . .
Cu12 Au4 Cu5 S10 6.50(16) . .
Cu12 Au4 Cu5 S18 117.32(17) . .
Cu12 Au4 Cu5 S11 -137.8(3) . .
Cu12 Au4 Cu8 Au4 -165.73(11) . 2_656
Cu12 Au4 Cu8 Au5 -93.68(12) . .
Cu12 Au4 Cu8 Cu2 59.61(15) . .
Cu12 Au4 Cu8 Cu8 126.54(15) . 2_656
Cu12 Au4 Cu8 Cu10 -127.46(13) . .
Cu12 Au4 Cu8 S18 10.9(2) . .
Cu12 Au4 Cu8 S16 179.3(3) . .
Cu12 Au6 Cu6 Au2 95.01(11) 2_656 2_656
Cu12 Au6 Cu6 Au3 165.03(10) 2_656 .
Cu12 Au6 Cu6 Cu11 29.37(13) 2_656 2_656
Cu12 Au6 Cu6 S4 -14.6(2) 2_656 2_656
Cu12 Au6 Cu6 S2 103.0(3) 2_656 2_656
Cu12 Au6 Cu6 S13 -120.84(19) 2_656 .
Cu12 Au6 Cu10 Au4 -65.28(8) 2_656 2_656
Cu12 Au6 Cu10 Au5 -137.90(9) 2_656 .
Cu12 Au6 Cu10 Cu8 -99.94(12) 2_656 .
Cu12 Au6 Cu10 Cu16 156.64(11) 2_656 .
Cu12 Au6 Cu10 S9 44.19(16) 2_656 2_656
Cu12 Au6 Cu10 S16 -55.1(2) 2_656 .
Cu12 Au6 Cu10 S15 154.0(2) 2_656 .
Cu12 Au6 Cu16 Au3 -167.99(10) 2_656 .
Cu12 Au6 Cu16 Au5 -96.20(11) 2_656 .
Cu12 Au6 Cu16 Cu10 -29.57(14) 2_656 .
Cu12 Au6 Cu16 Cu13 160.39(16) 2_656 .
Cu12 Au6 Cu16 Cu15 -137.13(12) 2_656 .
Cu12 Au6 Cu16 S15 -26.8(3) 2_656 .
Cu12 Au6 Cu16 S13 119.1(2) 2_656 .
Cu12 Cu4 Cu11 Au1 -58.31(9) . .
Cu12 Cu4 Cu11 Au2 -84.19(18) . .
Cu12 Cu4 Cu11 Au6 -6.75(12) . 2_656
Cu12 Cu4 Cu11 Cu6 51.7(5) . 2_656
Cu12 Cu4 Cu11 S4 89.4(2) . .
Cu12 Cu4 Cu11 S7 -145.0(2) . .
Cu12 Cu4 S10 Cu5 75.9(3) . .
Cu12 Cu4 S10 C64 -114.0(10) . .
Cu12 Cu4 S7 Cu9 -45.9(4) . .
Cu12 Cu4 S7 Cu11 29.85(19) . .
Cu12 Cu4 S7 C43 146.5(10) . .
Cu12 Cu4 S6 Au9 -22.7(4) . .
Cu12 Cu4 S6 C36 83.1(9) . .
Cu12 Cu5 S10 Cu4 -77.9(3) . .
Cu12 Cu5 S10 C64 112.1(10) . .
Cu12 Cu5 S18 Cu2 16.7(3) . .
Cu12 Cu5 S18 Cu8 97.09(19) . .
Cu12 Cu5 S18 C120 -148.3(8) . .
Cu12 Cu5 S11 Cu14 -140.4(3) . .
Cu12 Cu5 S11 Cu15 -52.4(3) . .
Cu12 Cu5 S11 C71 66.5(10) . .
Cu12 Cu11 S4 Cu3 22.91(19) . .
Cu12 Cu11 S4 Cu6 -103.68(16) . 2_656
Cu12 Cu11 S4 C22 141.3(9) . .
Cu12 Cu11 S7 Cu4 -30.78(19) . .
Cu12 Cu11 S7 Cu9 105.82(17) . .
Cu12 Cu11 S7 C43 -143.2(8) . .
Cu12 S9 C57 C58 -28(2) . .
Cu12 S9 C57 C62 152.7(19) . .
Cu12 S10 C64 C65 129.6(19) . .
Cu12 S10 C64 C69 -53(2) . .
Cu13 Au10 Cu14 S11 -65.3(2) . .
Cu13 Au10 Cu14 S15 72.8(3) . .
Cu13 Au10 Cu14 S14 172.4(4) . .
Cu13 Au10 S14 Cu14 -10.8(5) . .
Cu13 Au10 S14 C92 -127.2(10) . .
Cu13 Au10 S12 C78 -122.6(14) . .
Cu13 Cu15 Cu16 Au3 -95.64(12) . .
Cu13 Cu15 Cu16 Au5 -172.70(14) . .
Cu13 Cu15 Cu16 Au6 -129.32(15) . .
Cu13 Cu15 Cu16 Cu10 169.28(17) . .
Cu13 Cu15 Cu16 S15 115.3(2) . .
Cu13 Cu15 Cu16 S13 -25.6(2) . .
Cu13 Cu15 S11 Cu5 -162.50(16) . .
Cu13 Cu15 S11 Cu14 -32.5(3) . .
Cu13 Cu15 S11 C71 87.6(9) . .
Cu13 Cu15 S8 Cu9 136.9(2) . .
Cu13 Cu15 S8 C50 -111.5(11) . .
Cu13 Cu16 S15 Cu10 170.89(17) . .
Cu13 Cu16 S15 Cu14 33.5(3) . .
Cu13 Cu16 S15 C99 -79.4(12) . .
Cu13 Cu16 S13 Cu6 -129.0(3) . .
Cu13 Cu16 S13 C85 119.1(13) . .
Cu13 S8 C50 C51 -32(3) . .
Cu13 S8 C50 C55 145(2) . .
Cu13 S13 C85 C86 115.7(17) . .
Cu13 S13 C85 C90 -68(2) . .
Cu13 S12 C78 C83 85(2) . .
Cu13 S12 C78 C79 -88(2) . .
Cu14 Au10 Cu13 Cu15 27.74(12) . .
Cu14 Au10 Cu13 Cu16 -32.00(12) . .
Cu14 Au10 Cu13 S8 73.2(2) . .
Cu14 Au10 Cu13 S13 -74.7(2) . .
Cu14 Au10 Cu13 S12 175.3(4) . .
Cu14 Au10 S14 C92 -116.4(11) . .
Cu14 Au10 S12 Cu13 -6.4(5) . .
Cu14 Au10 S12 C78 -129.0(13) . .
Cu14 S11 C71 C76 131.9(19) . .
Cu14 S11 C71 C72 -52(3) . .
Cu14 S15 C99 C100 -47.8(19) . .
Cu14 S15 C99 C104 130.8(13) . .
Cu14 S14 C92 C93 114.8(14) . .
Cu14 S14 C92 C97 -67.6(19) . .
Cu15 Au1 Au2 Au2 64.00(8) . 2_656
Cu15 Au1 Au2 Au3 127.54(8) . 2_656
Cu15 Au1 Au2 Au3 27.62(7) . .
Cu15 Au1 Au2 Au6 164.69(8) . 2_656
Cu15 Au1 Au2 Cu6 -168.73(10) . 2_656
Cu15 Au1 Au2 Cu7 0.37(10) . .
Cu15 Au1 Au2 Cu7 88.2(3) . 2_656
Cu15 Au1 Au2 Cu9 -41.23(10) . .
Cu15 Au1 Au2 Cu11 -125.83(11) . .
Cu15 Au1 Au3 Au2 -149.08(9) . .
Cu15 Au1 Au3 Au2 173.30(9) . 2_656
Cu15 Au1 Au3 Au5 72.34(8) . .
Cu15 Au1 Au3 Au6 108.91(9) . .
Cu15 Au1 Au3 Cu6 135.9(3) . .
Cu15 Au1 Au3 Cu7 -122.83(11) . .
Cu15 Au1 Au3 Cu9 -79.30(11) . .
Cu15 Au1 Au3 Cu16 46.99(11) . .
Cu15 Au1 Au4 Au4 -62.15(8) . 2_656
Cu15 Au1 Au4 Au5 -24.19(8) . .
Cu15 Au1 Au4 Au5 -123.99(8) . 2_656
Cu15 Au1 Au4 Au6 -162.71(8) . 2_656
Cu15 Au1 Au4 Cu5 46.00(10) . .
Cu15 Au1 Au4 Cu8 -91.6(3) . 2_656
Cu15 Au1 Au4 Cu8 -1.08(11) . .
Cu15 Au1 Au4 Cu10 172.88(10) . 2_656
Cu15 Au1 Au4 Cu12 127.62(11) . .
Cu15 Au1 Au5 Au3 -66.63(8) . .
Cu15 Au1 Au5 Au4 -166.07(8) . 2_656
Cu15 Au1 Au5 Au4 154.98(8) . .
Cu15 Au1 Au5 Au6 -103.07(8) . .
Cu15 Au1 Au5 Cu5 84.21(11) . .
Cu15 Au1 Au5 Cu8 131.67(11) . .
Cu15 Au1 Au5 Cu10 -137.1(3) . .
Cu15 Au1 Au5 Cu16 -38.50(11) . .
Cu15 Au1 Cu5 Au4 -136.76(9) . .
Cu15 Au1 Cu5 Au5 -66.60(8) . .
Cu15 Au1 Cu5 Cu12 157.67(10) . .
Cu15 Au1 Cu5 S10 113.78(17) . .
Cu15 Au1 Cu5 S18 -130.3(3) . .
Cu15 Au1 Cu5 S11 6.61(15) . .
Cu15 Au1 Cu9 Au2 137.52(9) . .
Cu15 Au1 Cu9 Au3 65.29(8) . .
Cu15 Au1 Cu9 Cu7 102.89(12) . .
Cu15 Au1 Cu9 S7 -112.26(18) . .
Cu15 Au1 Cu9 S3 147.1(3) . .
Cu15 Au1 Cu9 S8 -2.72(17) . .
Cu15 Au1 Cu11 Au2 92.86(11) . .
Cu15 Au1 Cu11 Au6 164.62(10) . 2_656
Cu15 Au1 Cu11 Cu4 -67.22(14) . .
Cu15 Au1 Cu11 Cu6 129.01(12) . 2_656
Cu15 Au1 Cu11 Cu12 -129.36(12) . .
Cu15 Au1 Cu11 S4 170.7(3) . .
Cu15 Au1 Cu11 S7 -18.6(2) . .
Cu15 Au1 Cu12 Au4 -96.91(12) . .
Cu15 Au1 Cu12 Au6 -167.66(11) . 2_656
Cu15 Au1 Cu12 Cu4 63.40(15) . .
Cu15 Au1 Cu12 Cu5 -30.00(14) . .
Cu15 Au1 Cu12 Cu11 125.55(14) . .
Cu15 Au1 Cu12 S9 -170.6(3) . .
Cu15 Au1 Cu12 S10 16.5(2) . .
Cu15 Au3 Au5 Au1 69.84(8) . .
Cu15 Au3 Au5 Au4 107.56(8) . .
Cu15 Au3 Au5 Au4 172.34(8) . 2_656
Cu15 Au3 Au5 Au6 -151.10(8) . .
Cu15 Au3 Au5 Cu5 43.12(11) . .
Cu15 Au3 Au5 Cu8 150.2(3) . .
Cu15 Au3 Au5 Cu10 -124.67(11) . .
Cu15 Au3 Au5 Cu16 -81.21(11) . .
Cu15 Au3 Au6 Au1 129.08(8) . 2_656
Cu15 Au3 Au6 Au2 165.60(9) . 2_656
Cu15 Au3 Au6 Au4 65.30(9) . 2_656
Cu15 Au3 Au6 Au5 27.81(8) . .
Cu15 Au3 Au6 Cu6 -124.29(11) . .
Cu15 Au3 Au6 Cu10 2.31(11) . .
Cu15 Au3 Au6 Cu11 -169.05(11) . 2_656
Cu15 Au3 Au6 Cu12 104.6(3) . 2_656
Cu15 Au3 Au6 Cu16 -38.78(11) . .
Cu15 Au3 Cu6 Au2 169.37(11) . 2_656
Cu15 Au3 Cu6 Au6 96.79(12) . .
Cu15 Au3 Cu6 Cu11 133.89(13) . 2_656
Cu15 Au3 Cu6 S4 97.5(3) . 2_656
Cu15 Au3 Cu6 S2 -116.03(18) . 2_656
Cu15 Au3 Cu6 S13 -8.4(2) . .
Cu15 Au3 Cu7 Au2 -93.89(11) . .
Cu15 Au3 Cu7 Au2 -166.79(10) . 2_656
Cu15 Au3 Cu7 Cu1 158.60(14) . 2_656
Cu15 Au3 Cu7 Cu7 -133.24(14) . 2_656
Cu15 Au3 Cu7 Cu9 -26.64(13) . .
Cu15 Au3 Cu7 S2 118.68(18) . 2_656
Cu15 Au3 Cu7 S3 -24.9(2) . .
Cu15 Au3 Cu9 Au1 -67.19(8) . .
Cu15 Au3 Cu9 Au2 -137.17(10) . .
Cu15 Au3 Cu9 Cu7 157.45(11) . .
Cu15 Au3 Cu9 S7 -63.5(3) . .
Cu15 Au3 Cu9 S3 155.91(19) . .
Cu15 Au3 Cu9 S8 47.92(18) . .
Cu15 Au3 Cu16 Au5 69.27(9) . .
Cu15 Au3 Cu16 Au6 142.11(10) . .
Cu15 Au3 Cu16 Cu10 105.95(13) . .
Cu15 Au3 Cu16 Cu13 -61.79(12) . .
Cu15 Au3 Cu16 S15 57.9(3) . .
Cu15 Au3 Cu16 S13 -110.4(2) . .
Cu15 Au5 Au6 Au1 -125.09(8) . 2_656
Cu15 Au5 Au6 Au2 -62.72(8) . 2_656
Cu15 Au5 Au6 Au3 -25.39(8) . .
Cu15 Au5 Au6 Au4 -164.01(8) . 2_656
Cu15 Au5 Au6 Cu6 1.05(11) . .
Cu15 Au5 Au6 Cu10 126.86(11) . .
Cu15 Au5 Au6 Cu11 -95.7(3) . 2_656
Cu15 Au5 Au6 Cu12 171.11(10) . 2_656
Cu15 Au5 Au6 Cu16 47.35(11) . .
Cu15 Au5 Cu5 Au1 64.59(8) . .
Cu15 Au5 Cu5 Au4 136.68(9) . .
Cu15 Au5 Cu5 Cu12 101.84(12) . .
Cu15 Au5 Cu5 S10 65.2(3) . .
Cu15 Au5 Cu5 S18 -149.09(19) . .
Cu15 Au5 Cu5 S11 -43.01(16) . .
Cu15 Au5 Cu8 Au4 94.06(13) . .
Cu15 Au5 Cu8 Au4 167.46(12) . 2_656
Cu15 Au5 Cu8 Cu2 58.0(2) . .
Cu15 Au5 Cu8 Cu8 127.88(15) . 2_656
Cu15 Au5 Cu8 Cu10 -125.02(14) . .
Cu15 Au5 Cu8 S18 19.0(2) . .
Cu15 Au5 Cu8 S16 -123.3(2) . .
Cu15 Au5 Cu10 Au4 -161.85(10) . 2_656
Cu15 Au5 Cu10 Au6 -91.83(12) . .
Cu15 Au5 Cu10 Cu8 132.64(13) . .
Cu15 Au5 Cu10 Cu16 -24.75(14) . .
Cu15 Au5 Cu10 S9 -88.8(3) . 2_656
Cu15 Au5 Cu10 S16 131.07(17) . .
Cu15 Au5 Cu10 S15 22.4(2) . .
Cu15 Au5 Cu16 Au3 -62.57(8) . .
Cu15 Au5 Cu16 Au6 -131.88(10) . .
Cu15 Au5 Cu16 Cu10 160.17(12) . .
Cu15 Au5 Cu16 Cu13 -7.07(14) . .
Cu15 Au5 Cu16 S15 110.65(19) . .
Cu15 Au5 Cu16 S13 -62.0(4) . .
Cu15 Cu9 S7 Cu4 -27.6(4) . .
Cu15 Cu9 S7 Cu11 -103.27(18) . .
Cu15 Cu9 S7 C43 140.1(9) . .
Cu15 Cu9 S3 Cu1 122.3(4) . .
Cu15 Cu9 S3 Cu7 46.1(4) . .
Cu15 Cu9 S3 C15 -61.5(9) . .
Cu15 Cu9 S8 Cu13 67.5(4) . .
Cu15 Cu9 S8 C50 -104.8(10) . .
Cu15 Cu13 Cu16 Au3 55.53(9) . .
Cu15 Cu13 Cu16 Au5 6.97(13) . .
Cu15 Cu13 Cu16 Au6 83.55(18) . .
Cu15 Cu13 Cu16 Cu10 -53.2(7) . .
Cu15 Cu13 Cu16 S15 -88.8(2) . .
Cu15 Cu13 Cu16 S13 144.9(3) . .
Cu15 Cu13 S8 Cu9 -65.2(4) . .
Cu15 Cu13 S8 C50 107.2(10) . .
Cu15 Cu13 S13 Cu6 52.6(4) . .
Cu15 Cu13 S13 Cu16 -30.3(2) . .
Cu15 Cu13 S13 C85 -143.0(16) . .
Cu15 Cu13 S12 Au10 46.3(5) . .
Cu15 Cu13 S12 C78 153.9(19) . .
Cu15 Cu16 S15 Cu10 108.83(17) . .
Cu15 Cu16 S15 Cu14 -28.6(3) . .
Cu15 Cu16 S15 C99 -141.5(12) . .
Cu15 Cu16 S13 Cu6 -98.80(19) . .
Cu15 Cu16 S13 Cu13 30.2(2) . .
Cu15 Cu16 S13 C85 149.3(13) . .
Cu15 S11 C71 C76 25(2) . .
Cu15 S11 C71 C72 -159(2) . .
Cu15 S8 C50 C51 58(3) . .
Cu15 S8 C50 C55 -125(2) . .
Cu16 Au3 Au5 Au1 151.05(8) . .
Cu16 Au3 Au5 Au4 -106.46(8) . 2_656
Cu16 Au3 Au5 Au4 -171.24(8) . .
Cu16 Au3 Au5 Au6 -69.89(8) . .
Cu16 Au3 Au5 Cu5 124.33(11) . .
Cu16 Au3 Au5 Cu8 -128.6(3) . .
Cu16 Au3 Au5 Cu10 -43.47(11) . .
Cu16 Au3 Au5 Cu15 81.21(11) . .
Cu16 Au3 Au6 Au1 167.86(9) . 2_656
Cu16 Au3 Au6 Au2 -155.62(8) . 2_656
Cu16 Au3 Au6 Au4 104.09(8) . 2_656
Cu16 Au3 Au6 Au5 66.59(8) . .
Cu16 Au3 Au6 Cu6 -85.50(11) . .
Cu16 Au3 Au6 Cu10 41.09(10) . .
Cu16 Au3 Au6 Cu11 -130.27(11) . 2_656
Cu16 Au3 Au6 Cu12 143.4(3) . 2_656
Cu16 Au3 Cu6 Au2 136.66(9) . 2_656
Cu16 Au3 Cu6 Au6 64.08(8) . .
Cu16 Au3 Cu6 Cu11 101.18(12) . 2_656
Cu16 Au3 Cu6 S4 64.8(3) . 2_656
Cu16 Au3 Cu6 S2 -148.74(18) . 2_656
Cu16 Au3 Cu6 S13 -41.1(2) . .
Cu16 Au3 Cu7 Au2 167.63(11) . .
Cu16 Au3 Cu7 Au2 94.73(13) . 2_656
Cu16 Au3 Cu7 Cu1 60.1(2) . 2_656
Cu16 Au3 Cu7 Cu7 128.28(14) . 2_656
Cu16 Au3 Cu7 Cu9 -125.13(14) . .
Cu16 Au3 Cu7 S2 20.2(2) . 2_656
Cu16 Au3 Cu7 S3 -123.4(2) . .
Cu16 Au3 Cu9 Au1 -91.10(12) . .
Cu16 Au3 Cu9 Au2 -161.09(10) . .
Cu16 Au3 Cu9 Cu7 133.53(13) . .
Cu16 Au3 Cu9 Cu15 -23.92(14) . .
Cu16 Au3 Cu9 S7 -87.5(3) . .
Cu16 Au3 Cu9 S3 131.99(17) . .
Cu16 Au3 Cu9 S8 24.0(2) . .
Cu16 Au3 Cu15 Au1 -132.02(10) . .
Cu16 Au3 Cu15 Au5 -62.64(8) . .
Cu16 Au3 Cu15 Cu9 160.60(12) . .
Cu16 Au3 Cu15 Cu13 61.97(12) . .
Cu16 Au3 Cu15 S11 -57.8(3) . .
Cu16 Au3 Cu15 S8 110.23(19) . .
Cu16 Au5 Au6 Au1 -172.44(9) . 2_656
Cu16 Au5 Au6 Au2 -110.07(9) . 2_656
Cu16 Au5 Au6 Au3 -72.74(8) . .
Cu16 Au5 Au6 Au4 148.64(9) . 2_656
Cu16 Au5 Au6 Cu6 -46.30(11) . .
Cu16 Au5 Au6 Cu10 79.51(11) . .
Cu16 Au5 Au6 Cu11 -143.0(3) . 2_656
Cu16 Au5 Au6 Cu12 123.76(11) . 2_656
Cu16 Au5 Cu5 Au1 98.30(12) . .
Cu16 Au5 Cu5 Au4 170.39(11) . .
Cu16 Au5 Cu5 Cu12 135.54(13) . .
Cu16 Au5 Cu5 S10 98.9(3) . .
Cu16 Au5 Cu5 S18 -115.39(19) . .
Cu16 Au5 Cu5 S11 -9.3(2) . .
Cu16 Au5 Cu8 Au4 -167.64(10) . .
Cu16 Au5 Cu8 Au4 -94.23(11) . 2_656
Cu16 Au5 Cu8 Cu2 156.29(15) . .
Cu16 Au5 Cu8 Cu8 -133.81(14) . 2_656
Cu16 Au5 Cu8 Cu10 -26.71(13) . .
Cu16 Au5 Cu8 S18 117.33(19) . .
Cu16 Au5 Cu8 S16 -25.0(2) . .
Cu16 Au5 Cu10 Au4 -137.10(10) . 2_656
Cu16 Au5 Cu10 Au6 -67.09(9) . .
Cu16 Au5 Cu10 Cu8 157.38(12) . .
Cu16 Au5 Cu10 S9 -64.0(3) . 2_656
Cu16 Au5 Cu10 S16 155.82(19) . .
Cu16 Au5 Cu10 S15 47.2(2) . .
Cu16 Au5 Cu15 Au1 142.66(10) . .
Cu16 Au5 Cu15 Au3 69.69(9) . .
Cu16 Au5 Cu15 Cu9 107.13(13) . .
Cu16 Au5 Cu15 Cu13 6.99(13) . .
Cu16 Au5 Cu15 S11 -107.41(18) . .
Cu16 Au5 Cu15 S8 57.3(3) . .
Cu16 Au6 Cu6 Au2 -136.34(9) . 2_656
Cu16 Au6 Cu6 Au3 -66.32(8) . .
Cu16 Au6 Cu6 Cu11 158.02(11) . 2_656
Cu16 Au6 Cu6 S4 114.09(18) . 2_656
Cu16 Au6 Cu6 S2 -128.3(3) . 2_656
Cu16 Au6 Cu6 S13 7.80(18) . .
Cu16 Au6 Cu10 Au4 138.08(9) . 2_656
Cu16 Au6 Cu10 Au5 65.45(8) . .
Cu16 Au6 Cu10 Cu8 103.41(13) . .
Cu16 Au6 Cu10 S9 -112.45(17) . 2_656
Cu16 Au6 Cu10 S16 148.3(3) . .
Cu16 Au6 Cu10 S15 -2.60(19) . .
Cu16 Cu10 S16 Cu2 123.3(4) . 2_656
Cu16 Cu10 S16 Cu8 47.6(4) . .
Cu16 Cu10 S16 C106 -60.7(9) . .
Cu16 Cu10 S15 Cu14 76.0(5) . .
Cu16 Cu10 S15 C99 -114.7(12) . .
Cu16 Cu13 Cu15 Au1 -79.6(2) . .
Cu16 Cu13 Cu15 Au3 -59.80(9) . .
Cu16 Cu13 Cu15 Au5 -6.48(12) . .
Cu16 Cu13 Cu15 Cu9 -116.61(12) . .
Cu16 Cu13 Cu15 S11 84.9(2) . .
Cu16 Cu13 Cu15 S8 -149.7(2) . .
Cu16 Cu13 S8 Cu9 -38.6(4) . .
Cu16 Cu13 S8 Cu15 26.7(2) . .
Cu16 Cu13 S8 C50 133.9(10) . .
Cu16 Cu13 S13 Cu6 82.9(4) . .
Cu16 Cu13 S13 C85 -112.6(16) . .
Cu16 Cu13 S12 Au10 -37.8(5) . .
Cu16 Cu13 S12 C78 70(2) . .
Cu16 Cu15 S11 Cu5 -101.08(16) . .
Cu16 Cu15 S11 Cu14 28.9(2) . .
Cu16 Cu15 S11 C71 149.0(9) . .
Cu16 Cu15 S8 Cu9 110.04(16) . .
Cu16 Cu15 S8 Cu13 -26.9(2) . .
Cu16 Cu15 S8 C50 -138.4(10) . .
Cu16 S15 C99 C100 51.4(19) . .
Cu16 S15 C99 C104 -129.9(13) . .
Cu16 S13 C85 C86 19(2) . .
Cu16 S13 C85 C90 -164.7(17) . .
S4 Cu3 S9 Cu10 -16.4(5) . 2_656
S4 Cu3 S9 Cu12 65.7(3) . .
S4 Cu3 S9 C57 -175.2(9) . .
S4 Cu3 S5 Au9 -87.7(3) . .
S4 Cu3 S5 C29 14.1(10) . .
S4 Cu6 S13 Cu13 -175.0(4) 2_656 .
S4 Cu6 S13 Cu16 -93.2(2) 2_656 .
S4 Cu6 S13 C85 19.6(15) 2_656 .
S4 Cu11 Cu12 Au1 150.05(18) . .
S4 Cu11 Cu12 Au4 111.83(17) . .
S4 Cu11 Cu12 Au6 73.28(16) . 2_656
S4 Cu11 Cu12 Cu4 -113.94(18) . .
S4 Cu11 Cu12 Cu5 170.80(17) . .
S4 Cu11 Cu12 S9 4.8(2) . .
S4 Cu11 Cu12 S10 -137.2(2) . .
S4 Cu11 S7 Cu4 88.7(3) . .
S4 Cu11 S7 Cu9 -134.7(3) . .
S4 Cu11 S7 C43 -23.8(9) . .
S4 C22 C23 C24 -177(2) . .
S4 C22 C27 C26 178(2) . .
S9 Cu3 S4 Cu6 16.7(5) . 2_656
S9 Cu3 S4 Cu11 -62.9(3) . .
S9 Cu3 S4 C22 -176.1(11) . .
S9 Cu3 S5 Au9 102.1(2) . .
S9 Cu3 S5 C29 -156.1(10) . .
S9 Cu10 Cu16 Au3 103.51(18) 2_656 .
S9 Cu10 Cu16 Au5 142.42(18) 2_656 .
S9 Cu10 Cu16 Au6 66.27(16) 2_656 .
S9 Cu10 Cu16 Cu13 -151.0(7) 2_656 .
S9 Cu10 Cu16 Cu15 160.61(18) 2_656 .
S9 Cu10 Cu16 S15 -110.4(3) 2_656 .
S9 Cu10 Cu16 S13 6.0(4) 2_656 .
S9 Cu10 S16 Cu2 -76.1(4) 2_656 2_656
S9 Cu10 S16 Cu8 -151.9(2) 2_656 .
S9 Cu10 S16 C106 99.9(8) 2_656 .
S9 Cu10 S15 Cu14 160.6(4) 2_656 .
S9 Cu10 S15 Cu16 84.6(2) 2_656 .
S9 Cu10 S15 C99 -30.1(12) 2_656 .
S9 Cu12 S10 Cu4 -92.8(3) . .
S9 Cu12 S10 Cu5 136.1(3) . .
S9 Cu12 S10 C64 21.9(9) . .
S9 C57 C58 C59 -176.8(19) . .
S9 C57 C62 C61 179(2) . .
S10 Cu4 Cu11 Au1 -34.64(19) . .
S10 Cu4 Cu11 Au2 -60.5(3) . .
S10 Cu4 Cu11 Au6 16.9(2) . 2_656
S10 Cu4 Cu11 Cu6 75.4(5) . 2_656
S10 Cu4 Cu11 Cu12 23.67(18) . .
S10 Cu4 Cu11 S4 113.1(3) . .
S10 Cu4 Cu11 S7 -121.3(3) . .
S10 Cu4 Cu12 Au1 -90.8(2) . .
S10 Cu4 Cu12 Au4 -65.5(3) . .
S10 Cu4 Cu12 Au6 -140.9(2) . 2_656
S10 Cu4 Cu12 Cu5 -35.8(2) . .
S10 Cu4 Cu12 Cu11 -147.7(2) . .
S10 Cu4 Cu12 S9 124.9(3) . .
S10 Cu4 S7 Cu9 0.5(5) . .
S10 Cu4 S7 Cu11 76.3(3) . .
S10 Cu4 S7 C43 -167.0(10) . .
S10 Cu4 S6 Au9 -85.3(3) . .
S10 Cu4 S6 C36 20.5(10) . .
S10 Cu5 Cu12 Au1 111.6(2) . .
S10 Cu5 Cu12 Au4 -171.4(2) . .
S10 Cu5 Cu12 Au6 149.6(2) . 2_656
S10 Cu5 Cu12 Cu4 33.12(19) . .
S10 Cu5 Cu12 Cu11 90.7(2) . .
S10 Cu5 Cu12 S9 -115.2(4) . .
S10 Cu5 S18 Cu2 66.8(4) . .
S10 Cu5 S18 Cu8 147.2(2) . .
S10 Cu5 S18 C120 -98.2(9) . .
S10 Cu5 S11 Cu14 179.9(3) . .
S10 Cu5 S11 Cu15 -92.1(2) . .
S10 Cu5 S11 C71 26.9(9) . .
S10 Cu12 S9 Cu3 91.8(3) . .
S10 Cu12 S9 Cu10 -135.0(3) . 2_656
S10 Cu12 S9 C57 -23.1(9) . .
S10 C64 C65 C66 -178(2) . .
S10 C64 C69 C68 179.6(19) . .
S7 Cu4 Cu11 Au1 86.7(2) . .
S7 Cu4 Cu11 Au2 60.8(3) . .
S7 Cu4 Cu11 Au6 138.2(2) . 2_656
S7 Cu4 Cu11 Cu6 -163.3(5) . 2_656
S7 Cu4 Cu11 Cu12 145.0(2) . .
S7 Cu4 Cu11 S4 -125.6(3) . .
S7 Cu4 Cu12 Au1 31.13(19) . .
S7 Cu4 Cu12 Au4 56.4(3) . .
S7 Cu4 Cu12 Au6 -19.0(2) . 2_656
S7 Cu4 Cu12 Cu5 86.2(2) . .
S7 Cu4 Cu12 Cu11 -25.74(19) . .
S7 Cu4 Cu12 S9 -113.1(3) . .
S7 Cu4 Cu12 S10 121.9(3) . .
S7 Cu4 S10 Cu5 0.8(5) . .
S7 Cu4 S10 Cu12 -75.1(3) . .
S7 Cu4 S10 C64 170.9(10) . .
S7 Cu4 S6 Au9 105.6(3) . .
S7 Cu4 S6 C36 -148.6(9) . .
S7 Cu9 Cu15 Au1 66.71(16) . .
S7 Cu9 Cu15 Au3 143.14(18) . .
S7 Cu9 Cu15 Au5 103.51(18) . .
S7 Cu9 Cu15 Cu13 -140.27(18) . .
S7 Cu9 Cu15 Cu16 161.21(18) . .
S7 Cu9 Cu15 S11 4.1(4) . .
S7 Cu9 Cu15 S8 -109.9(3) . .
S7 Cu9 S3 Cu1 -76.2(3) . .
S7 Cu9 S3 Cu7 -152.4(2) . .
S7 Cu9 S3 C15 100.0(9) . .
S7 Cu9 S8 Cu13 152.9(4) . .
S7 Cu9 S8 Cu15 85.4(2) . .
S7 Cu9 S8 C50 -19.4(10) . .
S7 Cu11 Cu12 Au1 -70.28(17) . .
S7 Cu11 Cu12 Au4 -108.50(18) . .
S7 Cu11 Cu12 Au6 -147.05(19) . 2_656
S7 Cu11 Cu12 Cu4 25.73(17) . .
S7 Cu11 Cu12 Cu5 -49.53(19) . .
S7 Cu11 Cu12 S9 144.4(2) . .
S7 Cu11 Cu12 S10 2.5(2) . .
S7 Cu11 S4 Cu3 -96.3(3) . .
S7 Cu11 S4 Cu6 137.1(3) . 2_656
S7 Cu11 S4 C22 22.0(10) . .
S7 C43 C44 C45 -173(2) . .
S7 C43 C48 C47 171(2) . .
S2 Cu1 S3 Cu7 67.8(3) . .
S2 Cu1 S3 Cu9 -3.5(5) . .
S2 Cu1 S3 C15 180.0(8) . .
S2 Cu1 S1 Au7 -106.8(2) . .
S2 Cu1 S1 C1 144.6(8) . .
S2 Cu6 S13 Cu13 62.8(5) 2_656 .
S2 Cu6 S13 Cu16 144.6(2) 2_656 .
S2 Cu6 S13 C85 -102.6(15) 2_656 .
S2 Cu7 Cu9 Au1 -101.1(3) 2_656 .
S2 Cu7 Cu9 Au2 -138.1(3) 2_656 .
S2 Cu7 Cu9 Au3 -61.2(3) 2_656 .
S2 Cu7 Cu9 Cu15 -41.7(3) 2_656 .
S2 Cu7 Cu9 S7 169.1(4) 2_656 .
S2 Cu7 Cu9 S3 116.8(3) 2_656 .
S2 Cu7 Cu9 S8 9.0(3) 2_656 .
S2 Cu7 S3 Cu1 98.4(3) 2_656 .
S2 Cu7 S3 Cu9 -128.3(3) 2_656 .
S2 Cu7 S3 C15 -9.7(8) 2_656 .
S2 C8 C13 C12 173(2) . .
S18 Cu2 Cu8 Au4 -88.7(2) . .
S18 Cu2 Cu8 Au4 -137.3(2) . 2_656
S18 Cu2 Cu8 Au5 -56.9(2) . .
S18 Cu2 Cu8 Cu8 -146.4(2) . 2_656
S18 Cu2 Cu8 Cu10 139.3(9) . .
S18 Cu2 Cu8 S16 124.4(3) . .
S18 Cu2 S17 Au8 -110.4(2) . .
S18 Cu2 S17 C113 144.5(10) . .
S18 Cu5 Cu12 Au1 -142.63(18) . .
S18 Cu5 Cu12 Au4 -65.59(16) . .
S18 Cu5 Cu12 Au6 -104.57(17) . 2_656
S18 Cu5 Cu12 Cu4 138.94(17) . .
S18 Cu5 Cu12 Cu11 -163.52(17) . .
S18 Cu5 Cu12 S9 -9.4(4) . .
S18 Cu5 Cu12 S10 105.8(2) . .
S18 Cu5 S10 Cu4 -169.6(3) . .
S18 Cu5 S10 Cu12 -91.7(2) . .
S18 Cu5 S10 C64 20.4(10) . .
S18 Cu5 S11 Cu14 58.6(4) . .
S18 Cu5 S11 Cu15 146.6(2) . .
S18 Cu5 S11 C71 -94.5(9) . .
S18 Cu8 Cu10 Au4 -138.0(3) . 2_656
S18 Cu8 Cu10 Au5 -61.5(3) . .
S18 Cu8 Cu10 Au6 -101.2(3) . .
S18 Cu8 Cu10 Cu16 -41.9(3) . .
S18 Cu8 Cu10 S9 169.2(4) . 2_656
S18 Cu8 Cu10 S16 116.5(3) . .
S18 Cu8 Cu10 S15 8.1(4) . .
S18 Cu8 S16 Cu2 100.5(3) . 2_656
S18 Cu8 S16 Cu10 -126.9(3) . .
S18 Cu8 S16 C106 -8.4(9) . .
S18 C120 C125 C124 177.9(18) . .
S3 Cu1 S2 Cu6 14.3(4) . 2_656
S3 Cu1 S2 Cu7 -70.3(3) . 2_656
S3 Cu1 S2 C8 173.9(10) . .
S3 Cu1 S1 Au7 81.4(3) . .
S3 Cu1 S1 C1 -27.2(9) . .
S3 Cu7 Cu9 Au1 142.0(2) . .
S3 Cu7 Cu9 Au2 105.13(19) . .
S3 Cu7 Cu9 Au3 -178.0(2) . .
S3 Cu7 Cu9 Cu15 -158.5(2) . .
S3 Cu7 Cu9 S7 52.3(4) . .
S3 Cu7 Cu9 S8 -107.8(2) . .
S3 Cu9 Cu15 Au1 -131.3(4) . .
S3 Cu9 Cu15 Au3 -54.9(3) . .
S3 Cu9 Cu15 Au5 -94.5(4) . .
S3 Cu9 Cu15 Cu13 21.7(4) . .
S3 Cu9 Cu15 Cu16 -36.8(4) . .
S3 Cu9 Cu15 S11 166.1(4) . .
S3 Cu9 Cu15 S8 52.1(4) . .
S3 Cu9 S7 Cu4 161.3(4) . .
S3 Cu9 S7 Cu11 85.6(2) . .
S3 Cu9 S7 C43 -31.0(10) . .
S3 Cu9 S8 Cu13 -88.7(4) . .
S3 Cu9 S8 Cu15 -156.21(19) . .
S3 Cu9 S8 C50 99.0(10) . .
S16 Cu2 Cu8 Au4 39.31(17) 2_656 .
S16 Cu2 Cu8 Au4 -9.2(2) 2_656 2_656
S16 Cu2 Cu8 Au5 71.1(2) 2_656 .
S16 Cu2 Cu8 Cu8 -18.32(16) 2_656 2_656
S16 Cu2 Cu8 Cu10 -92.7(9) 2_656 .
S16 Cu2 Cu8 S18 128.1(3) 2_656 .
S16 Cu2 Cu8 S16 -107.59(19) 2_656 .
S16 Cu2 S18 Cu5 12.6(4) 2_656 .
S16 Cu2 S18 Cu8 -70.6(3) 2_656 .
S16 Cu2 S18 C120 177.0(8) 2_656 .
S16 Cu2 S17 Au8 78.4(3) 2_656 .
S16 Cu2 S17 C113 -26.6(10) 2_656 .
S16 Cu8 Cu10 Au4 105.49(19) . 2_656
S16 Cu8 Cu10 Au5 -178.0(2) . .
S16 Cu8 Cu10 Au6 142.2(2) . .
S16 Cu8 Cu10 Cu16 -158.4(2) . .
S16 Cu8 Cu10 S9 52.6(4) . 2_656
S16 Cu8 Cu10 S15 -108.4(3) . .
S16 Cu8 S18 Cu2 -89.3(3) . .
S16 Cu8 S18 Cu5 141.5(3) . .
S16 Cu8 S18 C120 27.4(9) . .
S16 Cu10 Cu16 Au3 -95.5(4) . .
S16 Cu10 Cu16 Au5 -56.6(4) . .
S16 Cu10 Cu16 Au6 -132.7(4) . .
S16 Cu10 Cu16 Cu13 10.0(9) . .
S16 Cu10 Cu16 Cu15 -38.4(4) . .
S16 Cu10 Cu16 S15 50.6(4) . .
S16 Cu10 Cu16 S13 167.1(4) . .
S16 Cu10 S15 Cu14 -81.1(5) . .
S16 Cu10 S15 Cu16 -157.1(2) . .
S16 Cu10 S15 C99 88.2(12) . .
S16 C106 C111 C110 -179.7(18) . .
S16 C106 C107 C108 -177(2) . .
S11 Cu5 Cu12 Au1 56.3(3) . .
S11 Cu5 Cu12 Au4 133.3(3) . .
S11 Cu5 Cu12 Au6 94.3(3) . 2_656
S11 Cu5 Cu12 Cu4 -22.2(3) . .
S11 Cu5 Cu12 Cu11 35.4(3) . .
S11 Cu5 Cu12 S9 -170.5(4) . .
S11 Cu5 Cu12 S10 -55.3(3) . .
S11 Cu5 S10 Cu4 72.5(4) . .
S11 Cu5 S10 Cu12 150.4(2) . .
S11 Cu5 S10 C64 -97.5(10) . .
S11 Cu5 S18 Cu2 -174.5(3) . .
S11 Cu5 S18 Cu8 -94.1(2) . .
S11 Cu5 S18 C120 20.6(9) . .
S11 Cu14 S15 Cu10 -4.7(7) . .
S11 Cu14 S15 Cu16 67.6(4) . .
S11 Cu14 S15 C99 -174.1(12) . .
S11 Cu14 S14 Au10 -91.1(4) . .
S11 Cu14 S14 C92 11.6(13) . .
S11 Cu15 Cu16 Au3 149.20(19) . .
S11 Cu15 Cu16 Au5 72.15(17) . .
S11 Cu15 Cu16 Au6 115.52(18) . .
S11 Cu15 Cu16 Cu10 54.1(2) . .
S11 Cu15 Cu16 Cu13 -115.2(2) . .
S11 Cu15 Cu16 S15 0.1(3) . .
S11 Cu15 Cu16 S13 -140.8(2) . .
S11 Cu15 S8 Cu9 -135.1(3) . .
S11 Cu15 S8 Cu13 88.0(3) . .
S11 Cu15 S8 C50 -23.5(11) . .
S11 C71 C76 C75 179(2) . .
S11 C71 C72 C73 -174(3) . .
S15 Cu10 Cu16 Au3 -146.1(2) . .
S15 Cu10 Cu16 Au5 -107.2(2) . .
S15 Cu10 Cu16 Au6 176.7(2) . .
S15 Cu10 Cu16 Cu13 -40.6(7) . .
S15 Cu10 Cu16 Cu15 -89.0(2) . .
S15 Cu10 Cu16 S13 116.4(4) . .
S15 Cu10 S16 Cu2 161.8(3) . 2_656
S15 Cu10 S16 Cu8 86.1(2) . .
S15 Cu10 S16 C106 -22.2(8) . .
S15 Cu14 S11 Cu5 15.3(5) . .
S15 Cu14 S11 Cu15 -69.4(4) . .
S15 Cu14 S11 C71 167.3(9) . .
S15 Cu14 S14 Au10 100.8(3) . .
S15 Cu14 S14 C92 -156.5(11) . .
S15 Cu16 S13 Cu6 141.1(3) . .
S15 Cu16 S13 Cu13 -89.8(4) . .
S15 Cu16 S13 C85 29.2(14) . .
S15 C99 C104 C103 -179(2) . .
S8 Cu9 Cu15 Au1 176.6(2) . .
S8 Cu9 Cu15 Au3 -107.0(2) . .
S8 Cu9 Cu15 Au5 -146.6(2) . .
S8 Cu9 Cu15 Cu13 -30.4(2) . .
S8 Cu9 Cu15 Cu16 -88.9(2) . .
S8 Cu9 Cu15 S11 114.0(4) . .
S8 Cu9 S7 Cu4 -78.3(4) . .
S8 Cu9 S7 Cu11 -154.0(2) . .
S8 Cu9 S7 C43 89.3(10) . .
S8 Cu9 S3 Cu1 162.2(3) . .
S8 Cu9 S3 Cu7 85.9(2) . .
S8 Cu9 S3 C15 -21.7(9) . .
S8 Cu13 Cu15 Au1 70.1(3) . .
S8 Cu13 Cu15 Au3 89.9(2) . .
S8 Cu13 Cu15 Au5 143.2(2) . .
S8 Cu13 Cu15 Cu9 33.1(2) . .
S8 Cu13 Cu15 Cu16 149.7(2) . .
S8 Cu13 Cu15 S11 -125.4(3) . .
S8 Cu13 Cu16 Au3 32.3(2) . .
S8 Cu13 Cu16 Au5 -16.2(3) . .
S8 Cu13 Cu16 Au6 60.4(3) . .
S8 Cu13 Cu16 Cu10 -76.4(7) . .
S8 Cu13 Cu16 Cu15 -23.2(2) . .
S8 Cu13 Cu16 S15 -112.0(3) . .
S8 Cu13 Cu16 S13 121.7(3) . .
S8 Cu13 S13 Cu6 4.7(6) . .
S8 Cu13 S13 Cu16 -78.2(4) . .
S8 Cu13 S13 C85 169.1(16) . .
S8 Cu13 S12 Au10 103.7(4) . .
S8 Cu13 S12 C78 -148.6(19) . .
S8 Cu15 Cu16 Au3 -73.08(18) . .
S8 Cu15 Cu16 Au5 -150.1(2) . .
S8 Cu15 Cu16 Au6 -106.76(19) . .
S8 Cu15 Cu16 Cu10 -168.15(19) . .
S8 Cu15 Cu16 Cu13 22.56(18) . .
S8 Cu15 Cu16 S15 137.8(3) . .
S8 Cu15 Cu16 S13 -3.1(3) . .
S8 Cu15 S11 Cu5 142.1(3) . .
S8 Cu15 S11 Cu14 -87.9(3) . .
S8 Cu15 S11 C71 32.2(10) . .
S8 C50 C51 C52 -179(2) . .
S8 C50 C55 C54 178(3) . .
S13 Cu13 Cu15 Au1 -54.2(3) . .
S13 Cu13 Cu15 Au3 -34.4(2) . .
S13 Cu13 Cu15 Au5 18.9(3) . .
S13 Cu13 Cu15 Cu9 -91.2(2) . .
S13 Cu13 Cu15 Cu16 25.4(2) . .
S13 Cu13 Cu15 S11 110.3(3) . .
S13 Cu13 Cu15 S8 -124.3(3) . .
S13 Cu13 Cu16 Au3 -89.4(2) . .
S13 Cu13 Cu16 Au5 -137.9(3) . .
S13 Cu13 Cu16 Au6 -61.3(3) . .
S13 Cu13 Cu16 Cu10 161.9(7) . .
S13 Cu13 Cu16 Cu15 -144.9(3) . .
S13 Cu13 Cu16 S15 126.3(3) . .
S13 Cu13 S8 Cu9 9.1(6) . .
S13 Cu13 S8 Cu15 74.4(4) . .
S13 Cu13 S8 C50 -178.4(10) . .
S13 Cu13 S12 Au10 -94.5(4) . .
S13 Cu13 S12 C78 13(2) . .
S13 Cu16 S15 Cu10 -132.1(3) . .
S13 Cu16 S15 Cu14 90.5(4) . .
S13 Cu16 S15 C99 -22.4(13) . .
S13 C85 C86 C87 177(3) . .
S13 C85 C90 C89 -176(3) . .
S17 Au8 Cu2 Cu8 -44.4(2) 2_656 .
S17 Au8 Cu2 Cu8 135.2(2) . .
S17 Au8 Cu2 S18 92.0(3) . .
S17 Au8 Cu2 S18 -87.6(3) 2_656 .
S17 Au8 Cu2 S16 55.9(3) 2_656 2_656
S17 Au8 Cu2 S16 -124.5(3) . 2_656
S17 Au8 Cu2 S17 -179.61(7) 2_656 .
S17 Au8 S17 Cu2 10.39(19) 2_656 .
S17 Au8 S17 C113 118.1(10) 2_656 .
S17 Cu2 Cu8 Au4 -175.6(3) . .
S17 Cu2 Cu8 Au4 135.8(3) . 2_656
S17 Cu2 Cu8 Au5 -143.8(3) . .
S17 Cu2 Cu8 Cu8 126.7(3) . 2_656
S17 Cu2 Cu8 Cu10 52.4(10) . .
S17 Cu2 Cu8 S18 -86.9(3) . .
S17 Cu2 Cu8 S16 37.5(3) . .
S17 Cu2 S18 Cu5 -158.6(3) . .
S17 Cu2 S18 Cu8 118.1(2) . .
S17 Cu2 S18 C120 5.7(9) . .
S17 C113 C114 C115 177.9(19) . .
S17 C113 C118 C117 -175(2) . .
S1 Au7 Cu1 Cu7 137.1(2) . 2_656
S1 Au7 Cu1 Cu7 -42.4(2) 2_656 2_656
S1 Au7 Cu1 S2 94.6(3) . .
S1 Au7 Cu1 S2 -84.9(3) 2_656 .
S1 Au7 Cu1 S3 -122.0(3) . .
S1 Au7 Cu1 S3 58.5(3) 2_656 .
S1 Au7 Cu1 S1 -179.50(7) 2_656 .
S1 Au7 S1 Cu1 9.05(16) 2_656 .
S1 Au7 S1 C1 118.3(8) 2_656 .
S1 Cu1 S2 Cu6 -157.4(3) . 2_656
S1 Cu1 S2 Cu7 117.9(2) . 2_656
S1 Cu1 S2 C8 2.1(10) . .
S1 Cu1 S3 Cu7 -121.6(3) . .
S1 Cu1 S3 Cu9 167.1(3) . .
S1 Cu1 S3 C15 -9.5(8) . .
S1 C1 C2 C3 -175.6(19) . .
S5 Au9 Cu3 S4 119.0(3) . .
S5 Au9 Cu3 S9 -100.3(3) . .
S5 Au9 Cu4 Cu11 38.5(3) . .
S5 Au9 Cu4 Cu12 -20.2(3) . .
S5 Au9 Cu4 S10 -62.5(3) . .
S5 Au9 Cu4 S7 79.9(3) . .
S5 Au9 Cu4 S6 176.5(4) . .
S5 Au9 S6 Cu4 -101(5) . .
S5 Au9 S6 C36 149(5) . .
S5 Cu3 S4 Cu6 -152.4(3) . 2_656
S5 Cu3 S4 Cu11 128.1(3) . .
S5 Cu3 S4 C22 14.9(12) . .
S5 Cu3 S9 Cu10 153.8(4) . 2_656
S5 Cu3 S9 Cu12 -124.1(3) . .
S5 Cu3 S9 C57 -4.9(10) . .
S5 C29 C34 C33 -177(2) . .
S5 C29 C30 C31 -179(3) . .
S6 Au9 Cu3 S4 -57.8(3) . .
S6 Au9 Cu3 S9 82.9(3) . .
S6 Au9 Cu3 S5 -176.8(3) . .
S6 Au9 Cu4 Cu11 -138.1(3) . .
S6 Au9 Cu4 Cu12 163.3(3) . .
S6 Au9 Cu4 S10 121.0(3) . .
S6 Au9 Cu4 S7 -96.6(3) . .
S6 Au9 S5 Cu3 86(5) . .
S6 Au9 S5 C29 -21(5) . .
S6 Cu4 Cu11 Au1 178.9(3) . .
S6 Cu4 Cu11 Au2 153.0(3) . .
S6 Cu4 Cu11 Au6 -129.6(3) . 2_656
S6 Cu4 Cu11 Cu6 -71.1(5) . 2_656
S6 Cu4 Cu11 Cu12 -122.8(3) . .
S6 Cu4 Cu11 S4 -33.4(3) . .
S6 Cu4 Cu11 S7 92.2(3) . .
S6 Cu4 Cu12 Au1 163.6(3) . .
S6 Cu4 Cu12 Au4 -171.1(3) . .
S6 Cu4 Cu12 Au6 113.5(3) . 2_656
S6 Cu4 Cu12 Cu5 -141.3(3) . .
S6 Cu4 Cu12 Cu11 106.8(3) . .
S6 Cu4 Cu12 S9 19.4(4) . .
S6 Cu4 Cu12 S10 -105.6(4) . .
S6 Cu4 S10 Cu5 -167.5(3) . .
S6 Cu4 S10 Cu12 116.6(3) . .
S6 Cu4 S10 C64 2.6(11) . .
S6 Cu4 S7 Cu9 170.4(4) . .
S6 Cu4 S7 Cu11 -113.8(3) . .
S6 Cu4 S7 C43 2.9(10) . .
S6 C36 C41 C40 176(2) . .
S6 C36 C37 C38 -176(3) . .
S14 Au10 Cu13 Cu15 36.2(4) . .
S14 Au10 Cu13 Cu16 -23.5(4) . .
S14 Au10 Cu13 S8 81.7(5) . .
S14 Au10 Cu13 S13 -66.2(5) . .
S14 Au10 Cu13 S12 -176.2(5) . .
S14 Au10 Cu14 S11 122.3(4) . .
S14 Au10 Cu14 S15 -99.6(4) . .
S14 Au10 S12 Cu13 150(4) . .
S14 Au10 S12 C78 27(5) . .
S14 Cu14 S11 Cu5 -151.9(5) . .
S14 Cu14 S11 Cu15 123.4(5) . .
S14 Cu14 S11 C71 0.0(11) . .
S14 Cu14 S15 Cu10 164.8(5) . .
S14 Cu14 S15 Cu16 -122.8(4) . .
S14 Cu14 S15 C99 -4.6(13) . .
S14 C92 C97 C96 -178(2) . .
S12 Au10 Cu13 Cu15 -147.6(4) . .
S12 Au10 Cu13 Cu16 152.7(4) . .
S12 Au10 Cu13 S8 -102.1(4) . .
S12 Au10 Cu13 S13 110.0(4) . .
S12 Au10 Cu14 S11 -60.4(4) . .
S12 Au10 Cu14 S15 77.6(4) . .
S12 Au10 Cu14 S14 177.3(5) . .
S12 Au10 S14 Cu14 -158(4) . .
S12 Au10 S14 C92 85(4) . .
S12 Cu13 Cu15 Au1 160.0(4) . .
S12 Cu13 Cu15 Au3 179.8(5) . .
S12 Cu13 Cu15 Au5 -126.9(4) . .
S12 Cu13 Cu15 Cu9 123.0(5) . .
S12 Cu13 Cu15 Cu16 -120.4(5) . .
S12 Cu13 Cu15 S11 -35.5(5) . .
S12 Cu13 Cu15 S8 89.9(5) . .
S12 Cu13 Cu16 Au3 177.1(4) . .
S12 Cu13 Cu16 Au5 128.6(4) . .
S12 Cu13 Cu16 Au6 -154.8(4) . .
S12 Cu13 Cu16 Cu10 68.4(8) . .
S12 Cu13 Cu16 Cu15 121.6(4) . .
S12 Cu13 Cu16 S15 32.8(5) . .
S12 Cu13 Cu16 S13 -93.5(5) . .
S12 Cu13 S8 Cu9 170.1(5) . .
S12 Cu13 S8 Cu15 -124.6(4) . .
S12 Cu13 S8 C50 -17.4(11) . .
S12 Cu13 S13 Cu6 -155.8(5) . .
S12 Cu13 S13 Cu16 121.3(4) . .
S12 Cu13 S13 C85 8.7(17) . .
C43 C44 C45 C46 4(4) . .
C6 C5 C4 C3 -2(4) . .
C6 C5 C4 C7 177(2) . .
C6 C1 C2 C3 0(4) . .
C22 C23 C24 C25 -2(4) . .
C22 C27 C26 C25 -1(4) . .
C64 C65 C66 C67 -7(4) . .
C57 C58 C59 C60 0(4) . .
C57 C62 C61 C60 -4(6) . .
C106 C111 C110 C109 0(4) . .
C106 C107 C108 C109 -7(5) . .
C44 C43 C48 C47 -2(4) . .
C44 C45 C46 C47 -5(4) . .
C44 C45 C46 C49 174(2) . .
C116 C117 C118 C113 0(4) . .
C71 C76 C75 C74 -2(5) . .
C71 C72 C73 C74 -8(6) . .
C9 C8 C13 C12 -4(4) . .
C9 C10 C11 C12 0(5) . .
C9 C10 C11 C14 178(3) . .
C119 C116 C117 C118 179(2) . .
C119 C116 C115 C114 -176(2) . .
C111 C106 C107 C108 3(4) . .
C111 C110 C109 C108 -4(4) . .
C111 C110 C109 C112 179(3) . .
C8 C9 C10 C11 0(4) . .
C23 C22 C27 C26 0(4) . .
C3 C4 C7 F1 -10(4) . .
C3 C4 C7 F3 112(3) . .
C3 C4 C7 F2 -127(3) . .
C45 C46 C49 F19 162(3) . .
C45 C46 C49 F20 41(3) . .
C45 C46 C49 F21 -76(4) . .
C5 C6 C1 S1 173.0(17) . .
C5 C6 C1 C2 -2(3) . .
C5 C4 C7 F1 171(2) . .
C5 C4 C7 F3 -66(3) . .
C5 C4 C7 F2 54(4) . .
C36 C41 C40 C39 -1(5) . .
C36 C37 C38 C39 1(7) . .
C76 C71 C72 C73 3(5) . .
C76 C75 C74 C73 -3(6) . .
C76 C75 C74 C77 178(4) . .
C102 C101 C100 C99 0.0 . .
C101 C102 C103 C104 0.0 . .
C101 C102 C105 F44 60(2) . .
C101 C102 C105 F43 177(2) . .
C101 C102 C105 F45 -61(3) . .
C101 C100 C99 S15 179(2) . .
C101 C100 C99 C104 0.0 . .
C100 C99 C104 C103 0.0 . .
C99 C104 C103 C102 0.0 . .
C103 C102 C101 C100 0.0 . .
C103 C102 C105 F44 -125(2) . .
C103 C102 C105 F43 -7(3) . .
C103 C102 C105 F45 115(3) . .
C113 C114 C115 C116 -6(4) . .
C114 C113 C118 C117 2(4) . .
C121 C120 C125 C124 1(4) . .
C50 C51 C52 C53 -3(5) . .
C50 C55 C54 C53 5(6) . .
C47 C46 C49 F19 -20(4) . .
C47 C46 C49 F20 -140(3) . .
C47 C46 C49 F21 103(3) . .
C4 C3 C2 C1 2(4) . .
C10 C9 C8 S2 -175(2) . .
C10 C9 C8 C13 2(3) . .
C10 C11 C14 F6 -4(5) . .
C10 C11 C14 F4 -120(5) . .
C10 C11 C14 F5 108(5) . .
C27 C22 C23 C24 1(4) . .
C27 C26 C25 C24 1(4) . .
C27 C26 C25 C28 -171(3) . .
C110 C109 C112 F46 57(4) . .
C110 C109 C112 F47 -55(4) . .
C110 C109 C112 F48 178(3) . .
C16 C17 C18 C19 -3(4) . .
C16 C17 C18 C21 180(3) . .
C1 C6 C5 C4 3(4) . .
C58 C57 C62 C61 -1(4) . .
C58 C59 C60 C61 -4(4) . .
C58 C59 C60 C63 174(3) . .
C48 C43 C44 C45 -1(4) . .
C48 C47 C46 C45 2(4) . .
C48 C47 C46 C49 -176(3) . .
C107 C106 C111 C110 0(4) . .
C107 C108 C109 C110 7(5) . .
C107 C108 C109 C112 -176(3) . .
C120 C121 C122 C123 2(4) . .
C120 C125 C124 C123 -4(4) . .
N2 C147 C148 C149 178(3) . .
N2 C143 C144 C145 -159(4) . .
C117 C116 C119 F50 -3(3) . .
C117 C116 C119 F49 116(3) . .
C117 C116 C119 F51 -127(3) . .
C117 C116 C115 C114 7(4) . .
C65 C64 C69 C68 -4(4) . .
C15 C20 C19 C18 -5(4) . .
C15 C16 C17 C18 1(4) . .
C68 C67 C66 C65 7(5) . .
C68 C67 C70 F30 -158(3) . .
C68 C67 C70 F29 80(4) . .
C68 C67 C70 F28 -42(5) . .
C59 C60 C61 C62 6(5) . .
C59 C60 C63 F27 159(4) . .
C59 C60 C63 F25 38(5) . .
C59 C60 C63 F26 -83(6) . .
C26 C25 C24 C23 1(4) . .
C26 C25 C28 F10 -139(3) . .
C26 C25 C28 F12 104(3) . .
C26 C25 C28 F11 -22(4) . .
C67 C68 C69 C64 4(4) . .
C46 C47 C48 C43 1(4) . .
C69 C64 C65 C66 5(4) . .
C69 C68 C67 C66 -6(4) . .
C69 C68 C67 C70 -173(3) . .
C24 C25 C28 F10 49(3) . .
C24 C25 C28 F12 -68(4) . .
C24 C25 C28 F11 166(3) . .
C122 C121 C120 S18 -177(2) . .
C122 C121 C120 C125 0(4) . .
C122 C123 C124 C125 7(4) . .
C122 C123 C126 F52 -85(4) . .
C122 C123 C126 F53 161(3) . .
C122 C123 C126 F54 32(5) . .
C66 C67 C70 F30 35(5) . .
C66 C67 C70 F29 -87(5) . .
C66 C67 C70 F28 151(3) . .
C115 C116 C119 F50 -179(2) . .
C115 C116 C119 F49 -61(3) . .
C115 C116 C119 F51 56(3) . .
C115 C116 C117 C118 -4(4) . .
C85 C86 C87 C88 0.0 . .
C86 C85 C90 C89 0.0 . .
C86 C87 C88 C89 0.0 . .
C86 C87 C88 C91 177(3) . .
C87 C88 C89 C90 0.0 . .
C87 C88 C91 F39 155(2) . .
C87 C88 C91 F38 -87(2) . .
C87 C88 C91 F37 30(3) . .
C88 C89 C90 C85 0.0 . .
C89 C88 C91 F39 -28(3) . .
C89 C88 C91 F38 90(2) . .
C89 C88 C91 F37 -153(2) . .
C90 C85 C86 C87 0.0 . .
C124 C123 C122 C121 -6(4) . .
C124 C123 C126 F52 100(3) . .
C124 C123 C126 F53 -14(5) . .
C124 C123 C126 F54 -143(4) . .
C2 C3 C4 C5 -1(4) . .
C2 C3 C4 C7 -179(3) . .
C17 C16 C15 S3 179.9(19) . .
C17 C16 C15 C20 0(4) . .
C17 C18 C19 C20 5(4) . .
C17 C18 C21 F7 160(3) . .
C17 C18 C21 F8 43(4) . .
C17 C18 C21 F9 -80(5) . .
C118 C113 C114 C115 1(4) . .
C29 C34 C33 C32 -8(5) . .
C29 C30 C31 C32 2(5) . .
C108 C109 C112 F46 -120(4) . .
C108 C109 C112 F47 128(3) . .
C108 C109 C112 F48 1(5) . .
C62 C57 C58 C59 3(4) . .
C12 C11 C14 F6 174(3) . .
C12 C11 C14 F4 58(6) . .
C12 C11 C14 F5 -74(5) . .
C51 C50 C55 C54 -5(5) . .
C51 C52 C53 C54 3(5) . .
C51 C52 C53 C56 176(4) . .
C72 C71 C76 C75 3(4) . .
C72 C73 C74 C75 8(6) . .
C72 C73 C74 C77 -172(4) . .
C13 C12 C11 C10 -2(5) . .
C13 C12 C11 C14 179(3) . .
C11 C12 C13 C8 4(5) . .
C34 C29 C30 C31 -4(5) . .
C75 C74 C77 F33 -108(8) . .
C75 C74 C77 F31 13(7) . .
C75 C74 C77 F32 121(7) . .
C75 C74 C77 F33A -66(9) . .
C75 C74 C77 F32A 180(4) . .
C75 C74 C77 F31A 58(11) . .
C19 C20 C15 S3 -178(2) . .
C19 C20 C15 C16 2(4) . .
C19 C18 C21 F7 -17(5) . .
C19 C18 C21 F8 -134(3) . .
C19 C18 C21 F9 103(4) . .
C41 C36 C37 C38 -2(6) . .
C41 C40 C39 C38 0(6) . .
C41 C40 C39 C42 -177(3) . .
C55 C50 C51 C52 4(5) . .
C61 C60 C63 F27 -24(7) . .
C61 C60 C63 F25 -145(4) . .
C61 C60 C63 F26 94(5) . .
C52 C53 C54 C55 -4(6) . .
C52 C53 C56 F24 53(7) . .
C52 C53 C56 F23 -68(6) . .
C52 C53 C56 F22 175(5) . .
C52 C53 C56 F23A -125(6) . .
C52 C53 C56 F22A 124(5) . .
C52 C53 C56 F24A 22(7) . .
C126 C123 C122 C121 179(3) . .
C126 C123 C124 C125 -178(3) . .
C73 C74 C77 F33 72(9) . .
C73 C74 C77 F31 -167(4) . .
C73 C74 C77 F32 -59(8) . .
C73 C74 C77 F33A 115(9) . .
C73 C74 C77 F32A 0(6) . .
C73 C74 C77 F31A -122(10) . .
C54 C53 C56 F24 -134(5) . .
C54 C53 C56 F23 104(6) . .
C54 C53 C56 F22 -13(8) . .
C54 C53 C56 F23A 48(8) . .
C54 C53 C56 F22A -63(6) . .
C54 C53 C56 F24A -166(5) . .
C40 C39 C38 C37 0(7) . .
C40 C39 C42 F16 -161(4) . .
C40 C39 C42 F17 84(5) . .
C40 C39 C42 F18 -46(6) . .
C30 C29 C34 C33 8(4) . .
C33 C32 C31 C30 -2(6) . .
C33 C32 C35 F14 24(5) . .
C33 C32 C35 F15 153(4) . .
C33 C32 C35 F13 -90(5) . .
C21 C18 C19 C20 -178(3) . .
C28 C25 C24 C23 173(3) . .
C147 N2 C155 C157 49(4) . .
C147 N2 C143 C144 -160(4) . .
C147 N2 C151 C152 69(5) . .
C147 C148 C149 C150 167(4) . .
C70 C67 C66 C65 174(3) . .
C31 C32 C33 C34 5(6) . .
C31 C32 C35 F14 -159(3) . .
C31 C32 C35 F15 -30(6) . .
C31 C32 C35 F13 87(4) . .
C37 C36 C41 C40 2(4) . .
C38 C39 C42 F16 22(6) . .
C38 C39 C42 F17 -92(6) . .
C38 C39 C42 F18 137(5) . .
C42 C39 C38 C37 177(4) . .
C141 C140 C139 N1 -148(4) . .
C93 C92 C97 C96 0.0 . .
C92 C93 C94 C95 0.0 . .
C92 C97 C96 C95 0.0 . .
C97 C96 C95 C94 0.0 . .
C97 C96 C95 C98 -174(3) . .
C96 C95 C94 C93 0.0 . .
C96 C95 C98 F40 116(2) . .
C96 C95 C98 F41 -124(2) . .
C96 C95 C98 F42 -4(3) . .
C94 C93 C92 S14 178(2) . .
C94 C93 C92 C97 0.0 . .
C94 C95 C98 F40 -58(2) . .
C94 C95 C98 F41 62(2) . .
C94 C95 C98 F42 -178.7(19) . .
C35 C32 C33 C34 -178(3) . .
C35 C32 C31 C30 -179(3) . .
C158 C157 C155 N2 172(3) . .
C105 C102 C101 C100 175(3) . .
C105 C102 C103 C104 -176(3) . .
C132 C131 N1 C135 99(4) . .
C132 C131 N1 C127 -32(4) . .
C132 C131 N1 C139 -176(4) . .
C155 N2 C147 C148 57(4) . .
C155 N2 C143 C144 74(4) . .
C155 N2 C151 C152 -172(4) . .
C155 C157 C158 C159 -75(6) . .
C143 N2 C147 C148 -66(4) . .
C143 N2 C155 C157 174(4) . .
C143 N2 C151 C152 -49(6) . .
C143 C144 C145 C146 -176(4) . .
C128 C127 N1 C135 -53(4) . .
C128 C127 N1 C131 77(4) . .
C128 C127 N1 C139 -136(3) . .
C135 N1 C139 C140 -166(3) . .
C133 C132 C131 N1 145(3) . .
C136 C135 N1 C131 67(3) . .
C136 C135 N1 C127 -148(3) . .
C136 C135 N1 C139 -44(3) . .
C142 C141 C140 C139 -144(4) . .
C153 C152 C151 N2 163(4) . .
C138 C137 C136 C135 -175(4) . .
C151 N2 C147 C148 174(3) . .
C151 N2 C155 C157 -61(4) . .
C151 N2 C143 C144 -49(5) . .
C151 C152 C153 C154 163(5) . .
C131 C132 C133 C134 133(5) . .
C131 N1 C139 C140 91(3) . .
C127 C128 C129 C130 -38(7) . .
C127 N1 C139 C140 -63(3) . .
C83 C82 C81 C80 0.0 . .
C83 C82 C81 C84 160(4) . .
C82 C83 C78 S12 -173(3) . .
C82 C83 C78 C79 0.0 . .
C82 C81 C80 C79 0.0 . .
C82 C81 C84 F36 11(7) . .
C82 C81 C84 F34 -140(5) . .
C82 C81 C84 F35 119(4) . .
C81 C80 C79 C78 0.0 . .
C80 C81 C84 F36 170(5) . .
C80 C81 C84 F34 19(7) . .
C80 C81 C84 F35 -82(4) . .
C80 C79 C78 S12 173(3) . .
C80 C79 C78 C83 0.0 . .
C78 C83 C82 C81 0.0 . .
C63 C60 C61 C62 -171(4) . .
C91 C88 C89 C90 -177(3) . .
C129 C128 C127 N1 -172(3) . .
N1 C135 C136 C137 -178(4) . .
C98 C95 C94 C93 175(2) . .
C84 C81 C80 C79 -158(4) . .
C56 C53 C54 C55 -176(4) . .
loop_
_platon_squeeze_void_nr
_platon_squeeze_void_average_x
_platon_squeeze_void_average_y
_platon_squeeze_void_average_z
_platon_squeeze_void_volume
_platon_squeeze_void_count_electrons
_platon_squeeze_void_content
1 0.000 0.500 0.000 954 375 ' '
2 0.500 0.500 0.500 954 376 ' '
3 0.750 0.413 0.250 118 57 ' '
4 0.722 0.407 0.021 8 2 ' '
5 0.778 0.407 0.479 8 2 ' '
6 0.250 0.587 0.750 118 56 ' '
7 0.222 0.592 0.521 8 2 ' '
8 0.278 0.592 0.979 8 2 ' '
